The history of textiles and ﬁbres spans thousands of years, beginning with the
style change from animal skins to the ﬁrst fabric used to clothe humanity. But
during the relatively short period of the past 50 years, the ﬁbre and textile
industries have undergone the most revolutionary changes and seen the most
remarkable innovations in their history. Chapter One discusses the most
important innovations together with the advent of the information industry.
In fact, it is the merger of these industries that has led to this book.
We are not talking merely of fabrics and textiles imparting information;
indeed, that has been occurring for many, many generations and numerous
examples exist from fabrics and tapestries that have told intricate tales of
warfare and family life and history, to those imparting information about the
wealth and social status of the owners of the fabrics. We are talking about
much more. Nor are we referring to fabrics that may have multifunctional
purposes, such as fashion and environmental protection, or rainwear, or those
fabrics providing resistance to a plethora of threats, such as ballistic, chemical
and ﬂame protection. These systems are all passive systems. No, we are
talking here about materials or structures that sense and react to environmental
stimuli, such as those from mechanical, thermal, chemical, magnetic or others.
We are talking ‘smart’ and ‘active’ systems. We are talking about the true
merger of the textile and information industries.
‘Smart textiles’ are made possible due to advances in many technologies
coupled with the advances in textile materials and structures. A partial list
includes biotechnology, information technology, microelectronics, wearable
computers, nanotechnology and microelectromechanical machines.
Many of the innovations in textile applications in the past 50 years have
started with military applications — from ﬁbreglass structures for radomes, to
fragment and bullet resistant body armour, to chemical agent protective
clothing, to ﬁbre-reinforced composites — indeed, many of our current defence
systems and advanced aircraft would not be possible without these materials.
So perhaps it is not surprising that the initial applications for smart textiles
have also come either directly from military R&D or from spin-oﬀs. Some of
the capabilities for smart textile systems for military applications are: sensing
and responding, for example to a biological or chemical sensor; power and
data transmission from wearable computers and polymeric batteries; trans-
mitting and receiving RF signals; automatic voice warning systems as to
‘dangers ahead’; ‘on-call’ latent reactants such as biocides or catalytic decon-
tamination in-situ for chemical and biological agents; and self-repairing materials.
In many cases the purpose of these systems is to provide both military and
civilian personnel engaged in high-risk applications with the most eﬀective
survivability technologies. They will thus be able to have superiority in
ﬁghtability, mobility, cognitive performance, and protection through materials
for combat clothing and equipment, which perform with intelligent reaction
to threats and situational needs. Thus, we will be providing high-risk personnel
with as many executable functions as possible, which require the fewest
possible actions on his/her part to initiate a response to a situational need.
This can be accomplished by converting traditional passive clothing and
equipment materials and systems into active systems that increase situational
awareness, communications, information technology, and generally improve
Some examples of these systems are body conformal antennas for integrated
radio equipment into clothing; power and data transmission — a personal area
network; ﬂexible photovoltaics integrated into textile fabrics; physiological
status monitoring to monitor hydration and nutritional status as well as the
more conventional heart monitoring; smart footwear to let you know where
you are and to convert and conserve energy; and, of course, phase change
materials for heating and cooling of the individual. Another application is the
weaving of sensors into parachutes to avoid obstacles and steer the parachutist
or the cargo load to precise locations.
There are, naturally, many more applications for ‘smart’ textiles than those
applied to military personnel, or civilian police, ﬁremen, and emergency
responders. Mountain climbers, sports personnel, businessmen with built-in
wearable microcomputers, and medical personnel will all beneﬁt from this
revolution in textiles.
You will learn of many more applications for ‘smart’ textiles in this book.
You will ﬁnd that the applications are limited only by your imagination and
the practical applications perhaps limited only by their cost. But we know
those costs will come down. So let your imagination soar. The current
worldwide textile industry is over 50 million metric tons per year, and if we are
able to capture only a measly 1% of that market, it is still worth more than
Dr Robert W. Lewis
Pushpa Bajaj, Toshihiro Hirai,
Department of Textile Technology, Department of Materials Chemistry,
Indian Institute of Technology, Faculty of Textile Science and
Hauz Khas, Technology,
New Delhi, Shinshu University,
India Tokida 3-15-1,
email@example.com Ueda-shi 386-8567,
Bischoﬀ Textile AG,
Switzerland Hartwig Hoecker,
bernhard.bischoﬀ@bischoﬀ-textil.com German Wool Research Institute at
Aachen University of Technology,
Philip J Brown, DWI,
School of Materials, Science & Veltmanplatz 8,
Engineering, D-52062 Aachen,
Clemson University, Germany
161 Sirrine Hall, firstname.lastname@example.org
Georgia Institute of Technology,
Elisabeth Heine, School of Textile and Fiber
Veltmanplatz 8, Atlanta,
D-52062 Aachen, GA 30332-0295,
So Yeon Kim, Seeram Ramakrishna,
School of Chemical Engineering, Faculty of Engineering,
College of Engineering, Department of Mechanical
Hanyang University, Engineering,
Haengdang-dong, Songdong-gu, National University of Singapore,
Seoul 133-791, 10 Kent Ridge Crescent,
Korea Singapore 119260
Young Moo Lee, Roland Seidl,
School of Chemical Engineering, Jakob Mueller Institute of Narrow
College of Engineering, Fabrics,
Hanyang University, Frick,
Haengdang-dong, Songdong-gu, Switzerland
Seoul 133-791, email@example.com
firstname.lastname@example.org Barbel Selm,
Swiss Federal Institute of Materials
Jin Kie Shim,
Heikki Mattila, School of Chemical Engineering,
Fibre Materials Science, College of Engineering,
Tampere University of Technology, Hanyang University,
PO Box 589, Haengdang-dong, Songdong-gu,
33101 Tampere, Seoul 133-791,
Sungmee Park, Hirofusa Shirai,
Georgia Institute of Technology, Faculty of Textile Science and
School of Textile and Fiber Technology,
Engineering, Shinshu University,
Atlanta, Tokida 3-15-1,
GA 30332-0295, Ueda-shi 386-8567,
Xiaoming Tao, Dongxiao Yang,
Institute of Textiles and Clothing, Department of Information and
The Hong Kong Polytechnic Electronic Engineering,
University, Zhejiang University,
Yuk Choi Road, Hangzhou 310027
Hung Hom, China
Hong Kong email@example.com
Devron P. Thibodeaux, Institute of Textiles and Clothing,
USDA, REE, ARS, MSA, The Hong Kong Polytechnic
1100 Robert E. Lee Boulevard, Yuk Choi Road,
New Orleans, Hung Hom,
LS 70124, Hong Kong
Institute of Functional Fibres,
Institute of Textiles and Clothing,
Tianjin Institute of Textile Science
The Hong Kong Polytechnic
Yuk Choi Road,
Tyrone L. Vigo, Faculty of Textile Science and
USDA, REE, ARS, MSA, Technology,
SRRC-CTCR, Shinshu University,
1100 Robert E. Lee Boulevard, Tokida 3-15-1,
New Orleans, Ueda-shi 386-8567,
LS 70124, Japan
Faculty of Textile Science and
The Editor wishes to thank the Hong Kong Polytechnic University for partial
support under the Area of Strategic Development Fund and Dr Dongxiao
Yang for assistance in compiling this book. The Editor also thanks all
contributing authors for their eﬀorts in making this book a reality.
List of contributors xiii
1 Smart technology for textiles and clothing
– introduction and overview 1
1.1 Introduction 1
1.2 Development of smart technology for textiles and clothing 3
1.3 Outline of the book 5
2 Electrically active polymer materials – application of
non-ionic polymer gel and elastomers for artiﬁcial
2.1 Introduction 7
2.2 Polymer materials as actuators or artiﬁcial muscle 9
2.3 Peculiarity of polymer gel actuator 10
2.4 Triggers for actuating polymer gels 10
2.5 Electro-active polymer gels as artiﬁcial muscles 15
2.6 From electro-active polymer gel to electro-active
elastomer with large deformation 28
2.7 Conclusions 30
3 Heat-storage and thermo-regulated textiles and
3.1 Development introduction 34
3.2 Basics of heat-storage materials 35
3.3 Manufacture of heat-storage and thermo-regulated textiles
and clothing 41
3.4 Properties of heat-storage and thermo-regulated textiles
and clothing 47
3.5 Application 52
3.6 Development trends 54
4 Thermally sensitive materials 58
4.1 Introduction 58
4.2 Thermal storage and thermal insulating ﬁbres 60
4.3 Thermal insulation through polymeric coatings 68
4.4 Designing of fabric assemblies 75
5 Cross-linked polyol ﬁbrous substrates as
multifunctional and multi-use intelligent materials 83
5.1 Introduction 83
5.2 Fibrous intelligent materials 83
5.3 Experimental 85
5.4 Results and discussion 86
5.5 Conclusions 91
6 Stimuli-responsive interpenetrating polymer network
hydrogels composed of poly(vinyl alcohol) and
poly(acrylic acid) 93
6.1 Introduction 93
6.2 Experimental 95
6.3 Results and discussion 97
6.4 Conclusions 106
7 Permeation control through stimuli-responsive
polymer membrane prepared by plasma and radiation
grafting techniques 109
7.1 Introduction 109
7.2 Experimental 110
7.3 Results and discussion 112
7.4 Conclusions 121
8 Mechanical properties of ﬁbre Bragg gratings 124
8.1 Introduction 124
8.2 Fabrication techniques 125
8.3 Mechanisms of FBG sensor fabrication 127
8.4 Mechanical properties 130
8.5 Inﬂuence of the UV irradiation on mechanical properties 133
8.6 Polymeric ﬁbre 141
8.7 Conclusions 145
9 Optical responses of FBG sensors under deformations 150
9.1 Introduction 150
9.2 Optical methodology for FBG sensors 151
9.3 Optical responses under tension 156
9.4 Optical responses under torsion 158
9.5 Optical responses under lateral compression 161
9.6 Optical responses under bending 165
9.7 Conclusions 166
10 Smart textile composites integrated with ﬁbre optic
10.1 Introduction 174
10.2 Optical ﬁbres and ﬁbre optic sensors 175
10.3 Principal analysis of embedded ﬁbre Bragg grating sensors 177
10.4 Simultaneous measurements of strain and temperature 181
10.5 Measurement eﬀectiveness 187
10.6 Reliability of FBGs 191
10.7 Error of strain measurement due to deviation of position and
10.8 Distributed measurement systems 195
10.9 Conclusions 195
11 Hollow ﬁbre membranes for gas separation 200
11.1 Historical overview of membranes for gas separation 200
11.2 Development of membranes for industrial gas separation 202
11.3 Theories of permeation processes 211
11.4 Phase inversion and hollow ﬁbre membrane formation 211
11.5 Future hollow ﬁbre membranes and industrial gas separation 214
12 Embroidery and smart textiles 218
12.1 Introduction 218
12.2 Basics of embroidery technology 218
12.3 Embroidery for technical applications — tailored ﬁbre
12.4 Embroidery technology used for medical textiles 221
12.5 Embroidered stamp — gag or innovation? 224
12.6 Summary 225
13 Adaptive and responsive textile structures (ARTS) 226
13.1 Introduction 226
13.2 Textiles in computing: the symbiotic relationship 226
13.3 The Georgia Tech Wearable Motherboard2+ 228
13.4 GTWM: contributions and potential applications 236
13.5 Emergence of a new paradigm: harnessing the opportunity 240
13.6 Conclusion 244
14 Wearable technology for snow clothing 246
14.1 Introduction 246
14.2 Key issues and performance requirements 247
14.3 The prototype 248
14.4 Conclusions 252
15 Bioprocessing for smart textiles and clothing 254
15.1 Introduction 254
15.2 Treatment of wool with enzymes 256
15.3 Treatment of cotton with enzymes 263
15.4 Enzymatic modiﬁcation of synthetic ﬁbres 270
15.5 Spider silk 270
15.6 ‘Intelligent’ ﬁbres 271
15.7 Conclusions 271
16 Tailor-made intelligent polymers for biomedical
16.1 Introduction 278
16.2 Fundamental aspects of shape memory materials 280
16.3 Concept of biodegradable shape memory polymers 281
16.4 Degradable thermoplastic elastomers having shape memory
16.5 Degradable polymer networks having shape memory
16.6 Conclusion and outlook 288
17 Textile scaffolds in tissue engineering 291
17.1 Introduction 291
17.2 Ideal scaﬀold system 295
17.3 Scaﬀold materials 296
17.4 Textile scaﬀolds 298
17.5 Conclusions 306
Smart technology for textiles and clothing –
introduction and overview
Since the nineteenth century, revolutionary changes have been occurring at an
unprecedented rate in many ﬁelds of science and technology, which have
profound impacts on every human being. Inventions of electronic chips,
computers, the Internet, the discovery and complete mapping of the human
genome, and many more, have transformed the entire world. The last century
also brought tremendous advances in the textile and clothing industry, which
has a history of many thousands of years. Solid foundations of scientiﬁc
understanding have been laid to guide the improved usage and processing
technology of natural ﬁbres and the manufacturing of synthetic ﬁbres. We
have learnt a lot from nature. Viscose rayon, nylon, polyester and other
synthetic ﬁbres were invented initially for the sake of mimicking their natural
counterparts. The technology has progressed so that synthetic ﬁbres and their
products surpass them in many aspects. Biological routes for synthesizing
polymers or textile processing represent an environmentally friendly, sustainable
way of utilizing natural resources. Design and processing with the aid of
computers, automation with remote centralized or distributed control, and
Internet-based integrated supply-chain management systems bring customers
closer to the very beginning of the chain than ever before.
Looking ahead, the future promises even more. What new capacities should
we expect as results of future developments? They should at least include
terascale, nanoscale, complexity, cognition and holism. The new capability of
terascale takes us three orders of magnitude beyond the present general-purpose
and generally accessible computing capabilities. In a very short time, we will be
connecting millions of systems and billions of information appliances to the
Internet. Technologies allowing over one trillion operations per second are on
the agenda for research. The technology in nanoscales will take us three orders
of magnitude below the size of most of today’s human-made devices. It will
allow us to arrange atoms and molecules inexpensively in most of the ways
2 Smart ﬁbres, fabrics and clothing
processing Electric and
1.1 A single cell living creature is an example of smart structures.
permitted by physical laws. It will let us make supercomputers that ﬁt on the
head of a ﬁbre, and ﬂeets of medical nanorobots smaller than a human cell to
eliminate cancers, infections, clogged arteries and even old age. Molecular
manufacturing will make exactly what it is supposed to make, and no
pollutants will be produced.
We are living in this exciting era and feeling the great impacts of technology
on the traditional textiles and clothing industry, which has such a long history.
Traditionally, many ﬁelds of science and engineering have been separate and
distinct. Recently, there has been considerable movement and convergence
between these ﬁelds of endeavour and the results have been astonishing. Smart
technology for materials and structures is one of these results.
What are smart materials and structures? Nature provides many examples
of smart structures. The simple single-celled living creature may highlight the
fundamentals. As shown in Fig. 1.1, various environmental conditions or
stimuli act on the outer layer. These conditions or stimuli may be in the form of
force, temperature, radiation, chemical reactions, electric and magnetic ﬁelds.
Sensors in the outer layer detect these eﬀects, and the resulting information is
conveyed for signal processing and interpretation, at which point the cell
reacts to these environmental conditions or stimuli in a number of ways, such
as movement, changing chemical composition and reproductive actions.
Nature has had billions of years and a vast laboratory to develop life, whereas
humankind has just begun to create smart materials and structures.
Smart materials and structures can be deﬁned as the materials and
structures that sense and react to environmental conditions or stimuli, such as
Smart technology for textiles and clothing – introduction and overview 3
those from mechanical, thermal, chemical, electrical, magnetic or other
sources. According to the manner of reaction, they can be divided into passive
smart, active smart and very smart materials. Passive smart materials can only
sense the environmental conditions or stimuli; active smart materials will
sense and react to the conditions or stimuli; very smart materials can sense,
react and adapt themselves accordingly. An even higher level of intelligence
can be achieved from those intelligent materials and structures capable of
responding or activated to perform a function in a manual or pre-programmed
Three components may be present in such materials: sensors, actuators and
controlling units. The sensors provide a nerve system to detect signals, thus in
a passive smart material, the existence of sensors is essential. The actuators act
upon the detected signal either directly or from a central control unit; together
with the sensors, they are the essential element for active smart materials. At
even higher levels, like very smart or intelligent materials, another kind of unit
is essential, which works like the brain, with cognition, reasoning and
activating capacities. Such textile materials and structures are becoming
possible as the result of a successful marriage of traditional textiles/clothing
technology with material science, structural mechanics, sensor and actuator
technology, advanced processing technology, communication, artiﬁcial in-
telligence, biology, etc.
1.2 Development of smart technology for textiles and
We have always been inspired to mimic nature in order to create our clothing
materials with higher levels of functions and smartness. The development of
microﬁbres is a very good example, starting from studying and mimicking silk
ﬁrst, then creating ﬁner and, in many ways, better ﬁbres. However, up to now,
most textiles and clothing have been lifeless. It would be wonderful to have
clothing like our skin, which is a layer of smart material. The skin has sensors
which can detect pressure, pain, temperature, etc. Together with our brain, it
can function intelligently with environmental stimuli. It generates large
quantities of sweat to cool our body when it is hot, and to stimulate blood
circulation when it gets cold. It changes its colour when exposed to a higher
level of sunlight, to protect our bodies. It is permeable, allowing moisture to
penetrate yet stopping unwanted species from getting in. The skin can shed,
repair and regenerate itself. To study then develop a smart material like our
skin is itself a very challenging task.
In the last decade, research and development in smart/intelligent materials
and structures have led to the birth of a wide range of novel smart products in
4 Smart ﬁbres, fabrics and clothing
aerospace, transportation, telecommunications, homes, buildings and infra-
structures. Although the technology as a whole is relatively new, some areas
have reached the stage where industrial application is both feasible and viable
for textiles and clothing.
Many exciting applications have been demonstrated worldwide. Extended
from the space programme, heat generating/storing ﬁbres/fabrics have now
been used in skiwear, shoes, sports helmets and insulation devices. Textile
fabrics and composites integrated with optical ﬁbre sensors have been used to
monitor the health of major bridges and buildings. The ﬁrst generation of
wearable motherboards has been developed, which has sensors integrated
inside garments and is capable of detecting injury and health information of
the wearer and transmitting such information remotely to a hospital. Shape
memory polymers have been applied to textiles in ﬁbre, ﬁlm and foam forms,
resulting in a range of high performance fabrics and garments, especially
sea-going garments. Fibre sensors, which are capable of measuring temperature,
strain/stress, gas, biological species and smell, are typical smart ﬁbres that can
be directly applied to textiles. Conductive polymer-based actuators have
achieved very high levels of energy density. Clothing with its own senses and
brain, like shoes and snow coats which are integrated with Global Positioning
System (GPS) and mobile phone technology, can tell the position of the wearer
and give him/her directions. Biological tissues and organs, like ears and noses,
can be grown from textile scaﬀolds made from biodegradable ﬁbres. Integrated
with nanomaterials, textiles can be imparted with very high energy absorption
capacity and other functions like stain prooﬁng, abrasion resistance, light
The challenges lie before us, as the research and development of smart
technology and its adoption by industries depend upon successful multidiscip-
linary teamwork, where the boundary of traditional disciplines becomes
blurred and cross-fertilization occurs at a rate much higher than that seen
previously. Some of the research areas can be grouped as follows:
∑ photo-sensitive materials
∑ conductive polymers
∑ thermal sensitive materials
∑ shape memory materials
∑ intelligent coating/membrane
∑ chemical responsive polymers
∑ mechanical responsive materials
∑ micro and nanomaterials.
Smart technology for textiles and clothing – introduction and overview 5
For signal transmission, processing and controls:
∑ neural network and control systems
∑ cognition theory and systems.
For integrated processes and products:
∑ wearable electronics and photonics
∑ adaptive and responsive structures
∑ tissue engineering
∑ chemical/drug releasing.
Research and development activities have been carried out worldwide, both
in academic/research institutions and companies. Research teams in North
American, European and Asian countries have been actively involved, with
noticeable outcomes either in the form of commercial products or research
1.3 Outline of the book
This edited book, being the ﬁrst on this topic, is intended to provide an
overview and review of the latest developments of smart technology for textiles
and clothing. Its targeted readers include academics, researchers, designers,
engineers in the area of textile and clothing product development, and senior
undergraduate and postgraduate students in colleges and universities. Also, it
may provide managers of textile and clothing companies with the latest
insights into technological developments in the ﬁeld.
The book has been contributed by a panel of international experts in the
ﬁeld, and covers many aspects of the cutting-edge research and development.
It comprises 17 chapters, which can be divided into four parts. The ﬁrst part
(Chapter 1) provides the background information on smart technology for
textiles and clothing and a brief overview of the developments and the book
structure. The second part involves material or ﬁbre-related topics from
Chapters 2 to 9. Chapter 2 is concerned with electrically active polymer
materials and the applications of non-ionic polymer gel and elastomers for
artiﬁcial muscles. Chapters 3 and 4 deal with thermal sensitive ﬁbres and
fabrics. Chapter 5 presents cross-linked polyol ﬁbrous substrates as multifunc-
tional and multi-use intelligent materials. Chapter 6 discusses stimuli-responsive
interpenetrating polymer network hydrogel. Chapter 7 is concerned with
permeation control through stimuli-responsive polymer membranes prepared
by plasma and radiation grafting techniques. Chapters 8 and 9 discuss the
6 Smart ﬁbres, fabrics and clothing
Table 1.1 Outline of the book
Chapter processing processes Bio-processes
no. Sensors/actuators and control and products and products
principles, manufacturing and properties of optical ﬁbre sensors, with
emphasis on ﬁbre Bragg grating sensors.
The third part contains ﬁve chapters, with a focus on integrating processes
and integrated structures. Chapter 10 provides an overview of the developments
and key issues in ﬁbre-optic smart textile composites. Chapter 11 presents
hollow ﬁbre membranes for gas separation. Chapter 12 describes embroidery
as one way of integrating ﬁbre-formed components into textile structures.
Chapters 13 and 14 are on wearable electronic and photonic technologies.
Chapter 13 provides insights on adaptive and responsive textile structures
(ARTS). Chapter 14 describes the development of an intelligent snowmobile suit.
The fourth part, embracing the last three chapters, is focused on
bioapplications. Chapter 15 outlines various bioprocesses for smart textiles
and clothing, and Chapter 16 concentrates on tailor-made intelligent polymers
for biomedical applications. Chapter 17 describes the applications of scaﬀolds
in tissue engineering, where various textile structures are used for cells to grow.
We have only seen a small portion of the emerging technology through the
window of this book. The possibilities oﬀered by this smart technology are
tremendous and widespread. Even as the book was being prepared, many new
advances were being achieved around the world. It is the hope of the editor and
contributors of this book that it will help researchers and designers of future
smart ﬁbres, textiles and clothing to make their dreams a reality.
Electrically active polymer materials –
application of non-ionic polymer gel and
elastomers for artiﬁcial muscles
TOSHIHIRO HIRAI, JIANMING ZHENG,
MASASHI WATANABE AND HIROFUSA SHIRAI
Many attempts have been made to functionalize polymer materials as
so-called ‘smart’ or ‘intelligent’ materials (see Fig. 2.1).— Artiﬁcial muscle or
intelligent actuators is one of the targets of such attempts. Historically,
actuator materials have been investigated mainly in inorganic compounds.
Particularly, triggers used for actuation are usually investigated in an electric
ﬁeld application because of the ease of control. Polymer materials investigated
from this point of view are very limited and have been known to generate much
smaller strain than inorganic materials.—
On the other hand, polymer materials such as polymer gels have been
known to generate huge strain by various triggers such as solvent exchange,
pH jump, temperature jump, etc., although the response and durability are
rather poor and they have not been used in practical actuators.
In the ﬁeld of mechanical engineering, the development of micromachining
procedure is facing the requirements of the technologies of microfabrication
and micro-device assembly, and there are high expectations of the emerging
smart materials that can greatly simplify the microfabrication process.—
Under these circumstances, the polymer gel actuator is mentioned as one of
the most likely candidates as a soft biological muscle-like material with large
deformation in spite of its poor durability. Much research has been done on
solid hard materials as actuators like poly(vinylidene ﬂuoride) (PVDF), which
is a well-known piezoelectrical polymer, and in which crystal structures play
critical role for the actuation and the induced strain is very small compared to
the gel artiﬁcial muscles that will be described in this chapter. Although PVDF
needs electrically oriented crystal structure in it, the materials that will be
discussed in this chapter do not require such a limitation.
Conventional electrically induced actuation has been carried out mostly on
ionic polymer gels. The reason is simply because ionic species are highly
8 Smart ﬁbres, fabrics and clothing
Trigger or stimuli Trigger or stimuli
Response or Response or
action (adaptation) action (adaptation)
2.1 Concepts of autonomic systems and materials. Three processes
(sensing, processing and actuation) are incorporated in materials (in one
system): (a) in autonomic materials, while they are separated and must be
uniﬁed by a controlling system; (b) in conventional autonomic systems.
responsive to the electric ﬁeld. Ionic gels have proved to be excellent
electroactive actuator materials.
However, we tried electrical actuation of non-ionic polymer gel or
elastomers. Why must non-ionic polymer gel be used for electrical actuation?
Because non-ionic polymer gel is superior to ionic polymer gel in several ways,
if it can be actuated by an electric ﬁeld. In ionic gel materials, electrolysis is
usually inevitable on the electrodes, and this is accompanied by a large electric
current and heat generation. In other words, elecrochemical consumption is
inevitable, although this fact has not been mentioned in most papers. In
non-ionic polymer gels, no such process is encountered, and this leads to the
good durability of the materials. In addition to these advantages, the
responding speed and magnitude of the deformation were found to be much
Electrically active polymer materials 9
faster (10 ms order) and larger (over 100%) than those induced in polyelectrolyte
gels. The motion reminds us of real biological muscle.
The concept of the mechanism is simple and can be applied to conventional
polymer materials, including materials commonly used in the ﬁbre and textile
industries. The concept is also applicable to non-ionic elastomers that do not
contain any solvent. The method we present will provide a promising way for
developing future artiﬁcial muscle. Several concepts developed by other
researchers and successfully used for actuating gels are also introduced in
comparison with our method.
2.2 Polymer materials as actuators or artiﬁcial muscle
Polymer gel is an electroactive polymer material. There are various types of
electroactive polymeric materials. As mentioned in the above section,
polyelectrolyte is one of them and is most commonly investigated as an
electroactive gel. We will come back to discuss this material in more detail in
the next section.
Ferroelectric polymer materials like PVDF or its derivatives are mentioned,
since they behave as ferroelectric materials (see Fig. 2.2). They have
crystallinity and the crystals show polymorphism by controlling the preparation
method. Much detailed work has been carried out on piezoelectric and/or
pyroelectric properties, together with their characteristics as electroactive
actuators. These materials have long been mentioned as typical electroactive
polymers. Through these materials, it is considered that the strain induced in
the polymer materials is not large. The electrostrictive coeﬃcient is known to
be small for polymers. These are non-ionic polymers and the induced strain
originates from the reorientation or the deformation of polarized crystallites in
the solid materials.
There is another type of electrically active polymer that is known as the
electroconductive polymer, in which polymer chains contain long conjugated
double bonds, and this chemical structure adds electroconductive properties
to the polymers. In these cases, the electrically induced deformation is
considered to have originated from the electrochemical reactions such as the
oxidation and reduction of the polymer chain. For the deformation, some
additives such as dopants have been known to be necessary for eﬀective
actuation. Therefore, the electrical actuation of these materials has been
2.2 Chemical structure of poly(vinylidene ﬂuoride) (PDVF).
10 Smart ﬁbres, fabrics and clothing
2.3 Chemical structures of (a) polypyrrole and (b) polyaniline.
investigated in the presence of water, similar to the case of polyelectrolyte gels.
Polypyrrole and polyaniline are typical examples (see Fig. 2.3).—
2.3 Peculiarity of polymer gel actuator
Polymer gels diﬀer in various ways from hard solid polymer materials. The
polymer chains in the gel are usually considered to be chemically or physically
cross-linked and to form a three-dimensional network structure. For instance,
polymer gel is usually a matter swollen with its good solvent, and the
characteristics are diversiﬁed from a nearly solid polymer almost to a solution
with very low polymer content but still maintaining its shape by itself. This
extreme diversity in physical properties widens the function of the gel (see Fig. 2.4).
From the standpoint of the actuator, the gel behaves like a conventional
solid actuator or biological muscle, or like a shapeless amoeba. The gels also
have various actuating modes, symmetric volume change with swelling and
de-swelling, asymmetric swelling behaviour, symmetric deformation and
asymmetric deformation (see Fig. 2.5). The strain induced in the gel can also be
extremely large, depending on the cross-link structure in the gel.
2.4 Triggers for actuating polymer gels
As can be expected from the diversiﬁed physical characteristics of the gel and
the wide variety of the actuating modes, there are various triggers for the
actuating polymer gels.
The triggers can be classiﬁed into two categories, chemical triggers and
physical triggers (see Fig. 2.6). As chemical triggers, solvent exchange includes
jumps in solvent polarity (e.g. from good solvent into poor solvent), in pH
(e.g. in weak polyelectrolyte gel from a dissociated condition into an associated
condition) and in ionic strength (utilizing salting-out or coagulation). These
Electrically active polymer materials 11
2.4 Extreme diversity in physical property widens the function of the gel.
2.5 Various actuating modes of polymer gels: (a) swelling and de-swelling,
(b) asymmetric swelling or de-swelling.
(a) Chemical triggers
oxidation and reduction
ionic strength change
(b) Physical triggers
magnetic field application
electric field application
2.6 Triggers for polymer and/or gel actuation can be classiﬁed into two
categories: chemical and physical.
12 Smart ﬁbres, fabrics and clothing
2.7 Chemical triggers including solvent exchange. These types
accompany swelling and de-swelling of the solvent, and the deformation
is usually symmetric as long as the gel has a homogeneous structure.
2.8 Temperature jump as a physical trigger: (a) poly(vinyl methyl ether)
and (b) poly(N-isopropyl acrylonide).
two types accompany swelling and de-swelling of the solvent, and the
deformation is usually symmetric as far as the gel has a homogeneous
structure (see Fig. 2.7). Temperature jump, which is a physical trigger, can also
induce symmetric deformation in particular polymer gels where the solubility
has a critical transition temperature. Typical examples are the gels of
poly(vinyl methyl ether) and poly(N-isopropyl acrylamide). These gels
have high water absorption at low temperatures and de-swell at the
characteristic critical temperature around 30—40 °C (see Fig. 2.8). The
transition temperature can be controlled by changing chemical structure.
In the case of urease immobilized gel, the addition of urea, a substrate of
Electrically active polymer materials 13
2.9 Chemical trigger can induce swelling and de-swelling of gel, e.g.
substrate of urease, urea, is changed into ammonia and the ammonia
induces swelling and de-swelling by varying pH.
2.10 Light-induced deformation of polymer ﬁlm. Example shown is the
case of PVC ﬁlm containing spyrobenzopyrane.
urease, induces swelling and deswelling by utilizing the pH change induced by
the enzyme reaction (see Fig. 2.9).
A physical trigger such as light irradiation is useful for actuating a gel in
which the light-induced reversible isomerization occurs and the isomerization
accompanies physical strain. In this case, the change is usually asymmetric
and the gel bends toward or against the direction of the irradiation, depending
on the photoinduced reaction (see Fig. 2.10).
In the case of electric ﬁeld application, the gels usually bend, because the
ﬁeld application induces asymmetric charge distribution and hence the
asymmetric strain in the gel. Asymmetric charge distribution can easily be
induced in polyelectrolyte gels, and this is why polyelectrolyte gel has mainly
been investigated as on electroactive polymer material (see Fig. 2.11).
Magnetic ﬁeld application can also induce a strain in a gel when a structure
or species sensitive to the magnetic ﬁeld is contained in it. We ﬁrst proposed
the idea of applying a super paramagnetic ﬂuid to a gel.— The gel was found
14 Smart ﬁbres, fabrics and clothing
2.11 Electrically induced deformation. In the case of electric ﬁeld
application, the gels usually bend, since ﬁeld application induces
asymmetric charge distribution and hence the asymmetric strain in the gel.
2.12 Magnetic ﬁeld active gel utilizing super paramagnetic property of a
ferro-ﬂuid-immobilized gel. , ferroﬂuid 75 wt %; *, ferroﬂuid 50 wt %;
ferroﬂuid 25 wt %.
Electrically active polymer materials 15
2.13 Magnetic ﬁeld induced large deformation. By turning the magnetic
ﬁeld (H) on and off, the gel deforms instantly.
to be sensitive to the magnetic ﬁeld gradient and to induce strain very
sensitively, and the structure change in the gel was investigated (see Fig. 2.12).
Zryhni and his coworkers investigated the same materials and found
discontinuous deformation of the gel by controlling the magnetic ﬁeld (see Fig.
2.5 Electro-active polymer gels as artiﬁcial muscles
Amongst the polymeric actuator materials mentioned above, polymer gel has
an important property as a huge strain generating material. As mentioned in
the previous section, the electric ﬁeld is one of the most attractive triggers for
practical actuation. Electroactivity has been mentioned in connection with
polyelectrolyte gels, since they contain ionic species. However, ionic species
are not only sensitive to an electric ﬁeld, but also usually electrochemically
active, and accompany electrolysis on the electrodes. Electrochemical reactions
often result in increased current and heat generation. These processes only
dissipate energy, and do not contribute to strain generation. Thus, elec-
trochemical reactions are an undesirable process in most cases. In spite of their
many diﬃculties for practical actuators, polyelectrolyte gels and related
materials still remain at the forefront of electroactive polymer materials.
To overcome diﬃculties in polyelectrolytes, such as electrochemical
consumption on the electrodes, we investigated the electroactive properties of
the non-ionic polymer gel.
2.5.1 Electroactive polyelectrolyte gels
As pointed out in the previous section, polyelectrolyte gels have been
investigated as electroactive actuator materials. The concept originates from
the presence of electroactive ionic species in the gels. The ionic species can
16 Smart ﬁbres, fabrics and clothing
2.14 Bending deformation of a poly(acrylonide-co-sodium acrylate) gel in
aqueous solution. Bending direction is changed with sodium acrylate
content in the gel. Acrylic acid content was controlled by hydrolysing
poly(acrylonide) gel. The mechanism was explained with the results
shown in Fig. 2.15.
2.15 Electrically induced asymmetric deformation of a
poly(acrylonide-co-sodium acrylate) gel. Sodium acrylate content is
(a) low, and (b) high. In (a) the gel shrinks on anode side, but swells in (b).
migrate and form localized distribution and/or electrochemical reactions in
the gel, which cause its deformation.
188.8.131.52 Poly(acrylic acid) gel
Among polyelectrolyte gels, poly(acrylic acid) (PAA) gel was the ﬁrst polyelec-
trolyte investigated as an electroactive polymer gel. Shiga et al. found that
PAA gel can be deformed by DC electric ﬁeld application in the presence of
salt.— A PAA gel rod was immersed in the saline aqueous solution (see Fig.
2.14). The platinum electrodes were apart from the gel surface, and the DC
ﬁeld was applied from both sides of the gel. Shiga et al. found a slow bending
motion of the gel, the magnitude of bending depending on the salt and its
concentration. They also found an asymmetric deformation of the gel, when
the ﬁeld was applied apart from both ends of the gel rod (see Fig. 2.15). In this
case, the gel shrinks at one end and swells at the other end. The motion is
explained by asymmetric swelling behaviour under the ﬁeld. The deformation
is explained by the following equation derived by Flory:
: ; ; [2.1]
Electrically active polymer materials 17
2.16 Gel ﬁnger in aqueous solution. Polymer gel contains poly(acrylic)
acid and poly(vinyl alchohol). One electrode is occluded in the gel, and the
other electrode is exposed in the solution.
: 9 [ln(1 9 ) ; ; x ]RT/V [2.2]
: ( 9 /2)RT /V [2.3]
: ( c 9 c )RT [2.4]
where is the overall osmotic pressure which is the summation of the three
types of osmotic pressure, , and , which originate from the interaction
between the polymer chain and solvent, from the rubber elasticity of the gel,
and from the concentration diﬀerences of the ionic species inside and outside
the gel, respectively. The parameters , x, V , , V , c , c , R and T are the
C G H
polymer volume fraction, the interaction parameter between polymer and
solvent, the volume of dried polymer, the eﬀective chain number in the
network, the molar volume of the solvent, the concentration of species i in the
gel, the concentration of species j in outer solution, the gas constant and the
absolute temperature, respectively.
The process was considered to originate from an osmotic pressure gap
induced by the localization of ionic species of diﬀerent solvation power. In this
movement, electrolysis usually occurred on the electrodes. Shiga et al. optimized
the preparation method in order to overcome the diﬃculty. They put the
electrodes on the gel surface, and successfully demonstrated the gel ﬁnger in
aqueous solution (see Fig. 2.16).
18 Smart ﬁbres, fabrics and clothing
2.17 Association and dissociation of polyelectrolyte gel of
poly(2-acrylamido-2-methylpropanesulfonic acid) (PAMPS) with cationic
surfactant was found to undergo worm-like motility in aqueous solution.
184.108.40.206 Poly(2-acrylamido-2-methylpropanesulfonic acid) gel
Poly(2-acrylamido-2-methylpropanesulfonic acid) (PAMPS) gel was found to
undergo worm-like motility (see Fig. 2.17).— The principle of this deformation
is based on an electrokinetic molecular assembly reaction of surfactant molecules
on the hydrogel, caused by both electrostatic and hydrophobic interactions
and resulting in anisotropic contraction to give bending towards the anode.
When the ﬁeld is reversed, the surfactant admolecules on the surface of the gel
lift oﬀ and travel away electrically towards the anode. Instead, new surfactant
molecules approach from the opposite side of the gel and form the complex
preferentially on that side of the gel, thus stretching the gel. Surfactants such
as N-dodecylpyridinium chloride (Cl PyCl) were used, which adsorbed within
a second and is easily calculated to give a complex formation ratio less than
1 ; 10, explaining that the quick and large bending under an electric ﬁeld is
dominated only by the surface complexation and shrinkage of the gel.
Electrically active polymer materials 19
2.18 Ion-exchange polymer–metal composite ﬁlm of Naﬁon, of Dupont or
Flemion of Asahi Glass Co. Ltd. can bend remarkably by applying low
220.127.116.11 Perﬂuorosulfonate ionomer gel
A hydrogel of perﬂuorosulfonate ionomer (Naﬁon of Dupont) ﬁlm, thickness
of ca. 0.2 mm, was found to be an eﬀective electroactive material (see Fig.
2.18).— This material can be actuated by a DC ﬁeld application of low
voltage such as 3 volts. Success was attained by the development of the
chemical deposition of the electrode on the membrane surface. The principle
of the deforming mechanism is somewhat similar to the case of other
polyelectrolyte gels. That is, the membrane requires the presence of water and
salts, and an encounter of electrochemical consumption is principally inevitable.
However, the response time and durability are much higher than with the
other gel materials. Moreover, the actuating process is not seriously aﬀected
by electrochemical reactions, provided the operating conditions are adequately
controlled. Improvement of the eﬃciency can be considered to originate from
the chemical structure of the membrane, and the coexistence of the strong
hydrophobicity and strong hydrophilicity in a polymer chain.
2.5.2 Electroactive non-ionic polymer gels
Reviewing the above-mentioned materials, one of the serious defects of
polyelectrolyte gels is the electrochemical consumption on the electrode under
an electric ﬁeld application. The electrochemical consumption causes poor
durability of the polyelectrolyte gels and limits their application ﬁelds.
Therefore, the authors tried to utilize non-ionic polymer gels as actuating
materials with large deformation. The results show that the idea works in a far
20 Smart ﬁbres, fabrics and clothing
2.19 Dependence of strain in the direction of the ﬁeld on the electric ﬁeld.
more eﬃcient manner than expected, but the mechanism turned out to be not
the same as they expected initially. The feature will be described below in a
18.104.22.168 Strain in the direction of the ﬁeld
Poly(vinyl alcohol)—DMSO gel was prepared by combining physical cross-
linking and chemical cross-linking with glutaraldehyde (GA). After the chemical
cross-linking, the physical cross-links were eliminated by exchanging solvent
into pure DMSO. The chemically cross-linked gel thus obtained has an
electronically homogeneous structure. Therefore, the PVA—DMSO gel has no
intrinsic polarization in its structure, and electrostrictive strain generation is
expected by applying a DC electric ﬁeld. The results agree with this expectation,
and the strain is proportional to the square of the ﬁeld (see Fig. 2.19). The
strain observed reached over 7% in the direction of the ﬁeld. The response
time is very fast, the large strain is attained within 0.1 s, and the shape of the
gel is instantly restored by turning oﬀ the ﬁeld. The current observed is
around 1 mA at 250 V/mm, which is much smaller than those of polyelectrolyte
gels. The current can be depressed by further puriﬁcation of the polymer and
solvent. This performance is much faster than conventional polyelectrolyte
gels. We can demonstrate the electro-activated quick strain in the ﬂapping
motion by amplifying the strain by 300 times. It is suggested that the ﬂapping
motion be accelerated up to 10 Hz, though the demonstration was carried out
at 2 Hz (see Fig. 2.20).
Electrically active polymer materials 21
Rod (12.5 cm)
with a span
DC power of 10 cm
Gel (thickness = 4 mm)
2.20 Flapping motion induced by an electrostrictive deformation of a
non-ionic polymer gel swollen with a dielectric solvent.
2.21 Structure of dimethylsulfoxide and its orientation by an electric ﬁeld.
Polarized Raman spectroscopy can be employed for investigating the
molecular orientation under the ﬁeld.
22.214.171.124 Electrical orientation of solvent
The strain induced in the direction of the ﬁeld cannot be explained by the
electrostatic attractive force between the electrodes. The eﬀect of the electrostatic
ﬁeld was expected to be less than 25% of the observed strain under our
experimental conditions. We therefore have to ﬁnd another explanation for
the strain generation in the gel.
Initially, we expected the orientation of solvent molecule under an electric
ﬁeld to lead the strain generation in the gel, through the changes of interactions
between solvent and solute polymer, which forms the gel network.
In order to observe the eﬀect of the electric ﬁeld on the orientation of the
solvent, DMSO, Raman spectroscopy was employed. The molecule has a
strong dipole moment, and can be expected to orient along the ﬁeld direction
(see Fig. 2.21). It is oriented very eﬃciently even in relatively low electric
ﬁelds, but the orientation decreases over the maximum ﬁeld intensity (see Fig.
2.22). The deformation of the gel becomes greater in the region of the higher
ﬁeld than that of the maximum orientation, suggesting that the solvent
orientation is not directly related to the deformation of the gel.
22 Smart ﬁbres, fabrics and clothing
Anisotropy of scattering intensity
0 25 50 75 100
2.22 Electrically induced orientation of DMSO. DMSO orients very
efﬁciently even in relatively low electric ﬁeld, but the orientation decreases
over the maximum ﬁeld intensity.
126.96.36.199 Bending and crawling motion accompanying huge strain
In observing the contraction along the direction of an electric ﬁeld, brass
plates were used as electrodes. The strain in the perpendicular direction of the
ﬁeld was also observable. In these measurements, the bending deformation of
the gels was prevented or completely depressed.
When we carefully observed the gel deformation, solvent ﬂow and some
asymmetric deformation was suggested in the gel. But conventional electrodes
or a thin metal sheet of 10 m thickness did not lead to any eﬀective deformation.
We used very thin gold electrodes whose thickness was 0.1 m, and covered
both surfaces of the gel with the thin metal sheet. The metal sheet is soft
enough and does not disturb even a slight deformation of the gel.
By applying a DC electric ﬁeld to the gel, the gel bent swiftly and held the
deformation as far as the ﬁeld was on (see Fig. 2.23).— The bending was
completed within 60 ms, and the bending angle reached over 90 degrees. By
turning oﬀ the ﬁeld, the strain was released instantly, and the gel resumed its
original shape (see Fig. 2.24). The curvature turned out to be proportional to
the square of the ﬁeld (see Fig. 2.25).
Taking the gel size (length 1 cm, width 5 mm and thickness 2 mm) into
account, and assuming the gel volume does not change in the deformation, the
strain in the gel can be estimated to be over 140% in length. The electric
current observed in this motion was less than 30 A under the ﬁeld of 500 V/mm.
This response and the huge strain attained in the PVA—DMSO gel is the
Electrically active polymer materials 23
(thickness = 2 mm
width = 5 mm
length = 1 cm)
Thin gold electrodes
(thickness = 0.1 m)
2.23 Assembling an electroactive non-ionic gel. The metal sheet was soft
enough and does not disturb even a slight deformation of the gel.
2.24 Swift bending of a non-ionic polymer gel. By applying a DC electric
ﬁeld to the gel, the gel bent swiftly and sustained the deformation while
the ﬁeld was on.
largest value among the electroactive polymer gel materials reported so far.
The low current suggests that there is much less energy loss in this motion
compared with the conventional polyelectrolyte gels. The energy loss as heat
was much less than that of Naﬁon or Flemion membrane overall, therefore it
is far less when the size (thickness and surface area) of the gel is taken into
24 Smart ﬁbres, fabrics and clothing
R (mm 1)
50 100 200 300
2.25 Dependence of bending curvature on an electric ﬁeld.
2.26 Crawling motion of a non-ionic polymer gel.
The gel could also show a crawling-type deformation. This is a novel type
of motion. The crawling motion was observed when a naked gel was placed on
an electrode stripe array. The motion was completed in ca. 1 second (see Fig. 2.26).
188.8.131.52 Origin of the asymmetric pressure distribution in the gel
Such a remarkable swift bending or crawling of a non-ionic polymer gel
cannot be explained by osmotic pressure gradient, which is usually considered
to be the reason for electrically induced bending in polyelectrolyte gel. As
pointed out in the previous section, the solvent ﬂow was suggested in the gel.
We investigated the eﬀect of an electric ﬁeld on its ﬂowing property.
Electrically active polymer materials 25
2.27 Electric ﬁeld-induced ﬂow of a dielectric solvent. A pair of cone-like
electrodes were dipped in a circular tray ﬁlled with DMSO.
Flow rate (mm/s)
0 200 400
2.28 Dependence of a ﬂow rate on an electric ﬁeld. The ﬂow rate was
proportionally increased with the square of the ﬁeld.
A pair of comb-like electrodes were dipped in a circular tray ﬁlled with
DMSO (see Fig. 2.27). When a DC ﬁeld was applied, the solvent started
ﬂowing from anode to cathode. The ﬂowing rate was measured by using
polystyrene powder ﬂoating on the solvent as a probe. The ﬂow rate increased
proportionally with the square of the ﬁeld (Fig. 2.28). This result suggests that
the pressure gradient is generated between the electrodes.
In order to establish a quantitative estimation of the pressure gradient, a
theoretical treatment was carried out under some hypotheses shown below:
1 Only one value of ion mobility exhibits for a kind of ion.
2 The turbulence in the gel can be neglected for the calculations of the
3 The ionizing and accelerating electrodes do not interfere with pressure
26 Smart ﬁbres, fabrics and clothing
2.29 Solvent DMSO is drawn up between the electrodes.
4 Although only a very small resultant current exists, it is enough to determine
the ﬁeld distribution.
5 Diﬀerent types of ions do not interfere with each other in the pressure
6 Surface charges on solvent boundaries have a negligible eﬀect on ion
current and ﬁeld distribution.
The following equation was deduced for the pressure distribution in a gel:
9 V9V x
p(x) 9 p(0) : [2.5]
8 d d
where p(x) 9 p(0), , V, V and d are pressure gaps between the two positions 0
(on the gel surface) and x (at x in the gel from the gel surface) in the direction of
the ﬁeld, dielectric constant, voltages on the gel surface and at x in the gel, and
the thickness of the gel, respectively.
This equation suggests that the pressure gradient generated in the gel is
proportional to the dielectric constant of the gel and to the square of an
electric ﬁeld. As the solvent content of the gel is ca. 98% in our experimental
system, the dielectric constant of the gel can be assumed to be the same as that
of the solvent. By taking the bending elasticity of the gel and the estimated
pressure, we could attain excellent agreement between our experimental data
and theoretical estimation (see Fig. 2.29).
In order to see the eﬀect of the polymer on the electrically induced deformation,
another type of experiment was carried out. A pair of plate electrodes were
Electrically active polymer materials 27
Height pulled up (mm)
0 200 400 600 800 1000
E (V/1.5 mm)
2.30 Dependence of drawn-up height of DMSO on the electric ﬁeld.
dipped in the solvent, and the DC ﬁeld was applied between the electrodes.
The solvent was pulled up between the electrodes (Fig. 2.30). The height was
theoretically estimated by the following equation:
h : ( 9 )(V/d)/ g [2.6]
where h, , , V, d, and g are liquid surface height, dielectric constant of the
gel, dielectric constant of vacuum, voltage applied, distance between the
electrodes, density of the gel and gravitational constant.
The curve in Fig. 2.30 was calculated to be one, and is in good agreement
with the experimental data. However, when we used a DMSO solution of
PVA, the height was much less than that observed in the solvent and,
furthermore, was extremely asymmetric on both electrodes (see Fig. 2.31). The
solution tends to climb up onto the cathode surface, but not onto the anode,
suggesting that the above equation is no longer applicable for the polymer
These phenomena imply that the polymer solution has the tendency to
retard the discharging process. The discharge retardation causes the accumu-
lation of the charge on the cathode side in the gel and enhances the pressure
gap between the cathode side and the anode side in the gel. Thus, the presence
of the polymer network also plays an important role in eﬃcient bending
For more detailed analysis, further quantitative investigation must be
28 Smart ﬁbres, fabrics and clothing
2.31 Climbing of PVA–DMSO solution onto an electrode under the ﬁeld.
184.108.40.206 Applicability of the ‘charge-injected solvent drag’ method for conventional
The concept proposed in the previous section can be described as the
‘charge-injected solvent drag’ method. The advantage of the method is its
wide applicability to conventional non-ionic polymeric gel-like materials. We
have been working on several non-ionic materials for soft artiﬁcial muscles
that can be actuated in air.
Here, the case of poly(vinyl chloride) (PVC) will be shown brieﬂy. In the
case of PVC, we used plasticizers as solvent. Although tetrahydrofurane is a
good solvent for PVC, its boiling point is too low for the preparation of the
stable gel at ambient temperature in air. In the example shown, the PVC gel
plasticized with dioctylphthalate (DOP) was found to creep reversibly like an
amoeba by turning on and oﬀ the electric ﬁeld (see Fig. 2.32). The electrically
induced deformation was suggested to be the asymmetric distribution of the
injected charge. The mechanism is somewhat similar, but not the same, to that
for the non-ionic polymer gel, since the solvent ﬂow has not been conﬁrmed in
2.6 From electro-active polymer gel to electro-active
elastomer with large deformation
Non-ionic polymer gel swollen with dielectric solvent is shown to be extremely
deformed, as is the non-ionic polymer plasticized with non-ionic plasticizer.
Electrically active polymer materials 29
2.32 Creeping motion of poly(vinyl chloride) plasticized with
dioctylphthalate. PVC gel plasticized with dioctylphthalate (DOP) was
found to creep reversibly like an amoeba by turning the electric ﬁeld on
The mechanism suggested for the gel actuation was ‘charge-injected solvent
drag’, and that for the plasticized polymer was ‘asymmetric charge distribution
of injected charge’.
The latter mechanism can be applied to the non-ionic elastomers in
which the motion of the polymer chain is relatively free and so is the migra-
tion of the injected charges. The migration of the injected charge and the bal-
ance of the charging and discharging rates must be a critical factor to the
deformation provided the electrostatic interaction is a major factor in the
The experimental results on polyurethane elastomers support the concept
described above.— In addition to our expectations, some novel features of
the motion are being clariﬁed in detail, such as memory eﬀect, bending
direction control, and so on (Fig. 2.33).
30 Smart ﬁbres, fabrics and clothing
Highly swollen gel Plasticized polymer
Swift bending motion Creeping motion Swift motion
Crawling motion Huge deformation Memory effect
Charge injected solvent drag Bending direction control
Poor durability Huge deformation
2.33 Wide span of large deforming non-ionic electro-active actuator
materials from polymer gel, through plasticized polymer, to elastomer
with no additives. A prosperous future for the conventional non-ionic
polymer materials as autonomic materials can be expected.
In this chapter, various types of electroactive polymers were introduced. Some
of them have a long history as electroactive materials. Recently, however,
polymer gels and/or elastomers, which have no intrinsic polarization in their
structure and do not contain any ionic species either, have been found to show
huge strain by applying electric ﬁelds with a low electric current. Energy
dissipation occurring as heat is much less than the conventional polyelectrolyte
materials. The concepts of ‘charge-injected solvent drag’ and ‘asymmetric
charge distribution of injected charge’ are proposed as a possible mechanism
of the huge deformation. These concepts can be applied to various non-ionic
conventional polymers. The author strongly expects that the concepts expand
the ﬁeld of actuator to that of practical artiﬁcial muscle, and contribute to the
development of the micro-machine or nano-machine in the future.
The work described in this article is partly supported by Grants-in-Aid for
COE Research (10CE2003) and Scientiﬁc Research B(12450382), and by the
Regional Science Promoter Program of Nagano Prefecture. The author (TH)
expresses his sincere thanks for the support.
1 Polymer Gels. Fundamentals and Biomedical Applications, ed. DeRossi, Danilo,
Kajiwara, Kanji, Osada, Yoshihito and Yamauchi, Aizo, Prenum (1991).
2 Osada, Y and Kajiwara K (eds), Gel Handbook, NTS Publishing Co. Ltd. (1997).
3 Handbook of New Actuators for Accurate Controlling, Supervised by K Uchino, Fuji
Electrically active polymer materials 31
Technosystem Publishing Co. Ltd. (1994).
4 Organic Polymer Gels, Kikan Kagaku Sosetsu, No. 8, ed. by the Chemical Society of
Japan, Gakkai Shuppan Center (1990).
5 Recent Trends and Development of Polymer Gels — For Professionals in the Advanced
Technology Field, Supervised by Y Osada and Lin Wang, CMC Co. Ltd. (1995).
6 Uchino K, Piezo/Electrostrictive Materials, Morikita Publishing Co. Ltd. (1986).
7 Jikken Kagaku Koza (Experimental Chemistry Series), ed. by the Chemical Society
of Japan, 9 (1991).
8 Miyata S and Furukawa T, Ferroelectric Polymers, ed. by Polymer Society of
Japan, New Polymer Materials, One Point Series 14, Kyoritsu Publishing Co. Ltd.
9 Micromachine Research Laboratory, The University of Tokyo, Super Technology —
Micromachine, NTT Publishing Co. (1993).
10 Fujita H, The World of Micromachine, K Books Series 85, Kogyochosakai
Publishing Co. Ltd. (1992).
11 Actuator Research Group, New Actuators Targeting Microworld, K Books Series
103, Kogyochosakai Publishing Co. Ltd. (1994).
12 Kinoshita G, Soft Machine, New Corona Series 16, Corona Publishing Co. Ltd. (1992).
13 Bar-Cohen Y, ‘Electroactive Polymer Actuators and Devices’, Proceedings of SPIE,
14 Bohannan G W, Schmidt V H, Conant R J, Hallenberg J H, Nelson C, Childs A,
Lukes C, Ballensky J, Wehri J, Tikalsky B and McKenzie E, ‘Piezoelectric polymer
actuators in a vibration isolation application’, Proceedings of SPIE, 3987, 331 (2000).
15 Wang H, Zhang Q M, Cross L E and Sykes A O, ‘Piezoelectric, dielectric, and
elastic properties of poly(vinylidene ﬂuoride/triﬂuoroethylene), J. Appl. Phys., 74,
16 Mazzoldi A and DeRossi D, ‘Conductive polymer based structures for a steerable
catheter’, Proceedings of SPIE, 3987, 271 (1999).
17 MacDiarmid A G and Epstein A J, ‘Polyanilines: A novel class of conducting
polymers’, Faraday Discussions, 1989, n. 88, 317.
18 Baughman R H, ‘Conducting polymer artiﬁcial muscles’, Synthetic Metals, 78, 339
19 Gandhi M R, Murray P, Spinks G M and Wallace G G, ‘Mechanism of
electromechanical actuation in polypyrrole’, Synthetic Metals, 73, 247 (1995).
20 Hirai T, Hanaoka K, Suzuki T and Hayashi S, ‘Preparation of oriented hydrogel
membrane’, Kobunshi Ronbunshu, 49, 613 (1989).
21 Hirai T, ‘Artiﬁcial muscle’, Shin-Sozai (New Materials), No. 4 (1992).
22 Suzuki M, ‘Nonlinear mechanochemical systems’, Nippon Gomu Kyokaishi, 60, 702
23 Osada Y, ‘Chemical valves and gel actuators’, Adv. Mater., 3, 107 (1991).
24 Hirai T, Asada Y, Suzuki T, Hayashi S and Nambu M, ‘Studies on elastic hydrogel
membrane. I. Eﬀect of preparation conditions on the membrane performance’, J.
Appl. Polym. Sci., 38, 491 (1989).
25 Hirasa O, Morishita Y, Onomura R, Ichijo H and Yamauchi I, ‘Preparation and
mechanical properties of thermo-responsive ﬁbrous hydrogels made from poly(vinyl
methyl ethers)’, Kobunshi Ronbunshu, 46, 661 (1989).
26 Okano T, Bae Y H and Kim S W, ‘Temperature dependence of swelling of
32 Smart ﬁbres, fabrics and clothing
crosslinked poly(N,N-alkyl substituted acrylamides in water’, J. Controlled
Release, 11, 255 (1990).
27 Tanaka T, Sato E, Hirokawa Y, Hirotsu S and Peeternians J, ‘Critical kinetics of
volume phase transition of gels’, Phys. Rev. Lett., 55, 2455 (1985).
28 Tokita M and Tanaka T, ‘Reversible decrease of gel-solvent friction’, Science, 253,
29 Kokufuta E, Zhang Y-Q and Tanaka T, ‘Saccharide-sensitive phase transition of a
lectin-loaded gel’, Nature, 351, 302 (1991).
30 Kokufuta E, ‘New development of immobilized enzymes’, Hyoumen (Surfaces), 29,
31 Tanaka T, ‘Phase transitions in ionic gels’, Phys. Rev. Lett., 45, 1636—1639 (1980).
32 Irie M, ‘Photoresponsive polymers’, Adv. Polymer Sci., 28 (1989).
33 Takamizawa T, Hirai T, Hayashi S and Hirai M, ‘Magnetostriction of a gel
immobilizing superparamagnetic ﬂuid’, Proceedings of International Symposium on
Fiber Science and Technology (ISF’94), in Yokohama, 293 (1994).
34 Hirai T, ‘Electrically and magnetically active gel’, ZairyoKagaku (Materials
Science), 32, 59 (1995).
35 Hirai T, Takamizawa T and Hayashi S, ‘Structural change induced in the gel
immobilizing superparamagnetic ﬂuid’, Polym. Preprints, Jpn., 43, 3126 (1993).
36 Zryhni M, Barsi L and Buki A, ‘Deformation of ferrogels induced by nonuniform
magnetic ﬁelds’, J. Chem. Phys., 104, 20 (1996).
37 Zryhni M, Barsi L, Szabo D and Kilian H-G, ‘Direct observation of abrupt shape
transition in ferrogels induced by nonuniform magnetic ﬁeld’, J. Chem. Phys., 106,
38 Zryhni M and Horkai F, ‘On the thermodynamics of chemomechanical energy
conversion realised by neutral gels’, J. Intell. Mater. Syst. and Struct., 4, 190 (1993).
39 Shiga T, Hirose Y, Okada A and Kurauchi T, ‘Bending of high-strength polymer gel
in an electric ﬁeld’, Kobunshi Ronbunshu, 46, 709 (1989).
40 Shiga T, Hirose Y, Okada A and Kurauchi T, ‘Bending of ionic polymer gel
caused by swelling under sinusoidally varying electric ﬁelds’, J. Appl. Polym. Sci., 47,
41 Shiga T, Fukumori K, Hirose Y, Okada A and Kurauchi T, ‘Plused NMR study of
the structure of poly(vinyl alcohol)—poly(sodium acrylate) composite hydrogel’, J.
Polym. Sci.: Part B: Polym. Phys., 32, 85 (1994).
42 Osada Y, Okuzaki H and Hori H, ‘A polymer gel with electrically driven motility’,
Nature, 355, 242 (1992).
43 Gong J P, Kawakami I, Sergeyev V G and Osada Y, ‘Electroconductive organogel.
3. Preparation and properties of a charge-transfer complex gel in an organic
solvent’, Macromolecules, 24, 5246 (1991).
44 Gong J P, Kawakami I and Osada Y, ‘Electroconductive organogel. 4. Electrodriven
chemomechanical behaviors of charge-transfer complex gel in organic solvent’,
Macromolecules, 24, 6582 (1991).
45 Oguro K, Kawami Y and Takanaka H, ‘An actuator element of polymer electrolyte
gel membrane-electrode composite’, Bull. Government Industrial Research Institute
Osaka, 43, 21 (1992).
46 Oguro K, Fujiwara N, Asaka K, Onishi K and Sewa S, ‘Polymer electrolyte
actuator with gold electrodes’, Proceedings of SPIE, 3669, 64 (1999).
Electrically active polymer materials 33
47 Mojarrad M and Shahinpoor M, ‘Noiseless propulsion for swimming robotic
structures using polyelectrolyte ion-exchange membrane’, Proc. SPIE, 1996 North
American Conference on Smart Structures and Materials, 2716, Paper no. 27, 183
48 Shahinpoor M, ‘Electro-mechanics of ion-elastic beams as electrically-controllable
artiﬁcial muscles’, Proc. SPIE, Electroactive polymer actuators and devices, 3669,
49 Hirai T, Maruyama H, Suzuki T and Hayashi S, ‘Shape memorizing properties of
poly(vinyl alcohol) hydrogel’, J. Appl. Polym. Sci., 45, 1849 (1992).
50 Hirai T, Nemoto H, Hirai M and Hayashi S, ‘Electrostriction of poly(vinyl alcohol)
gel — a possible application for artiﬁcial muscle’, J. Appl. Polym. Sci., 53, 79 (1994).
51 Errede L A, Osada Y and Tiers V D, ‘Molecular interpretation of chemo-mechanical
reponses in polymer liquid systems’, J. Intell. Mater. Systems Struct., 4, 2, 161 (1993).
52 Hirai M, Hirai T, Sukumoda A, Nemoto H, Amemiya Y, Kobayashi K and Ueki T,
‘Electrically induced reversible structural change of a highly swollen polymer gel
network’, J. Chem. Soc., Faraday Trans., 91, 473 (1995).
53 Hirai T and Hirai M, Polymer Sensors and Actuators, ed. Y Osada and D E DeRossi,
Chapter 8, p. 245, Springer-Verlag, Berlin, Heidelberg (2000).
54 Hirai T, Jianming Zheng and Watanabe M, Proc. of SPIE, SPIE’s 6th Annual
International Symposium on Smart Structures and Materials, Electro-active
Polymer Actuators and Devices, 3669, 209 (1999).
55 Zheng J, Watanabe M, Shirai H and Hirai T, ‘Electrically induced rapid
deformation of nonionic gel’, Chem. Lett., 500—501 (2000).
56 Hirai T, Zheng J, Watanabe M and Shirai H, ‘Autonomic gel and its application as
artiﬁcial muscle’, Zairyo Kagaku (Materials Science), 36, 186 (2000).
57 Yamaguchi M, Watanabe M and Hirai T, ‘Electrical actuation of poly(vinyl
chloride) gel’, Polym. Preprints, Jpn., 48, 2124 (1999).
58 Hirai T, Zheng J, Watanabe M and Shirai H, ‘Electro-active non-ionic gel and its
application’, Proceedings of SPIE, 3987, 281 (2000).
59 Hirai T, Zheng J, Watanabe M, Shirai H and Yamaguchi M, ‘Electroactive
nonionic polymer gel swift bending and crawling motion’, Materials Research
Society Symposium Proceedings, 600, 267—272 (2000).
60 Hirai T, Sadatoh H, Ueda T, Kasazaki T, Kurita Y, Hirai M and Hayashi S,
‘Polyurethane elastomer actuator’, Angew. Makromol. Chem., 240, 221 (1996).
61 Watanabe M, Yokoyama M, Ueda T, Kasazaki T, Hirai M and Hirai T, ‘Bending
deformation of monolayer polyurethane ﬁlm induced by an electric ﬁeld’, Chem.
Lett., 773 (1997).
62 Watanabe M, Suzuki M, Amaike Y and Hirai T, ‘Electric conduction in bending
electrostriction of polyurethanes’, Appl. Phys. Lett., 74, 2717 (1999).
63 Watanabe M, Kato T, Suzuki M, Amaike Y and Hirai T, ‘Bending electrostriction
in polyurethanes containing ions as contaminants or additives’, Jpn. J. Appl. Phys.,
38, Part 2, No. 8A, L872 (1999).
Heat-storage and thermo-regulated
textiles and clothing
3.1 Development introduction
The human body is itself is an automatic thermo-regulated organism. The
body constantly generates heat, CO and H O by the metabolism of food and
muscle activity. The human body controls the release speed of heat by blood
vessel dilatation or constriction, muscle and sweat gland activity, etc., and then
regulates the body temperature.
It has been shown that the most comfortable skin temperature is 33.4 °C.
When the temperature of any part of the skin diﬀers by within 1.5—3.0 °C of this
ideal temperature, the human body is unaware of the warmth or coolness. If
the diﬀerence is more than 4.5 °C, the human body feels discomfort. In
addition, a core body temperature of 36.5 °C is required, and a rise or fall of
1.5 °C can be fatal. A balance between the rates of heat loss and heat generated
must be maintained. When the thermal resistance of their clothing is
insuﬃcient, and a person stays in a relatively low temperature condition for a
long time, the body temperature drops. The human body must produce more
heat by eating more food or increasing exercise. Also, the body will adjust to
the heat loss by constricting the blood capillaries within the skin. Hypothermia
may result, if the core temperature is lower than 35 °C. Conversely, in a hot
environment, the body must cool itself. The body generates heat and the heat
absorbed by the skin from the environment must be dissipated. Under these
conditions the body will dilate the blood capillaries, which enables the
evaporation of water diﬀused from the body interior to increase, thereby
increasing the cooling eﬀect. This action is known as insensible perspiration. If
the environment temperature increases further, the body will activate sweat
glands and evaporate liquid water for increased cooling, known as sensible
perspiration. In some special environments, due to the high temperature or
high thermal resistance of the clothing, hyperthermia can result if the body
fails to dissipate suﬃcient heat.
Heat-storage and thermo-regulated textiles and clothing 35
The traditional heat insulation materials, for example, fabrics such as
cotton, hemp, silk, wool and polyester, polyamide and polyacrylic ﬁbre, etc.
provide a degree of resistance to body heat loss, which is determined by the
number of air pockets present in the fabric. The solar ray selective absorbing
textile that has been manufactured since the late 1980s can absorb the near
infra-red ray in the sun rays, and convert it to heat, thus enhancing the inner
temperature of the clothing. The far infra-red textile that has been produced
since the late 1980s can absorb the body’s irradiated far infra-red ray and turn
it to heat, enhancing thermal resistance. The ultra-violet absorbing and
cool-feeling fabric that has been industrialized since the beginning of the 1990s
can absorb the ultra-violet and reﬂect the near infra-red rays from the sun,
lowering the inner temperature of the clothing. All of these new functional
textiles are one-way thermo-regulated heat insulating materials.
To keep the skin temperature within the 30.4 to 36.4 °C interval, we must put
on or take oﬀ our clothing according to the external temperature. If clothing
could automatically change its thermal resistance according to the temperature,
it could control the speed of heat release, and then regulate the inner
temperature. We would not need to put it on or take it oﬀ very often, and the
proper inner temperature would not only increase body comfort, but also
3.1.2 Development history
The heat-storage and thermo-regulated textiles and clothing are newer
concepts: they are two-way thermo-regulated new products, and have been
studied for more than 30 years. The development history of heat-storage and
thermo- regulated textiles and clothing is outlined in Table 3.1.
Scientists have increasingly been studying the manufacture process and
properties of heat-storage and thermo-regulated textiles and clothing for
several decades. There will be more reports about basic, dynamic thermal
resistance and its applications in the near future.
3.2 Basics of heat-storage materials
There are three types of heat storage: sensible, latent and chemical reaction
heat storage. Latent heat storage is the most important way of storing heat,
and is also called ‘phase change heat storage’. Latent heat-storage materials
have been widely used for about 40 years.
The US National Aeronautics and Space Administration (NASA) accelerated
the application research of latent heat-storage materials for the space
laboratory in the 1960s. They were used to improve the protection of
instruments and astronauts against extreme ﬂuctuations in temperature in
36 Smart ﬁbres, fabrics and clothing
Table 3.1 Development history of heat-storage and thermo-regulated textile and
Time Researcher Research introduction no.
1965 Mavelous and Designed a heat-insulating garment containing 1
Desy molten lithium salts pouches. The salts exchanged
heat with water in the pouches and the hot
water was circulated to tubing throughout the
1971 Hansen Incorporated CO2 into liquid inside the hollow ﬁbre. 2
When the liquid solidiﬁed and the solubility of the
CO2 decreased, the diameter of ﬁbre increased and
the heat-insulating ability rose.
1981 Vigo and Frost Incorporation of hydrated inorganic salts into 3
1983 Vigo and Frost Incorporation of polyethylene glycol (PEG) and 4
plastic crystal materials into hollow rayon or
1985 Vigo and Frost Coated PEG on the surface of fabrics. The thermal 5
storage and release properties of the fabrics were
reproducible after 150 heating and cooling cycles.
Chemical Week and Wall Street Journal reviewed 6, 7
Vigo’s research work.
1987 Bruno and Vigo The thermal storage and release, anti-static, water 8
absorbence, reliancy, soil release and conditional
wrinkle recovery of PEG-coated fabrics were
1988 Bryant and A ﬁbre with integral microcapsules ﬁlled with 9
Colvin phase change materials (PCM) or plastic crystals
had enhanced thermal properties at predetermined
Vigo and Bruno PEG was cross-linked on the surface of knit fabrics. 10
1989 Vigo et al. Coated PEG modiﬁed the resiliency and resistance 11
to the oily soiling, static charge, pilling, wear life
and hydrophilicity of fabric and ﬁbres.
1990 Watanabe et al. Melt spun heat-releasing and heat-absorbing 12
composite ﬁbre using aliphatic polyester as core or
island component, ﬁbre-forming polymer as sheath
or sea component.
1991 Zhang Designed the heat insulation clothing containing 13
Mitsui Corp. Licensed Vigo’s invention and commercialized 14
skiwear and sportswear that contain fabrics with
Neutratherm Licensed Vigo’s invention and commercialized 14
Corp. fabrics incorporating PEG. The fabrics were used
for thermal underwear.
1992 Mitamura A composite ﬁbre was melt spun by using 15
polytetramethylene glycol (av. MW 3000) as a
core, and poly(ethylene terephthalate) (PET) as a
Heat-storage and thermo-regulated textiles and clothing 37
Table 3.1 (cont.)
Time Researcher Research introduction no.
1992 Bryant and Fabrics coated with a binder containing 16
Colvin microcapsules ﬁlled with PCM or plastic crystals.
1993 Vigo The antibacterial properties of PEG-coated fabrics 17
Umbile Fabrics were coated with a binder containing 18
microcapsules ﬁlled with PEG (av. MW 300–4000).
Momose et al. A blend of linear chain hydrocarbon, particles of 19
ZrC, thermoplastic elastomer and polyethylene is
used as a coating materials for nylon fabrics
Colvin and A cooling garment contained pouches containing 20
Bryant macroencapsulated PCM.
1994 Renita et al. The wicking effect, antibacterial and liquid barrier 21
properties of non-woven coated with PEG were
Bruno and Vigo Formaldehyde-free cross-linking PEG-coated fabrics 22
Bruno and Vigo The dyeability of PEG-coated polyester/cotton fabric 23
Tsujito et al. Carpet coated with a binder containing 24
microcapsules ﬁlled with parafﬁn.
Imanari and Heat insulation clothing with pouches containing 25
Yanatori parafﬁn and salts was designed.
1995 Pause The basic and dynamic thermal insulation of fabrics 26
coated with or without microencapsulated PCM
1996 Zhang et al. The heat storage and crystallizability of PET–PEG 27
block copolymers were studied.
Zhang et al. Melt spun composite ﬁbre using aliphatic polyester, 28
PET–PEG, parafﬁn or PEG as core component,
ﬁbre-forming polymer as sheath component.
Sayler PCM with melting point 15–65 °C incorporated 29
throughout the structure of polymer ﬁbres.
1997 Zhang et al. Melt spun heat-storage and thermo-regulated 30
composite ﬁbre using PEG (av. MW 1000–20 000) as
core component, polypropylene as sheath
Outlast Inc. Properties of the ﬁbres were studied. 31
Frisby Inc. Coated fabrics and wet spinning polyacrylic ﬁbre 32
containing microencapsulated PCM came onto the
Vigo Intelligent ﬁbrous substrates with thermal and 33
dimensional memories were studied.
1999 Pause The basic and dynamic thermal insulation of coated 34
fabrics and non-woven containing
microencapsulated linear chain hydrocarbons were
studied, and the skin temperature of a simulated
skin apparatus in 20 °C and − 20 °C conditions were
38 Smart ﬁbres, fabrics and clothing
space. Latent heat-storage materials were used in the lunar vehicle and the Sky
lab project for the Apollo 15 mission in the 1980s.
3.2.1 Sensible heat-storage materials
There is an obvious temperature change during the heat-absorbing and release
process of sensible heat-storage materials. Water, steel and stone are widely
used sensible heat-storage materials. Water is the cheapest, most useful
sensible heat-storage materials in the temperature interval from 1 °C to 99 °C
at 1 standard atmosphere. The absorbing heat content of water for a 1 °C rise
in temperature is 4.18 J/g.
3.2.2 Latent heat-storage materials
Latent heat-storage materials are also called phase change materials (PCM).
PCM can absorb or release heat with a slight temperature change. PCM may
be repeatedly converted between solid and liquid phases to utilize their latent
heat of fusion to absorb, store and release heat or cold during such phase
conversions. The latent heats of fusion are greater than the sensible heat
capacities of the materials.
Material usually has three states. When a material converts from one state
to another, this process is called phase change. There are four kinds of phase
change, 1 solid to liquid, 2 liquid to gas, 3 solid to gas, 4 solid to solid.
Heat is absorbed or released during the phase change process. The absorbed
or released heat content is called latent heat. The PCM, which can convert
from solid to liquid or from liquid to solid state, is the most frequently used
latent heat-storage material in the manufacture of heat-storage and thermo-
regulated textiles and clothing. The melting heat-absorbing temperature
interval is from 20 to 40 °C, and the crystallization heat-releasing temperature
interval is from 30 to 10 °C. The phase change temperature of hydrated
inorganic salts, polyhydric alcohol—water solution, polyethylene glycol (PEG),
polytetramethylene glycol (PTMG), aliphatic polyester, linear chain hydro-
carbon, hydrocarbon alcohol, hydrocarbon acid, etc., is in this interval.
220.127.116.11 Hydrated inorganic salts
Hydrated inorganic salt is an inorganic salt crystal with n water molecules.
The hydrated inorganic salt that can be used in the manufacture of heat-storage
and thermo-regulated textiles and clothing usually has a heat-absorbing and
-releasing temperature interval of about 20 to 40 °C. Some of the hydrated
inorganic salts are listed in Table 3.2. It was observed that incongruent
melting and super cooling of most inorganic salt hydrates incorporated into,
Heat-storage and thermo-regulated textiles and clothing 39
Table 3.2 The hydrated inorganic salts35
Density heat capacity Heat-
Melting Melting kg/m3 (J/(kg K)) storage
Hydrated point heat density
inorganic salts (°C) (kJ/kg) Solid Liquid Solid Liquid (MJ/m3)
CaCI2.6H2O 29 190 1800 1560 1460 2130 283
LiNO3.3H2O 30 296
Na2SO4.10H2O 32 225 1460 1330 1760 3300 300
CaBr2.6H2O 34 138
Na2HPO4.12H2O 35 205
Zn2SO4.6H2O 36 147 1340 2260
Na2SO4.5H2O 43 209 1650 1460 2300 345
or topically applied to, ﬁbres occurred after several heating/cooling cycles.
Lithium nitrite trihydrate lasted 25 cycles, calcium chloride hexahydrate
lasted only a few cycles, and sodium sulfate decahydrate only one cycle.
18.104.22.168 Polyhydric alcohol
2,2-Dimethyl-1,3-propanediol (DMP), 2-hydroxymethyl-2-methyl-1,3-
ropanediol (HMP) and 2-bis-(hydroxyl methyl)-1,3-propanediol are often
used as PCM. They produce endothermic and exothermic eﬀects without a
change in state at temperatures far below the melting point of the substance;
the heat absorption and release of such substances is called the heat of
transition. However, they are not suitable for the manufacture of heat-storage
and thermo-regulated textiles and clothing due to their phase change tem-
perature being higher than 40 °C. However, if two of the polyhydric alcohols
are mixed, the phase change temperature can be in the range 24 to 40 °C.
22.214.171.124 PEG and PTMG
Polyethylene glycol is one of the most important PCMs. The melting
temperature of PEG is proportional to the molecular weight when its molecular
weight is lower than 20 000. The melting point of PEG that has an average
molecular weight higher than 20 000 is almost the same. The PEGs with
molecular weight lower than 20 000 are listed in Table 3.3. The PEGs with
molecular weight from 800 to 1500 have melting points of about 33 °C.
The maximum theory melting point of PTMG is 43 °C. The PTMG is used
as PCM in some patents. The melting point of PTMG with molecular weight
3000 is 33 °C, and the heat of melting is 150 J/g. However, the crystallization
40 Smart ﬁbres, fabrics and clothing
Table 3.3 The phase change behaviour of different molecular weight PEG
measured with DSC37
Average Melting Crystallization
PEG molecular Melting heat Crystallization heat
sample weight point (kJ/kg) point (kJ/kg)
1 400 3.24 91.37 − 24.00 85.40
2 600 17.92 121.14 − 6.88 116.16
3 1000 35.10 137.31 12.74 134.64
4 2000 53.19 178.82 25.19 161.34
5 4000 59.67 189.69 21.97 166.45
6 6000 64.75 188.98 32.89 160.93
7 10 000 66.28 191.90 34.89 167.87
8 20 000 68.70 187.81 37.65 160.97
point is supercooling due to the weak interaction between the molecular chain
of PTMG. This limits its application.
126.96.36.199 PET—PEG block copolymer
When the average molecular weight of PEG used in the synthesis of PET—PEG
block copolymer is higher than 1540, and the PEG weight content in block
copolymer is more than 50%, the PEG segment can crystallize alone. The
melting point measured by DSC of the PEG segment is 6.86 °C. When the
average molecular weight of PEG is 4000, and PEG weight content is 50%,
the melting point of the PEG segment is 33.05 °C, and the melting endotherm
is 30.56 J/g. The PET—PEG block copolymer can be melt spun into ﬁbre.
188.8.131.52 Linear chain hydrocarbon
Linear chain hydrocarbon is a byproduct of oil reﬁning. The formula is
CH . The melting and crystallization points of hydrocarbons with
n : 16 : 21 are in the temperature range 10 to 40 °C, Table 3.4. The commodity
linear chain hydrocarbon is usually a mixture of n 1 or n 2.
Linear chain hydrocarbons are a non-toxic, inexpensive, extensive source of
raw materials, suitable for varied usage. They are the most important PCMs
in the manufacture of heat-storage and thermo-regulated textiles and clothing.
Organic acid, alcohol and ether, for example decanoic acid, 1-tetradecanol,
and phenyl ether, at proper phase change temperature, can also be used as PCMs.
Heat-storage and thermo-regulated textiles and clothing 41
Table 3.4 The phase change properties of linear chain hydrocarbons9,25
Number Melting Heat of Crystallization
Phase change of carbon point melting point
materials atoms (°C) (kJ/kg) (°C)
n-hexadecane 16 16.7 236.58 16.2
n-heptadecane 17 21.7 171.38 21.5
n-octadecane 18 28.2 242.44 25.4
n-eicosane 20 36.6 246.62 30.6
n-heneicosane 21 40.2 200.64
3.3 Manufacture of heat-storage and thermo-regulated
textiles and clothing
3.3.1 Phase change materials or plastic crystal-ﬁlled or
184.108.40.206 Hydrated inorganic salt-ﬁlled or -impregnated ﬁbres
Vigo and Frost ﬁlled hollow rayon ﬁbres with LiNO .3H O, Zn(NO ) .6H O,
CaCl .6H O/SrCl .6H O and Na SO .10H O/NaB O .10H O. When the
content of lithium nitrate trihydrate within the rayon is 9.5 g per gram of ﬁbre,
the heat endotherm is 302.63, 312.24 and 156.32 J/g, respectively, and the heat
exotherm is 221.95, 176.39 and 40.96 J/g, respectively, in the temperature
interval 9 40—60 °C, after one, ten and 50 heat—cool cycles. It is quite obvious
that the decrease of heat capacity of the ﬁbre is greater after more heat—cool
220.127.116.11 PEG-ﬁlled or -impregnated ﬁbres
Although many inorganic salt hydrates within hollow ﬁbres were initially
eﬀective in imparting heat-absorbing and -releasing characteristics to hollow
ﬁbres, they exhibited unreliable and poor thermal behaviour on repeated
thermal—cool cycles. In 1983, Vigo and Frost ﬁlled ﬁbres with 57% (wt./wt.)
aqueous solution of PEG, with average molecular weight (average MW) of
400, 600, 1000 and 3350. Hollow ﬁbres were ﬁlled with PEG by aspirating
aqueous solutions of the various diﬀerent average molecular weights at, or
above, room temperature through ﬁbre bundles tightly aligned inside an
O-ring until visual observation indicated that the ﬁbres were completely ﬁlled.
The ﬁlled ﬁbres were then placed horizontally and cooled at 9 15 °C or lower.
Excess moisture was removed from the modiﬁed ﬁbres by drying them to
constant weight in the presence of anhydrous CaSO (a) in a desiccator for
24 h. The measured results of DSC show that the heat-absorbing and -releasing
42 Smart ﬁbres, fabrics and clothing
capacity of ﬁlled hollow polypropylene ﬁbre is 1.2—2.5 times that of untreated
ﬁbre, and that of ﬁlled hollow rayon is 2.2—4.4 times that of untreated rayon.
18.104.22.168 Polyhydric alcohol ﬁlled or -impregnated ﬁbre
Vigo and Frost ﬁlled hollow rayon and hollow polypropylene ﬁbre with
2,2-dimethyl-1,3-propanediol (DMP) and impregnated non-hollow rayon
with DMP. The heat-absorbing capacity of treated hollow polypropylene
ﬁbre was 136.68 J/g in the temperature range 72—102 °C, and the heat-releasing
capacity of treated hollow polypropylene ﬁbre was 120.38 J/g in the temperature
range 77—47 °C. It is less obvious that there is a decrease of the heat capacity
of the ﬁbre after 50 heat—cool cycles. The ﬁbre is not suitable for clothing
textiles, due to its high phase change temperature.
3.3.2 Coated fabric
22.214.171.124 Fabrics coated with PEG
Although the PEG and polyhydric alcohols were eﬀective as heat-storage and
-release agents in modiﬁed ﬁbres/fabrics, they were only suitable for applications
that did not require laundering of the fabrics, since they were still water
soluble. Vigo and Frost studied fabrics coated with cross-linked PEG in
1985. The average MW of PEG was from 600 to 8000. Fabrics were treated
with aqueous solutions containing the following cross-linking agents: 40%
solids dimethyloldihydroxy-ethyleneurea (DMDHEU), 40% solids
dimethylolethyleneurea (DMEU), 50% solids dimethylolisopropyl carbamate
and 80% solids trimethylolmelamine. Acid catalysts used were
MgCI .6H O/citric acid in a mole ratio of 20 to 1, NaHSO and
Zn(NO ) .6H O. PEG was also present in the pad bath. The cotton, PET and
wool fabrics having thermal activity were produced using 50% aqueous
solutions of the PEG-600 or PEG-1000 containing 8—12% DMDHEU and
2.4—3.6% mixed catalysts (MgCl .6H O/citric acid). All fabrics were padded
to wet pickup of about 100%, dried and cured, then machine washed and
dried. The PET treated with 50% aqueous solution of PEG-600, was dried at
60 °C for 7 minutes, and cured at 160 °C for 3 minutes. The weight gains were
42.9%, and the heat-absorbing capacity was 53.92 J/g measured by diﬀerential
scanning calorimetry (DSC). The heat capacity was 53.08 J/g after ten heat—cool
cycles. There was no obvious decrease of the heat capacity of the ﬁbre. The
heat-absorbing capacity of untreated polyester fabric was 42.21 J/g and 40.12 J/g.
If the weight gains of the fabric were less than 20%, only the antistatic
performance of the fabric was improved, and the thermal activity was not
obvious. Fabrics treated with PEG-600/DMDHEU and an appropriate acid
Heat-storage and thermo-regulated textiles and clothing 43
catalyst had weight gains of 27—47% and were thermally active compared to
the untreated and cross-linked controls. When concentrations of less than 8%
DMDHEU were used in the treatments with PEG-600, the weight gains were
not suﬃcient to impart thermal activity to the fabric. Conversely, when higher
concentrations of DMDHEU were used ( 9 12%) or when zinc nitrate catalysts
were used at any DMDHEU concentration, extensive cross-linking occurred
and the fabric was thermally inactive. When DMDHEU and the mixed acid
catalyst were used with PEG of higher molecular weights ( 9 3350), there was
little reaction, resulting in low add-on. Preliminary cross-link density and
thermal analysis data indicate that the PEG are insolubilized on the ﬁbres and
exhibit thermal activity only when the PEG are of low crystallinity and can
react with the polyfunctional cross-linking agent. Further experiments dem-
onstrated that a wide range of one-step curing conditions (with temperatures
as low as 80 °C) could be utilized to insolubilize the polymer on ﬁbrous
substrates and provide superior thermal storage and release properties than
those obtained by the two-step (dry/cure) process that employed high curing
However, the DMEHEU or DMEU can be gradually decomposed to
release toxic formaldehyde. A formaldehyde-free cross-linking system was
discovered using a stoichiometric amount of sulfonic acids and glyoxal to
form polyacetals with the same polyols. These polyacetals exhibit the same
multifunctional properties and are durable to laundering.
126.96.36.199 Fabrics coated with polyhydric alcohols
Polyhydric alcohols undergo solid-to-solid thermal transitions (SSTs). The
often-used plastic crystals are DMP (DSC onset mp 126 °C) and 2-
hydroxymethyl-2-methyl-1,3-propanediol (HMP, DSC onset mp 181 °C). The
50% (wt./wt.) aqueous solutions of the plastic crystals were made for subsequent
application to fabrics.
Regardless of ﬁbre type, all fabrics immersed in 50% aqueous solutions of
the DMP and padded to about 100% wet pickup, then dried at 100 °C, had
only slight weight gains after conditioning. Presumably, the high vapour
pressure of the DMP precludes the conventional or elevated temperature
drying of treated fabrics.
In contrast to the other plastic crystal substance DMP, the HMP did not
volatilize from the fabric when it was dried at conventional or elevated
temperature to remove excess water. The modiﬁed fabrics had heat contents
of 87.78—104.5 J/g on heating and 79.42—96.14 J/g on cooling after one to ten
thermal cycles. The heat contents of HMP-treated fabrics were 1.7—2.5 times
those of untreated fabrics. The fabrics are not suitable for clothing textiles, due
to their high phase change temperature.
44 Smart ﬁbres, fabrics and clothing
188.8.131.52 Fabrics coated with a binder containing microcapsules
Bryant adapted a coating to apply to a substrate such as a fabric in order to
enhance the thermal characteristics thereof. The coating includes a polymer
binder in which are dispersed integral and leak-resistant microcapsules ﬁlled
with PCM or plastic crystals that have speciﬁc thermal properties at predeter-
Zuckerman invented a coating composition for fabrics including wetted
microcapsules containing PCM dispersed throughout a polymer binder, a
surfactant, a dispersant, an antifoam agent and a thickener. The most
preferred ratios of components of the coating composition of the invention
were: 70 to 300 parts by dry weight of microcapsules for each 100 parts by dry
weight of acrylic polymer latex, 0.1% to 1% dry weight each of surfactant and
dispersant to dry weight of microcapsules, water totalling 40% to 60% of the
ﬁnal wet coating composition and antifoam agent of from 0.1% to 0.5% dry
weight to total weight of the ﬁnal wet coating composition.
The microcapsules containing Na SO .10H O as PCM were also used for
the fabric coating.
Umible had coated a woven polyester with a mixture of microcapsules and
polymer binder. The coating layer is composed of 1: 1—3 (wt. ratio) mixtures
of microcapsules containing PEG with average MW 300—4000 and a polyacrylic
binder. The coated fabric evolves heat at 7—11 °C, and absorbs heat at
28—31 °C. Umible thought the fabrics were useful for garments for workers in
freezer units and mountaineering.
184.108.40.206 Other coated fabrics
Momose invented a coating agent containing n-octadecane 80, n-hexadecane
20, thermoplastic elastomer kraton G1650 12, linear polyethylene 20, ZrC 10
and an antioxidant 0.2 part. The mixture was melted and mixed to give a
non-bleeding solid with heat content 129.48 J/g and good shape-retaining
properties. The mixture was molten at 140 °C and applied to a nylon cloth to
give a textile with good heat storage properties, useful for skiwear.
Heat-storage and thermo-regulated textiles can be manufactured by ﬁlling
hollow ﬁbres or impregnating non-hollow ﬁbres with PCM and plastic
crystals or coating fabric surfaces with PEG, plastic crystals or microcapsules.
There are still some defects in the wash-resistance, durability and handle of the
heat-storage and thermo-regulated textiles produced by these processes. The
ﬁbre-spinning process has developed quickly since the 1990s.
Heat-storage and thermo-regulated textiles and clothing 45
220.127.116.11 Composite ﬁbre-spinning
The copolymers of diacid, for example, glutaric acid, hexanedioic acid and
decanedioic acid, with diols, for example, 1,3-propylene glycol, 1,4-butanediol
and 1,6-hexanediol have heat-absorbing and -releasing properties. The
melting points of some of the aliphatic polyesters are in the temperature range
20—40 °C, but their crystallization points are usually beyond the temperature
range 30—10 °C. Watanabe used the mixture of two aliphatic polyesters as
the core component, PET as the sheath component, and melt span to produce
heat-absorbing and heat-releasing synthetic conjugate ﬁbres for heat-insulating
PTMG was used as the core component in the composite ﬁbre-spinning
process. A composite ﬁbre that uses PTMG as the core and PET as the
sheath was designed.
18.104.22.168 Fibre spun with a mixture
When aliphatic polyester or polyether is used alone as the core or island
component in the composite ﬁbre-spinning process, the spinning process is
very hard to control, due to its very low melting viscosity. If the aliphatic
polyester or polyether is blended with ethylene copolymer, the melting viscosity
of the mixture can be high enough for the ﬁbre-spinning process.
Zhang et al. had studied the melt spinnability of PEG alone, and PEG
mixed with ethylene—vinyl acetate as the core component, and polypropylene
as the sheath. The results showed that the PEG could be spun alone only
when the average MW was higher than 20 000. When the average MW was
higher than 1000, it could be melt spun well for the PEG and ethylene—vinyl
acetate 1: 1 (wt./wt.) mixture. Sayler’s invention showed that the preferred
weight percentages are about 55% PCM, about 15—21% polyoleﬁn, about
7—11% ethylene copolymer, about 7—15% silica particles and about 7.5%
The mixture of paraﬃn and polyethylene was melt spun into the ﬁbre
directly. The surface of the ﬁbre was coated with epoxy resin in order to
prevent leakage of the paraﬃn.
22.214.171.124 Fibre with integral microcapsules
Embedding the microcapsules directly within the ﬁbre adds durability as the
PCM is protected by a dual wall, the ﬁrst being the wall of the microcapsule
and the second being the surrounding ﬁbre itself. Thus, the PCM is less likely
to leak from the ﬁbre during its liquid phase, thus enhancing its life and the
repeatability of the thermal response.
46 Smart ﬁbres, fabrics and clothing
Bryant and Colvin produced a ﬁbre with integral microcapsules with
PCMs or plastic crystals. The ﬁbre has enhanced thermal properties at
predetermined temperatures. The microcapsules can range in size from about
1 to about 10 microns. In fabricating the ﬁbre, the desired microencapsulated
PCMs are added to the liquid polymer, polymer solution or base material and
the ﬁbre is then expended according to conventional methods such as dry or
wet spinning of the polymer solutions and extrusion of the polymer melts.
According to the report, the maximum content of PCM in the polyacrylic
ﬁbre is about 10%. The minimum ﬁlament denier is 2.2dtex.
3.3.4 Heat-storage and thermo-regulated clothing
126.96.36.199 Water circulation clothing
This kind of clothing is usually used as protective clothing for extremely warm
or cool environments. It uses ordinary water as a sensible heat-storage
material, circulating warm water in winter and circulating cool water in
summer through tubing that is incorporated into the body garment or vest. A
battery-powdered pump circulates the water through the tubing in the suit
load. It has been commercialized for several decades.
188.8.131.52 PCM pouches attached to clothing
These garments were designed by Mavleous and Desy, Zhang, Colvin and
Imanari and Yanatori. They use PCMs instead of water as heat-storage
materials. They are used in extreme high or low temperature environments for
body cooling or warming.
184.108.40.206 Heat-storage and thermo-regulated textile clothing
As the manufacturing technology of heat-storage and thermo-regulated ﬁbres
and textiles became more advanced, new types of clothing came onto the
market. The PEG-coated fabrics produced by the Mitsui Corporation were
used as ski- and sportswear.
Outlast Inc. and Frisby Inc. licensed the thermal regulation technology
from Bryant of Triangle Research and Development Corporation in about
1991. Since then, the scientists at Outlast and Frisby have worked diligently to
create thermal regulating materials for use in many diﬀerent products. The
microcapsules were either coated onto the surface of a fabric or manufactured
directly into polyacrylic ﬁbres. Other heat-storage and thermo-regulated
textile products, such as blankets, sleeping bags, underwear, jackets, sports
garments, socks, ski boots, helmets, etc., have come onto the market since
1997. Output has gradually increased in the last 3 years.
Heat-storage and thermo-regulated textiles and clothing 47
3.4 Properties of heat-storage and thermo-regulated
textiles and clothing
3.4.1 Thermal resistance
220.127.116.11 Traditional thermal resistance
The traditional thermal resistance is measured by the standard stationary
methods (for example, those involving the use of a guarded hot plate apparatus).
But in Pause’s opinion, none of these methods is suitable for the determination
of materials with PCM, because a long continual thermal stress could activate
the phase change which would lead to measurements that deviate signiﬁcantly
from those that should be obtained. Some experiments are still necessary in
order to enable us to decide whether this is true.
The thermal resistance of coated fabrics with or without microcapsules was
measured by Zuckerman et al. The thermal resistance of coated fabrics with
microcapsules is higher than that of untreated fabrics; the results are listed in
Tables 3.5 and 3.6. That is mainly due to the action of binder that seals the
cloth pore of the fabric.
18.104.22.168 Dynamic thermal resistance
There are phase change materials on the surface of the ﬁbre or in the ﬁbre, so
the fabric or ﬁbre is going to absorb heat in the temperature range 20—40 °C,
and release it in the range 30—10 °C. Vigo and Frost studied the endotherm
and exotherm behaviour of the fabrics and ﬁbres by DSC.— The plots of
DSC measurement are shown in Fig. 3.1 and 3.2. But the DSC measuring
results were not translated to the thermal resistance of the textile.
When Neutratherm Corporation studied a wear trial with 50 human subjects
Table 3.5 Thermal resistance of coated fabrics40
Acrylic Acrylic Substrate Substrate
with without with without
Materials tested PCM PCM PCM PCM
Wt/unit area (g/m2) 270 250 227 207
Stand thickness (mm) 5.40 5.63 0.63 0.61
Compressibility (lb) 12 16 13 20
Raw density (kg/m3) 49 44 360 339
Thermal conductivity (w/m K) 0.0398 0.0342 0.1012 0.1782
Thermal resistance (m2 K/w) 0.1281 0.1491 0.0057 0.0029
Speciﬁc thermal capacity
(kJ/kg K) 3.022 2.391 2.468 1.840
48 Smart ﬁbres, fabrics and clothing
Table 3.6 The basic and dynamic thermal resistance of coated fabrics26
Basic thermal Dynamic thermal
Test material (m2 K/W) (m2 K/W)
Membrane material 0.0044
Membrane material/foam coating 0.0187
Membrane m./foam/40 g/m2 PCM 0.0181 0.0863
Membrane m./foam/90 g/m2 PCM 0.0176 0.1481
3.1 DSC cooling scans (10 °C/min) of melt-blown polypropylene treated
with PEG 1000/DMDHEU and dried/cured: (a) 1.5 min/90 °C and (b)
5 min/100 °C.
3.2 DSC heating scans (10 °C/min) of woven cotton pritcloth treated with
PEG-1450/DMDHEU and dried/cured: (a) 2 min/100 °C and (b) 4 min/80 °C.
Heat-storage and thermo-regulated textiles and clothing 49
5 1 6
3.3 Testing arrangement. 1: Radiant (panel) heater with temperature
sensor, 2: Testing sample, 3: Panel heater/cooler with temperature sensor,
4: Heat insulation, 5: Power supply for panel heater, 6: Computer for
recording and processing of measured values.
New design with PCM
0 0.5 1 1.5 2 2.5
Thermal resistance in clo
3.4 Comparison of the total thermal insulation of the coated fabrics.
, Basic thermal resistance; , Dynamic thermal resistance.
with cotton thermal underwear containing bound PEG, enhanced wind
resistance was the property giving the highest percentage of satisfaction (82%)
to the wearers.
In order to measure the basic and dynamic thermal resistance, Pause
designed a measurement method; the basic arrangement of the measuring
apparatus is presented in Fig. 3.3. The thermal resistance of the coated fabrics
with microcapsules is shown in Table 3.6. The total thermal insulation values
obtained for the coated fabrics with microcapsules containing linear chain
hydrocarbon compared to the thermal insulation of the materials without
microcapsules are shown in Fig. 3.4.
Pause compared the thermal insulation eﬀects of a batting (thickness
24 mm) of polyester ﬁbre, outer fabric (0.2 mm) and liner fabric (0.1 mm) with
50 Smart ﬁbres, fabrics and clothing
a batting (thickness 12 mm) of acrylic ﬁbre with incorporated PCM, outer
fabric (0.2 mm) and liner fabric with PCM-coating. The test results show
that the basic thermal insulation of the textile substrate is reduced by
approximately 30% when replacing the thick batting made of polyester ﬁbres
with a batting of acrylic ﬁbres with incorporated PCM only 12 mm thick.
However, the dynamic thermal insulation eﬀect resulting from the heat emitted
by the PCM inside the coated layer of the liner materials as well as inside the
batting ﬁbres more than doubled the thermal insulation eﬀect of the new
garment conﬁguration. The total thermal insulation eﬀect of the new garment
exceeds the total thermal insulation eﬀect of the previous garment by
The dynamic thermal resistance of any one heat-storage and thermo-regulated
fabric is not a constant. The dynamic thermal resistance of the fabric changes
with time during the measurement process: it should be like a Gaussian
distribution, just like the DSC plot. However, it is like a rectangle in Fig. 3.4.
Pause’s is the only report on dynamic thermal resistance. The main diﬃculty
is in the design of new testing apparatus.
3.4.2 Thermo-regulating properties
There is no standard method for measuring the thermal regulating properties
of heat-storage and thermo-regulated textiles and clothing. Much still needs to
Watanabe et al. attached the plain fabric containing aliphatic polyester and
the plain fabric containing PET on a metal plate. The temperature of the
plate was increased from room temperature to 40 °C, kept constant for a few
minutes, and then reduced from 40 °C to 5 °C. The surface temperatures of the
fabrics were recorded with an infra-red camera. The diﬀerence in the surface
temperatures of these two plain fabrics can be calculated from the infra-red
picture. The surface temperature of the fabric which is woven by ﬁbre
produced by poly(glutaric 1,6-hexanediol) as the core and PET as the sheath is
4.5 °C lower than that of the PET fabric at 40 °C, and 3.2 °C higher than that of
the PET fabric at 5 °C.
Vigo and Bruno’s preliminary experiments using infra-red thermograph
indicated that fabrics containing the cross-linked polyols had a surface
temperature diﬀerence as much as 15 °C lower than that of a corresponding
untreated fabric exposed to a heat source.
Neutratherm TM-treated cotton thermal underwear (based on Vigo’s
process) was evaluated during skiing and skiing-like conditions, and was
found by wearers to be superior to untreated cotton thermal underwear by
75% or more with regard to preventing overheating and chilling due to wind
and/or cold weather.
Heat-storage and thermo-regulated textiles and clothing 51
3.5 Comparison of the thermo-regulated effect of the previous and the
PCM garment design.
A thermal active ﬁbre was manufactured using PEG (average MW 1000) as
the core and PP as the sheath. Zhang et al. manufactured a non-woven using
this ﬁbre. The temperature of a drying chamber with fan was kept steady at
50 °C. The temperature of a refrigerator was kept steady at 0 °C. The thermal
active non-woven and normal PP non-woven with the same area density were
attached on a thin metal plate. The inner temperature of these two non-woven
was measured by thermocouple thermometer during the temperature interval
up from 0 °C to 50 °C and down from 50 °C to 0 °C. The maximum inner
temperature diﬀerence of thermal active non-woven and normal PP non-woven
is 3.3 °C in a period when the temperature is rising, and 6.1 °C in a period when
the temperature is falling.
The garment containing PCM was tested in a climatic chamber at various
temperatures to determine the thermo-regulating eﬀect from heat absorption
and heat release of the PCM. In this test, the garment samples were attached
to a simulated skin apparatus, the temperature of which was measured over
time at various ambient temperatures and metabolic heat rates. Based on these
tests, time intervals were estimated within which the skin temperature could be
stabilized within a desired temperature range. The test results for the two
garments under ambient temperature exposures of 9 20 °C and ; 20 °C are
summarized in Fig. 3.5.
The results show that, at both ambient temperatures, the temperature of the
simulated skin on the back side of the new garment is stabilized in the comfort
temperature range between 31 °C and 35 °C. In Pause’s opinion, that means
the heat absorption and release of the PCM has created a thermo-regulating
eﬀect resulting in a comfortable microclimate temperature during the entire
test. On the other hand, in the test of the previous garment, the skin
temperature is in the discomfort temperature zones as low as 29 °C and as high
as 38 °C.
52 Smart ﬁbres, fabrics and clothing
In other reports, cold weather trials showed a usual drop of 3 °C in the skin
temperature for control and only 0.8 °C for the heat-storage and thermo-
3.4.3 Antibacterial properties
The PEG-coated fabrics gain not only absorbed and released heat, but also
antibacterial properties. The PEG-treated fabric can inhibit the growth of
gram-positive S. aureus and gram-negative E. coli and P. aeruginosa.
The mechanism by which PEG-treated fabrics inhibit bacterial growth is
being investigated by Vigo. It results from three factors. A slow release of
formaldehyde from the DMDHEU cross-linking resin may have an antibacterial
eﬀect, as formaldehyde can be used as a disinfecting agent. The PEG may
exhibit a form of surfactant behaviour, which also is known to reduce bacterial
growth. A third explanation relates to the ﬁnish imparting thermal absorption
and release properties. The temperature may reach beyond some micro-
organisms’ growth range, killing those species.
A thermal active non-woven were produced by PEG-treated 100%
polypropylene spun bonded-melt blown-spun bonded. The PEG-treated
non-woven inhibited bacterial growth. The most probable eﬀects that
inhibit microbial growth may be attributable to the surfactant-like properties
of the bond PEG, which disrupts cell membranes due to the dual
hydrophilic—hydrophobic characteristics of the PEG. This was reported in
Vigo and Leonas’s recent work.
3.4.4 Other properties
The cross-linked PEG treatment changes a fabric’s properties relative to
untreated fabrics. Properties imparted include heat-absorbing and -releasing,
antibacterial activity, resiliency/antiwrinkling, wear, toughness, absorbency
and exsorbency of liquids, improved abrasion and linting resistance, decreased
static propensity and increased oily soil release.
The possible applications of heat-storage and thermo-regulated textiles and
clothing are under development. There are many possible end uses of these
Heat-storage and thermo-regulated textiles and clothing 53
3.5.1 Casual clothing
Heat-storage and thermo-regulated textiles can be used as casual textiles, for
example, face fabric, liner fabric, batting, etc. Thermal underwear, jackets,
sports garments and skiwear have now come onto the market.
3.5.2 Professional clothing
Examples are ﬁreﬁghter uniforms, bullet-proof vests, diver’s coveralls, space
suits, airman suits, ﬁeld uniforms, sailor suits, etc. Special gloves for extremely
high or low temperatures are being studied. Personnel supporting the
operations of Air Force One now wear thermo-regulated ﬂight gloves.
3.5.3 Textiles for interior decoration, bedclothes and sleeping
Heat-storage and thermo-regulated textiles can be used as curtains, quilts,
quilt covers or batting. They are already used as sleeping bags.
3.5.4 Shoe lining
Heat-storage and thermo-regulated textiles can absorb, store, redistribute and
release heat to prevent drastic changes in the wearer’s head, body, hands and
feet. In the case of ski boots, the PCM absorbs the heat when the feet generate
excess heat, and send the stored heat back to the cold spots if the feet get chilly.
This keeps the feet comfortable. Ski boots, footwear and golf shoes are coming
onto the market.
3.5.5 Medical usage
PEG-treated fabric may be useful in medical and hygiene applications where
both liquid transport and antibacterial properties are desirable, such as
surgical gauze, nappies and incontinence products. Heat-storage and thermo-
regulated textiles can keep the skin temperature within the comfort range, so
they can be used as a bandage and for burn and heat/cool therapy.
3.5.6 Building materials
Such textiles can be used in architectural structures embedded in concrete, in
roofs and in other building materials.
54 Smart ﬁbres, fabrics and clothing
3.5.7 Other uses
They can be used as automotive interiors, and battery warmers. They can also
be used in agriculture and geotextiles.
3.6 Development trends
The manufacture, properties and applications of heat-storage and thermo-
regulated textiles have been extensively studied since the 1980s but their future
development is still not very clear. It is expected that similar importance will be
attached to improving comfort to the wearer as was seen in the development of
breathable membranes (Gore-Tex, Sympatex). These textiles were selected
as one of the ‘21 inventions that will shape the 21st century’ by the editorial
staﬀ of Newsday.
The traditional heat insulation textile, which works by trapping heat in the
dead-air spaces of a material, is meant to retain heat as long and eﬃciently as
possible. The heat-storage and thermo-regulated textile is not a traditional
textile or an evolutionary textile with higher heat insulation ability. The
heat-storage and thermo-regulated textile keeps you warm when it is cool and
cool when it is warm. It is a product that will make you more comfortable
during extreme temperature changes. Thus, it is an intelligent textile. When
the temperature changes dramatically, the inner temperature of the heat-storage
and thermo-regulated garment is stabilized in the comfort temperature range
between 31 °C and 35 °C.
The thermo-regulated properties of the garment oﬀered against extremes of
cold and/or heat are available only for a limited period however, depending on
the garment construction and the temperature of the environment. Thus it is
more useful in an environment in which the temperature is quickly changing
than in a steady temperature environment. However, if the released heat is not
absorbed quickly, or the absorbed heat is not released, the textile loses its
thermo-regulating function. To improve its durability, there is still much to be
3.6.1 Enhancing heat content
The maximum PCM load in the heat-storage and thermo-regulated polyacrylic
ﬁbre is 10%. In other words, the maximum heat content of the ﬁbre is 25 J/g.
The thermo-regulating function oﬀered against extremes of cold and/or heat is
available only for a limited period. The maximum heat content of the fabric is
over 40 J/g in patent application and heat content over 50 J/g is possible in
technology. The more PCMs there are in the textile, the longer the duration of
Heat-storage and thermo-regulated textiles and clothing 55
3.6.2 Combining heat-storage and thermo-regulated textiles
with trapped-air materials
The experiment results show that a thermo-regulated textile that can regulate
inner temperature eﬀectively must have enough high thermal resistance. How
to combine the heat-storage and release technology with the trapped-air
technology is an area for future research.
3.6.3 Combining with other energy conversion technology
The group VI transition metal carbon compound can convert near infra-red
rays into heat. If the particles of ZrC are added to the heat-storage and
thermo-regulated textile, they can absorb the near infra-red rays of the sun in
daylight and convert them into heat that makes the PCMs in the textile change
phase from solid to liquid. The textile releases its heat to keep its temperature
relatively steady when the inner temperature is lower than the crystallizing
point of the PCMs.
Some of the polyacrylic acid or polyacryl—nitrile copolymers can absorb
moisture from the air and release heat. They can be made into fabrics that can
regulate inner moisture and temperature but such fabrics are not durable for
limited moisture absorbency ability. If the moisture-absorbing fabrics are
laminated with heat-storage and thermo-regulated fabrics, the composite
fabrics can absorb moisture or heat and prevent drastic changes in the inner
temperature. This kind of fabric is useful for ski- and sportswear.
1 Mavleous M G and Desy J J, US Pat 3 183 653.
2 Hansen R H, ‘Temperature-adaptable fabrics’, US Pat 3 607 591.
3 Vigo T L and Frost C M, ‘Temperature-sensitive hollow ﬁbers containing phase
change salts’, Textile Res. J., 1982, 55(10), 633—7.
4 Vigo T L and Frost C M, ‘Temperature-adaptable hollow ﬁbers containing
polyethylene glycols’, J. Coated Fabrics, 1983, 12(4), 243—54.
5 Vigo T L and Frost C M, ‘Temperature-adaptable fabrics’, Textile Res. J., 1985,
6 ‘Fibers with built-in antifreeze’, Chemical Week, 1986, July 9, 20, 22.
7 ‘Fabrics that respond to changes in temperature may emerge from a textile
chemist’s research’, Wall St. Journal, 25 (June 13, 1986).
8 Bruno J S and Vigo T L, ‘Temperature-adaptable fabrics with multifunctional
properties’, Book Pap. — Int. Conf. Exhib., AATCC, 1987, 258—64.
9 Bryant Y G and Colvin D P, ‘Fiber with reversible enhanced thermal storage
properties and fabrics made therefrom’, US Pat 4 756 985.
10 Vigo T L and Bruno J S, ‘Properties of knits containing crosslinked PEG’, Book
Pap. — Int. Conf. Exhib., AATCC, 1988, 177—83.
56 Smart ﬁbres, fabrics and clothing
11 Vigo T L and Bruno J S, ‘Improvement of various properties of ﬁber surfaces
containing crosslinked polyethylene glycols’, J. Appl. Polym. Sci., 1989, 37, 371—9.
12 Watanabe T, Matsumoto T and Toshikazu A, ‘Heat-evolving heat-absorbing
synthetic conjugate ﬁbers for insulative garments’, JK6-41818.
13 Zhang P R, ‘Heat-Storage Garment’, CN2107799U.
14 Vigo T L and Bruno J S, ‘Fibers with multifunctional properties: a historic
approach’, Handbook of Fiber Science and Technology, Volume III, High Technology
Fibers Part C, Menachem Lavin, Jack Preston, Marcel Dekker, Inc., 1993.
15 Mitamura H, ‘Synthetic conjugate ﬁbers with latent heat and their manufacture’,
16 Bryant Y G and Colvin D P, ‘Fabric with reversible enhanced thermal properties’,
US Pat 5 366 801.
17 Vigo T L, ‘Antimicrobial acting of cotton fabrics containing crosslinked polyols’,
Proc. — Beltwide Cotton Conf., 1993, (3), 1424—5.
18 Hiroyoshi U, ‘Heat-evolving and heat-absorbing fabrics’, JK7-70943.
19 Chiaki M, Toshinori F and Wataru S, ‘Heat-storing textile products’, JK5-214672.
20 Colvin D P and Bryant Y G, ‘Micro-climate cooling garment’, US Pat 5 415 222.
21 Jinkins R S and Leonas K K, ‘Inﬂuence of a polyethylene glycol treatment on
surface, liquid barrier and antibacterial properties’, Text. Chem. Colorist, 1994,
22 Bruno J S and Vigo T L, ‘Thermal properties of insolubilized polyacetals derived
from non-formaldehyde crosslinking agents’, Thermochim. Acta, 1994, 243(2), 155—9.
23 Bruno J S and Vigo T L, ‘Dyeing of cotton/polyester blends in the presence of
crosslinked polyols’, Am. Dyest Rep., 1994, 83(2), 34—7.
24 Tsujito Yatake, ‘Manufacture of heat-storage materials for bedding and clothing’,
25 Imanari M and Yanatori Midio, ‘Heat-storing materials’, JK8-29081.
26 Pause B, ‘Development of heat and cold insulating membrane structures with phase
change material’, J. Coated Fabrics, 1995, 25(7), 59.
27 Zhang X X, Zhang H, Hu L et al., ‘Crystallizable and heat-storage properties of
PET—PEG block copolymers’, Mater. Rev., 1996, 10(6), 63.
28 Zhang X X, Zhang H, Niu J J et al., ‘Thermoregulated ﬁber and its products’, China
Pat ZL96 105 229 5.
29 Sayler I O, ‘Phase change materials incorporated through the structure of polymer
30 Zhang X X, Wang X C, Hu L et al., ‘Spinning and properties of PP/PEG composite
ﬁbers for heat storaging and thermoregulated’, J. Tianjin Inst. Text. Sci. Technol.,
1999, 18(1), 1.
31 ‘This sporting life’, Textile Month, 1998, (12), 12—13.
32 ‘Blowing Hot and Cold to Balance Yin and Yang’, Textile Month, 1999, (12), 16—18.
33 Vigo T L, ‘Intelligent ﬁbers substrates with thermal and dimensional memories’,
Polymer Adv. Technol., 1997, 8(5), 281—8.
34 Pause B H, ‘Development of new cold protective clothing with phase change
material’, Int Con Safety and Protective Fabrics, April 29—May 1, 104, 1998.
35 Hale D V, Hoover M J and O’Neill M J, ‘Phase Change Materials Handbook
Report’, NASA CR61363, Lockheed Missiles and Space Co., Sept. 1971.
36 Zhang Y P, Hu H P, Kong X D et al., Phase Change Heat Storage Theory and
Heat-storage and thermo-regulated textiles and clothing 57
Application, Hefei University of Science Technology of China Publishing House,
37 Son Change, Moreshouse H L and Jeﬀrey H, ‘An experimental investigation of
solid-state phase-change materials for solar thermal storage’, J. Sol. Energy Eng.,
1991, 113(4), 244—9.
38 Zhang X X, Zhang H, Wang X C et al., ‘Crystallisation and low temperature
heat-storage behaviour of PEG’, J Tianjin Inst. Textile Sci. Technol., 1997, 16(2), 11.
39 Vigo T L and Frost C M, ‘Temperature-adaptable textile ﬁbers and method of
preparing same’, US Pat 4 871 615.
40 Zuckerman J L, Perry B T, Pushaw R J et al., ‘Energy absorbing fabric coating and
manufacturing method’, WO 95/34609.
41 Zhang X X, Zhang H, Hu L et al., ‘Synthesis and crystallizable properties of
aliphatic polyester’, Synthetic Technol. Appl., 1997, 12(3), 10—14.
42 Vigo T L and Leonas K K, ‘Antimicrobial activing of fabrics containing crosslinked
PEG’, Text. Chem. Colorist Amer. Dyestuﬀ Reporter, 1999, 1(1), 42—6.
43 Vigo T L, ‘Intelligent ﬁber substrates with thermal and dimensional memories’,
Polym. Adv. Technol., 1997, 8(5), 281—8.
44 Oji Shunsaku, Fujimoto, Masanori Furata, ‘Thermally insulating synthetic ﬁbers
with selective solar absorpting’, JK1-132816.
Thermally sensitive materials
An ideal clothing fabric, in terms of thermal comfort, should have the
following attributes: (1) high thermal resistance for protection from the cold;
(2) low water vapour resistance for eﬃcient heat transfer under a mild thermal
stress conditions; and (3) rapid liquid transport characteristics for transferring
heat eﬃciently and eliminating unpleasant tactile sensations due to perspiration
under high thermal stress conditions.
Extremely cold weather protective clothing refers to garments that are used
in extreme climates such as on the Trans-Antarctica expeditions, in skiwear,
mountaineering and for army personnel posted in hilly areas at high altitudes.
For this purpose, clothing that provides a high degree of insulation with the
least amount of bulk is most desirable. For such applications, breathable
membranes and coatings, and high-loft battings of special ﬁbres in conjunction
with reﬂective materials have been suggested.—
For the International Trans-Antartica Expedition in 1990, the outerwear
was made with Gore-Tex fabric constructed of a highly porous membrane
bonded to a high performance textile. This outerwear was found to be
completely windproof and waterproof, yet ‘breathable’ to allow the body’s
perspiration vapour to escape. To encounter the harshest weather in the
Antarctic region, where winds can reach 150 miles per hour during storms and
temperatures fall to 9 46 °C, a layered clothing system has been developed to
enable the wearer to continually adjust his clothing to conserve and manage
his body heat.The protection of an individual in a cold environment would
depend on the following main factors: (1) metabolic heat, (2) wind chill, (3)
thermal insulation, (4) air permeability and (5) moisture vapour transmission.
Survival depends on the balance of heat losses due to (2)—(5) and heat output
due to metabolic heat (1).
US Army Research Institute of Environmental Medicine (USARIEM)
studies have examined the eﬀects of temperature and wind chill on a human
body and indicated that the sensations of warmth and cold at wind velocities
between 2 to 32 m/s may be as below:
Thermally sensitive materials 59
32 °C Hot
28 °C Pleasant
22 °C Cool
16 °C Very cool
10 °C Cold
5 °C Very cold
0 °C Bitterly cold
9 5 °C Exposed ﬂesh freezes
9 24 °C Exposed area of face freezes within one minute
9 32 °C Exposed area of face freezes within minute
Wind chill depends on the temperature as well as velocity of the wind. In
cold climates, consideration of the wind chill eﬀect is very important, because
80% of heat losses are due to wind chill.
Wind chill factor can be derived from the Siple Passel formula (source:
Slater K, J. Text. Inst. 1986 77(3) 157—171):
H : (10.45 ; (V 9 V)(33 9 T ) [4.1]
H : heat loss from the body in kcal/m/h,
V : wind velocity in m/s, and
T : air temperature in °C
The skin temperature under calm conditions is taken as 33 °C. The signiﬁcance
of the wind chill factor may be understood by reviewing its eﬀect on the
freezing time of exposed ﬂesh. At a wind chill factor of 1000, an individual
would feel very cold and at 1200, bitterly cold. When the wind chill factor is
1400, the exposed ﬂesh would freeze in 20 min, at a wind chill factor of 1800, the
exposed ﬂesh would freeze in 10 min, and when the wind chill factor is 2400,
exposed ﬂesh freezes in 1 min only.
It is evident from Table 4.1 that textile ﬁbres are much better conductors of
heat than air (i.e. bad insulators). Therefore, the ideal insulator would be still
air. However, there should be some means to entrap the air. Fibrous materials
serve this purpose eﬀectively as they have the capacity to entrap huge volumes
of air because of their high bulk. For example, a suiting fabric is 25% ﬁbre and
75% air; a blanket is 10% ﬁbre and 90% air; a fur coat is 5% ﬁbre and 95% air.
In other words, a textile-based thermal insulator should be capable of
entrapping maximum amount of air. The contribution of the ﬁbre itself to
thermal insulation comes second. The contribution of convection can be
reduced by optimizing the interﬁbre space. The heat loss due to radiation is
not signiﬁcant. In clothing for extreme cold regions, it is further reduced by
incorporating a thin layer of metal-coated ﬁlm.
60 Smart ﬁbres, fabrics and clothing
Table 4.1 Thermal conductivity of pads of ﬁbres with a packing density of
Fibre (mW/m K)
Cellulose acetate 230
Air (still) 25
Source: Physical Properties of Textile Fibres, Morton W E and Hearle J W S, Third
edition, Textile Inst., Manchester, UK, 1993, p. 590.
In this chapter, a brief account of polymers, ceramics, phase change
materials as melt additives, breathable coatings and design of fabric assembly
for thermal insulation is given.
4.2 Thermal storage and thermal insulating ﬁbres
4.2.1 Use of ceramics as melt dope additives
Zirconium, magnesium oxide or iron oxide can be used as particulate ﬁllers in
the molten polymer for producing heat generating polyester, polyamide,
polyethylene, polypropylene and other functional ﬁbres.
By applying the heat insulation principle, heat-regenerating ﬁbres produced
from ceramic composites utilize the far infra-red radiation eﬀect of ceramics,
which heat the substrate homogeneously by activating molecular motion. For
example, zirconium, magnesium or iron oxide, when blended into manufactured
ﬁbres, radiate ca. 60 mW far infra-red of wavelengths 8—14 m at a body
temperature of 36 °C. Such ﬁbres have been found suitable for sportswear and
winter goods, particularly for those working in extremely cold regions.
There are two possible ways to insulate heat:
1 By using a passive insulating material which encloses the body heat
2 By use of an active material as an additive or coating that absorbs heat
The far infra-red radiation ceramics activated by body heat belong to the
ﬁrst category of insulating materials.
Thermally sensitive materials 61
Light Heat (infra-red)
Ultra-violet Visible Infra-red Far infra-red
4.1 Heat absorption and insulation of Solar- (Descente).
The active insulating materials which fall in the second category are those
electrically heated materials where the electrical energy of a battery is
transformed into heat energy by the heater, with this heat supplied by the heat
from the oxidation of iron powder. In another system, the conductive
particulate is selected from SnO , BaSO , K titanate and TiO , and the far-IR
particulate from one or more of ZrO , Al O , TiO , Kaolin and MgO for
producing thermal storage and thermal insulating ﬁbres.
Zirconium carbide compounds have been used for their excellent character-
istics in absorbing and storing heat in a new type of solar system, including
domestic water heaters and large-scale generators. Zirconium carbide reﬂects
the light of long wavelengths over 2 m, but absorbs the light energy of rather
short wavelengths ( : 2 m), which make up 95% of sunlight, and converts it
into stored heat energy. Descente researchers used this property of zirconium
carbide to achieve ‘active insulation’, by enclosing microparticles of zirconium
carbide in polyamide or polyester ﬁbres. They developed the technology to
encapsulate zirconium carbide powder within the core of synthetic ﬁbres, in
cooperation with Unitika. The clothes made of this ﬁbre, Solar- (Fig. 4.1)
absorb solar visible radiations eﬃciently and convert them into heat in the
form of infra-red radiation which is released in the clothing. The released heat
and the heat radiated from the body are reﬂected by Solar- and will not
escape from the inside to the outside of clothing.
62 Smart ﬁbres, fabrics and clothing
Unitika has also disclosed the manufacture of self-stretchable heat-retentive
polyester yarns containing Group IV transition metal carbides. Thus, a blend
of 95 parts PET and ﬁve parts Zr carbide was melt-spun at 3100 m/min and
heat-treated at non contacting-type heater temperature 425 °C to give
self-stretchable yarn (B) exhibiting stretch at 185 °C of 4.5% and conventionally
spun PET ﬁbres drawn at non contacting heater temperature of 285 °C to
give yarn (A) having dry heat shrinkage of 4.5%. Interlacing yarns A and B
and subsequent twisting produced woven fabric which exhibited surface
temperature 21.1 °C initially, 24.5 °C on exposure of fabric to a source of 100 W
for 10 min, and 23.2 °C on storing the fabric for 5 min after exposure to light
for 10 min.
Mitsubishi Rayon Co. has reported the development of heat-storage and
electrically conductive acrylic ﬁbres with electrical conductivity 9 10 S/cm
and clothes for winter clothing and sportswear. These bicomponent ﬁbres
comprise a core—sheath structure, a core of P(AN/MA/Sod. methallyl
sulphonate) containing 15—70 vol % white electrical conductive ceramic
particles (e.g. W-P) and P (acrylonitrile/vinyl acetate) as a sheath.
Toyo Kogyo Co. disclosed the production of insulative antistatic polyester
ﬁbres. A blend of PET and 20% pellets comprising 4 : 1 (wt. ratio) mixture of
ceramic powder containing 70 parts Sb O and 30 parts SnO (particle size
: 1 m) and one part adipic acid-butylene glycol polymer was melt-spun and
drawn. A unit of this ﬁbre showed surface temperature of 53.5 °C after
exposure to light (300 W) for 60 s and surface resistivity 3.0 ; 10 vs. 46.5 °C
and 5.2 ; 10 , respectively for ﬁbres containing no ceramic powder.
Kuraray claimed the formation of PET ﬁbres with heat-storing/heat
insulating properties. Such ﬁbres contain heat-storing agents obtained by
impregnating porous materials with organic compounds having melting point
10—50 °C, heat of melting P 20 mJ/mg and crystallization temperature
10—45 °C. Thus, a composition containing PET and decanoic acid-impregnated
SiO support was spun to give ﬁbres with heat evolution of 40 mJ/mg.
Insulative ﬁbres with improved heat retention properties have been made
by Unitika. A melt-kneaded mixture of calcium laurate treated six parts
-alumina (A 50N) with average particle size of 1.0 m; four parts of Zr carbide
were blended with 90 parts of PET as the core, and PET as the sheath were
together melt-spun to give ﬁbres showing a surface temperature of 26.9 °C on
exposure to a white light source (100 W) at 20 °C and 65% relative humidity
and heat conductivity 29 W/cm °C.
In another patent, production of thermally insulative fabrics from ﬁbres
comprising 98 parts nylon 6 and two parts Na stearate-treated -type Al O
(AKP-30) particles with average particle diameter 0.4 m has been disclosed.
The mixture was melt spun at 250 °C, drawn, heat-treated at 165 °C, and made
into a woven fabric with heat conductivity 2.4 ; 10 W/cm °C.
Heat-ray-radiating ﬁbres with high warming and heat insulating properties
Thermally sensitive materials 63
have been produced. The ﬁbres, useful for clothes, bed clothes, etc., contain
n-type semiconductors showing volume resistivity 30—500 cm. Thus, a
non-woven fabric was manufactured from multiﬁlament yarns comprising
PET and 3% Al-doped electrical conductive ZnO powder.
Thermally insulative undergarments from blends of metal containing
spandex and other ﬁbres have been produced. A blend containing 15%
spandex ﬁbres having alumina, silica, titania and Pt at 10: 82: 3: 5 wt. ratio,
and 85% cotton showed heat conductivity 4.906 ; 10 W/cm °C and heat
retention 28.6%. A ladies’ stocking of a blend comprising 6.4% spandex
ﬁbres containing alumina, silica, titania and Pt at 10: 82: 3: 5 wt. ratio, 24.1%
acrylic ﬁbres and 13.5% nylon ﬁbres also showed heat conductivity
3.525 ; 10 W/cm °C and heat retention 42.3%.
Kuraray has also produced heat storing ﬁbres which contain 0.5—40%
mixtures of Group VIII transition metal oxide and TiO at 1/(0.3—2.0 ratio).
Thus, Septon KL 2002 (hydrogenated isoprene—styrene triblock rubber)
containing 15% powder Fe O and 15% powder TiO as the core and PET as
the sheath were spun at core/sheath : 1/3, stretched, and heat-set to give
multiﬁlaments (75 denier/24 ﬁlaments), which were plain-woven, scoured,
dyed in black and irradiated with a reﬂector lamp for 40 s at inside
temperature 20 °C (inside temperature is the temperature of air between the
specimen and a heat insulator in a test apparatus). The fabric showed surface
temperature of 54.8 °C and inside temperature 33.0 °C immediately after the
irradiation, and 22.0 °C and 25.3 °C, respectively, 5 min after the irradiation.
Shimizu has demonstrated the use of substances containing high amounts
of H O of crystallization, e.g. powdered borax, Al(OH) , Zn borate, Ca(OH)
or powdered alum as ﬁllers for producing self-extinguishing far-IR radiating
heat insulative ﬁbres. A blend comprising 100 parts master batch containing
PET and 30% Al(OH) and 500 parts PET was pelletized and spun to give
self-extinguishing ﬁbres containing 5% Al(OH) .
4.2.2 Hollow ﬁbres
Use of hollow ﬁbres in place of cylindrical ﬁbres aﬀects the physical properties
of the product. A reduced heat transfer is of special interest under the changed
physical properties for ﬁbre-ﬁlled products such as pillows, mattresses,
sleeping bags, etc. In such products, synthetic hollow ﬁbres have been given
preference for many years.
Kawabata also used an empirical approach to show that the thermal
conductivity of single ﬁbres along their axis is about ten times as great as heat
conductivity in a direction transverse to the ﬁbre axis. This thermal anisotropy
and its implications on the eﬀects of ﬁbre orientation within the web become
especially interesting when considering the hollow ﬁbres now often used in
64 Smart ﬁbres, fabrics and clothing
Lightweight hollow ﬁbre thermally insulating fabrics for winter clothing
have been produced by Unitika. A composition containing 98 parts nylon 6
and two parts sodium stearate treated- -Al O particles (AKP-30) was
melt-spun to form ﬁbres with degree of hollowness 30%, drawn and made into
woven fabric exhibiting heat transmission 1.6 ; 10 W/cm °C.
Nylon ﬁbres having a hollow, square-shaped cross-section (A) with two
perpendicular protrusions (B) at each end for insulative garments are
produced as follows: A composition containing 96 parts nylon 6 and four parts
zirconium carbide as the (A) section-forming component and nylon 6 only as
the (B) portion-forming component were melt-spun together at 275 °C to give
hollow non-circular ﬁbres with heat retention temperature by a speciﬁed test
as 26.1 °C.
Hollow insulative lightweight polyester ﬁbres have also been produced by
Toray Industries. The ﬁbres have a circular cross-section with a triangular
hollow portion having a speciﬁed dimension. A polyester was melt-spun
through a spinneret with each hole comprising three arc-shaped slits, cooled
by blowing air onto the ﬁbres, lubricated, and drawn to give ﬁbres with degree
of hollowness 20.2% and lustre 98.5%.
Hollow hygroscopic insulative PET ﬁbres with good pilling resistance
have been produced. A composition comprising 100 parts ethylene glycol-sodium
5-sulfoisophthalate-terephthalic acid copolymer (I) and three parts polyethylene
glycol as the core, and PET as the sheath were together melt-spun at 50 : 50
ratio, made into a woven fabric and subsequently treated with an alkali
solution to dissolve I and give a lightweight insulative fabric with water
absorption 146 mm and good pilling resistance.
Heat-insulative hollow PET ﬁbres with pores extending from the surface of
the ﬁbres to the hollow portion of the ﬁbres and with the hollow portion
containing slowly releasable hygroscopic polymer gels have been disclosed by
Teijin. The ﬁbres are useful for undergarments and gloves. Poly(ethylene
terephthalate) was melt-spun through a spinneret and drawn to form hollow
ﬁbres with degree of hollowness 40%. They were made into a tricot, then
treated with NaOH solution to cause weight loss of 20% to give ﬁbres having
P 1 pore with width 0.2—2.0 m and length 10—15 m per 100 m. In another
system, the knit was immersed in an aqueous solution containing Na acrylate
20, acrylic acid 5, and polyethylene glycol dimethacrylate 10 parts in a
container for 10 min at 0.2 torr, subsequently immersed in H O for 3 min at
100 °C, dried and heat-treated for 1 min at 120 °C to give a knit with weight
increase 23.5% and exhibiting moisture absorption 15.0% and average body
temperature retention rating (5 best, 1 worst) 4.5 by a speciﬁed test.
Porous insulative polypropylene ﬁbres have been produced by melt-spinning
of polypropylene (I) with melt index (MI) 0.8, heat-treated at 150 °C for 24 h,
and drawn to give ﬁbres with porosity 80% and average pore diameter 2.2 m.
Thermally sensitive materials 65
Thermally insulating hollow side-by-side bicomponent polyester ﬁbres
have been produced. PET with [ ] 0.64 and PET with [ ] 0.58 were together
melt-spun through a ring-shaped spinneret at 1: 1 throughput ratio, drawn,
crimped, heat-treated at 120 °C in the relaxed state, and cut to give hollow
ﬁbres with the degree of hollowness 5—30% and latent crimp 18/25 mm on
heat-treating the ﬁbres at 180 °C.
The author has also documented the developments in acrylic ﬁbres,
wherein hollow acrylic ﬁbres ﬁnd their use in making insulative garments and
in preparation of hollow ﬁbre membranes for water treatment in food,
pharmaceutical and electronic industries and in nuclear power plants. These
ﬁbres are also useful as precursors to carbon ﬁbres, because they may dissipate
heat more eﬀectively than the conventional acrylic precursors.
Hollow acrylic ﬁbres can be produced by a wet or dry spinning method or as
bicomponents having sheath/core structure wherein the core is disposed or
dissolved to get the hollow structure in the form of an internal linear
continuous channel. Toray Industries has disclosed a process to manufacture
hollow acrylic ﬁbres by spinning a liquid containing acrylonitrile—methacrylic
acid copolymer as a sheath and polyvinyl alcohol as a core. The resultant
hollow acrylic ﬁbre was used to produce hollow carbon ﬁbres for use in
4.2.3 Insulating structures with phase change materials
Phase change materials (PCM) absorb energy during the heating process as
phase change takes place, otherwise this energy can be transferred to the
environment in the phase change range during a reverse cooling process.
The insulation eﬀect reached by the PCM is dependent on temperature and
time. PCMs as such are not new; they exist in various forms in nature. The
most common example of a PCM is that of water at 0 °C, which crystallizes
as it changes from a liquid to a solid (ice). A phase change also occurs when
water is heated to a temperature of 100 °C, at which point it becomes steam.
More than 500 diﬀerent phase change materials have been documented by
However, use of the special thermophysical properties of PCMs to improve
the thermal insulation of textile materials only became possible by entrapping
them in microcapsules, each with a diameter of 1 m to 6 m.
Pause has developed heat and cold insulating membranes for using on a
roof structure. For this purpose, PCMs with a crystallization temperature
between 9 25 °C and 20 °C (Table 4.2) were selected to minimize the heat
emission into the outside environment. Further, to reduce heat absorption
from the outside environment, PCMs with melting points of 25 °C to 40 °C
66 Smart ﬁbres, fabrics and clothing
Table 4.2 Characteristics of phase change materials (PCM).
Temperature range from − 25 °C to 20 °C
PCM Crystallization point (°C)
Dodecane − 15.5
Tridecane − 8.8
Tetradecane − 0.2
Hexadecane − 12.2
Heptadecane − 16.5
PCMs for temperature range 25 °C to 40 °C
Melting point (°C)
Source: Ref. 28.
Vigo and Frost pioneered the use of phase change materials for
developing temperature-adaptable fabrics. Polyester, cotton, nylon 66 and
wool fabrics were treated with an aqueous solution of polyethylene glycol
(mol. wt. 600 or 3350) or one of the crystal materials (2,2-dimethyl-1,3-propanediol
or 2-hydroxymethyl-2-methyl-1,3-propanediol). Such fabrics exhibited up to
250% greater thermal storage and release properties than the untreated ones.
The energy storage capacity of hollow polypropylene ﬁbres and viscose rayon
ﬁlled with carbowax during thermal cycling between 230 and 330 K has also
Vigo and Bruno developed NeutraTherm fabrics, the ﬁrst ever ‘phase
change clothing’, by coating the fabric with PEG 1000, a polyethylene glycol
waxy solid. The phase change of the fabrics lasts only about 20 min; after that,
the garments revert to their original insulating properties. The PEG 1000
structure changes from soft to solid in keeping with the temperature,
absorbing heat when it softens, and releasing heat when it solidiﬁes. It is now
reported that the lack of durability of such topical treatments to laundering
and leaching, which remove the water-soluble polyethylene glycols, can be
overcome by insolubilizing low-molecular-weight polyethylene glycols (average
molecular weights 600—1000) on fabrics by their reaction with dimethylol
dihydroxyethylene urea under conventional pad-dry-cure conditions to
produce textiles that are thermally adaptable even after laundering.
Acrylic ﬁbres with increased latent heat retention have been prepared by
treating wet-spun acrylic ﬁbres in the swollen gelled state with substances
having latent heat and having properties for transition from the solid state to
Thermally sensitive materials 67
the liquid state, drying the ﬁbres and heat-treating the ﬁbre. Acrylonitrile-Me
acrylate-sodium-2-(acrylamido)-2-methylpropanesulfonate copolymer was
wet-spun, treated with an aqueous solution containing 50 g/l polyethylene
glycol (I) to get a weight add-on of 6.2% dried, and heat-treated at 125 °C to
give ﬁbres with heat retention 33% as per the JIS L-1096 test.
Gateway Technologies has reported the application of heneicosane,
eicosane, nonadecane, octadecane, and heptadecane as phase change materials
for insulative fabrics. This material can be 425% as warm as a high bulk
wadding. Schoeller Textil AG Switzerland has also explored the application
of micro-encapsulated phase change materials like waxes, which oﬀer
‘interactive’ insulation for skiwear, snowboarding and ski boats. They store
surplus heat and the wax liqueﬁes; when temperatures drop, the microcapsules
release the stored heat.
There are some hydrogels than can modulate the swelling ratio in response
to environmental stimuli such as temperature, pH, chemical, photo-irradiation,
electric ﬁeld, etc. The collapse of a gel in response to environmental changes
predicted by Dusek and Patterson, was also investigated extensively by
Tanaka et al. Thermosensitive hydrogel collapses at elevated temperature
through the lower critical solution temperature (LCST). The volume change
occurs within a quite narrow temperature range. The permeability of water
through the gel can be changed by an ‘on—oﬀ’ switch according to the
environmental temperature. Therefore, such materials can be used as coatings
for temperature adaptable fabrics, drug delivery systems and enzyme activity
Lee and Hsu reported the swelling behaviour of thermosensitive hydrogel
based on N-isopropyl acrylamide—trimethyl methacryloyloxy ethyl ammonium
iodide (TMMAI) copolymers, a nearly continuous volume transition and
associated phase transition from low temperature, and a highly swollen gel
network to high temperature, a collapsed phase near its critical point between
31 and 35 °C. The gel with little TMMAI content (Table 4.3) showed a good
reversibility and, the higher the TMMAI content (2—6%) in the copolymer, the
higher the gel transition temperature.
CH2 C CH3
O C O (CH 2 )2 N CH3 I
Zhang and Peppas have also studied the interpenetrating polymeric
network (IPN) composed of the temperature-sensitive poly(N-isopropyl
68 Smart ﬁbres, fabrics and clothing
Table 4.3 Characterization of NIPAAm/TMMAI copolymer gels
Feed composition (%) Cloud point ratio
point temp. (g H2O/g
Sample NIPAAm TMMAI effecta (°C) dry gel)
TMM0 100 0 st 30–35 14.1
TMM1 99 1 st 30–35 19.3
TMM2 98 2 st 40–50 24.1
TMM3 97 3 vw 40–50 31.9
TMM5 95 5 vw 50–60 44.5
TMM6 94 6 vw 50–60 53.2
ast, strong; vw, very weak.
Source: Ref. 36.
acrylamide) (PNIPAAm) and the pH-sensitive polymethacrylic acid (PMAA).
The results showed that these hydrogels exhibited a combined pH and
temperature sensitivity at a temperature range of 31—32 °C, a pH value of
around 5.5, the pk of PMAA. The LCSTs of the polymers were signiﬁcantly
inﬂuenced by the polymer concentration. The addition of saccharides into
aqueous polymer solutions decreased the LCST of all polymers. As the
polymer concentration increased, the saccharide eﬀects became more
pronounced. A monosaccharide, glucose, was more eﬀective than a disaccharide,
maltose, in lowering the LCST, especially in Pluronic solutions.
The phase transitions of N-isopropylacrylamide and the light-sensitive
chromophore-like trisodium salt of copper chlorophyllin copolymers induced
by visible light has also been reported by Suzuki and Tanaka. The transition
mechanism in such gels is due only to the direct heating of the network
polymers by light. As this process is extremely fast, such systems might be used
as photo-responsive artiﬁcial muscles, switches and memory devices. All these
phase change materials have great potential as coating materials in making
skiwear, clothing for cold regions and high altitudes, etc.
4.3 Thermal insulation through polymeric coatings
Heat transfer can take place by means of conduction, convection or radiation
across a barrier from the hot side to the cooler side. In conduction, heat passes
from a hotter to a colder region along the static material. Convection is the
transfer of heat by a ﬂow of gases or liquids of diﬀerent temperatures. In
radiation, thermal energy is transmitted as electromagnetic waves.
PVC and PU are some of the widely used thermal insulators. They are
invariably used in their foamed, expanded forms. The reason for this is the
contribution of entrapped air or other gases to the total thermal insulation.
Thermally sensitive materials 69
Table 4.4 Thermal conductivity of different substances
Materials (mWm−1K−1 at 20 °C)
Aluminium 200 000
PVC tiles 700
Clothing fabrics 40
Air (still) 25
Source: Ref. 40.
The total heat conduction of a polymeric material is the sum of components
, , and , where G : gas in the cell, R : radiation across the cell of the
% 0 1 !
foam, S : conduction through the wall and C : convection of the gas.
The highest resistance to heat ﬂow comes from the air entrapped in the cell.
Still air has one of the lowest thermal insulations, 25 mW/m K (Table 4.4).
Therefore, polymeric materials in the form of foam have more entrapped air
and show improved thermal insulation, the factor, which depends on the
type of polymer itself and contributes approximately 30% of the total
resistance to heat ﬂow. Therefore, the type of polymer used in thermal
insulators is the next major factor to be considered while designing a thermal
insulator. The other two contributions, i.e. due to the radiation across the
cell of the foam and due to the convection of the gas, is kept to optimum
levels by proper design of the cell structure of the foam coating.
Requirements for extreme cold weather are:
∑ breathable membranes and coatings
∑ down and feather mixtures
∑ high-loft batting of special ﬁbres
∑ reﬂective materials
4.3.1 Why breathable fabrics?—
To avoid the condensation of perspiration in a garment, breathable fabrics
are required. The garment can also become damp in rain or snowfall or
in sportswear. The moisture diﬀuses through the clothing and can reach
the human skin. As the moisture evaporates, the wearer feels cold and
70 Smart ﬁbres, fabrics and clothing
Table 4.5 Water vapour permeability data of polymeric coatings/ﬁlms
Cup method 20 °C, 95% RH
Film (g/m2 24 h)
Normal compact PUR 286
Microporous ﬂuorocarbon 2140
Hydrophilic polyester 1290
Coated microporous PUR 1500–2000
Coated hydrophilic PUR 1000–1700
Grabotter ﬁlm directly coated to the textile 1700–2000
Source: Gottwald L, ‘Water vapor permeable PUR membranes for weatherproof
laminates’, J. Coated Fabrics, Jan 1996 25, 168–175.
A breathable fabric is waterproof and breathable because of the enormous
diﬀerence between the size of a water droplet and a water vapour molecule.
The former is 100 m, in diameter whereas the latter is 0.0004 m, i.e. there is a
factor of around 250 000 between the two sizes.
Waterproof/moisture permeable fabrics from several synthetic ﬁbres have
been designed for skiwear, track suits, rainwear, and mountaineering clothing.
The application of a one-piece overall made from a woven nylon fabric (30-den
ﬂat nylon warp yarns; weft of 900-den air jet textured yarns) in the 1986
dogsled race in Alaska has been described. A nylon glove with a Gore-Tex
liner was also designed for this purpose (Table 4.5).
Breathable fabrics can be classiﬁed into three main categories:
∑ coated fabrics
∑ high-density woven fabrics.
4.3.2 Waterproof breathable coatings
The microporous barrier layer ‘breathes’ primarily through a permanent air
permeable pore structure. Diverse techniques have been used to manufacture
microporous coatings and ﬁlms. The most important methods are listed below.
22.214.171.124 Mechanical ﬁbrillation
For certain polymers, biaxial stretching produces microscopic tears through-
out the membrane, which imparts a suitable microporous structure. For
example, PTFE membranes are used in the Gore-Tex (two-layer and three-layer
laminates). The thin microporous membrane is made from a solid PTFE sheet
by a novel drawing and annealing process. In drawn form, the tensile strength
is increased threefold. The manufacturers claim that these PTFE membranes
Thermally sensitive materials 71
contain approximately nine billion pores per square inch, with a pore volume
of up to 80% and a maximum pore size of 0.2 m.
126.96.36.199 Solvent exchange
In this process, a polymer dissolved in a water miscible solvent is coated thinly
onto the fabric. The porous structure is developed by passing through a
coagulation bath where water displaces the solvent. For example, the textile
substrate is coated with polyurethane solution, where DMF is used exclusively
as the solvent, and the fabric is passed through a coagulation bath containing
water, where water displaces the solvent to give a porous structure.
188.8.131.52 Phase separation
The coating polymer is applied from a mixture of a relatively volatile solvent
with a proportion of higher boiling non-solvent. Precipitation of the polymer
as a microporous layer occurs as the true solvent evaporates faster during the
subsequent drying process. For example, the polyurethane-based Ucecoat
2000 system operates on this principle. Here, a lower boiling solvent (methyl
ethyl ketone) evaporates preferentialy as the fabric passes through the oven,
thereby increasing the concentration of the non-solvent in the coating. When
the concentration of the non-solvent reaches a critical level, the polyurethane
precipitates out in a highly porous form and the remainder of the solvent and
the non-solvent evaporate from the coating as the fabric passes through the oven.
The fabrics useful for apparel for keeping the body warm in cold weather or
for sporting have porous polyurethane-based ﬁlms. Nylon fabric penetrated
with Asahiguard 710 was coated with polyurethane, hardener, DMF and
hydrophobic silica (0.016 m size) and washed with water. It was then printed
with polyurethane and sodium stearate-treated -alumina, dried at 100 °C for
2 min, and later impregnated with F-type water repellent, dried and set at
170 °C for 30 s. This treated fabric showed moisture permeability 7630 g m
24 h and thermal conductivity 4.1 W cm °C ; 10.
184.108.40.206 Solvent extraction
Finely divided water soluble salts or other compounds can be formulated into
the polymer and subsequently extracted from the dried ﬁlm or coating with
water to get a microporous structure.
220.127.116.11 Electron bombardment
A process has been developed for rendering the solid coated fabrics microporous
by bombarding the polymer coating with electron beams. The technique
72 Smart ﬁbres, fabrics and clothing
Table 4.6 Water vapour resistance of clothing fabrics for comparison
Water vapour resistance
Fabrics (mm still air)
PVC coated 1000–2000
Waxed cotton 1000 +
Typical non-wovens 1–3
Woven microﬁbre (nylon or polyester) 3–5
Closely woven cotton 2–4
Ventile L28 3–5
Two-layer PTFE laminates 2–3
Three-layer laminates (PTFE, PE) 3–6
Microporous PU (various types) 3–14
Open pores 3–5
Sealed pore 6–14
Hydrophilic PU coated 4–16
Witcoﬂex staycool in nylon, polyester 9–16
On cotton, poly/cotton 5–10
Source: Handbook of technical textiles, Ed Horrocks A R and Anand S C,
Woodhead Publishing, UK, 2000, 304.
involves feeding the coated fabric between two electrodes, generating high
voltage electrons which can be focused into discreet beams which drill through
the coating without damaging the fabric beneath.
18.104.22.168 UV-EB curing
The sunbeam process is used to manufacture microporous ﬁlms and coatings
in-situ by cross-linking suitable monomers with electron beam or UV light.
Radiation curing has the following advantages over the conventional methods:
∑ low energy consumption
∑ low environmental pollution
∑ fast curing and thus fast processing
∑ short start-up times.
22.214.171.124 Crushed foam coating
Mechanically foamed and thickened lattices are coated onto fabric and dried.
Large surface pores are formed, which are compacted by calendering through
a pressure nip which yields a microporous fabric. The water-vapour permeability
values of various polymeric coatings are given in Table 4.6.
Woods has studied the relation between clothing thickness and cooling
Thermally sensitive materials 73
Table 4.7 Some commercially available insulation materials
Products Manufacturer Characteristics End use
Drylete® Hind Combines Hydroﬁl nylon Skiwear, running and
and hydrophobic polyester cycling apparel
to push moisture away
from the body and then
pull it through fabric for
Gore-Tex® W. L. Gore The original Outerwear, hat,
waterproof/breathable gloves, footwear,
laminated fabric with pores running and cycling
large enough for water to apparel
escape, small enough to
Hydroﬁl® Allied A new super-absorbent Linings, long
hydrophilic nylon that underwear, cycling
sucks moisture away from apparel
Silmond® Teijin A durable water repellent Outerwear
and windproof fabric made
from polyester microﬁbres
Synera® Amoco A strong, lightweight Long underwear,
polypropylene fabric that jacket lining
transports moisture away
from the skin
Supplex® DuPont Extremely soft, quick Outerwear, skiwear,
Tactel drying nylon in smooth or running and cycling
textured version apparel apparel
Thermolite® DuPont An insulation made of Skiwear, climbing
polyester ﬁbres that have apparel
Thermoloft® DuPont A semithick insulation that Skiwear, outdoor
contains hollow polyester apparel
ﬁbres that trap warm air
Thinsulate® 3M Thin insulation made of Skiwear, gloves,
polyester and footwear
Thintech® 3M A waterproof/breathable Skiwear, outerwear
laminated fabric that is
highly resistant to
detergents or perspiration
Source: Ref. 40.
74 Smart ﬁbres, fabrics and clothing
during motor-cycling in the range from 9 1 to 24 °C. To maintain a normal
body temperature in winter on a motor-cycle without a protective shield,
much thicker clothing (mean clothing thickness of 20 mm) inside windproof
oversuit is needed at 5 °C, but it is only eﬀective if perspiration does not
accumulate inside the clothing.
4.3.3 Waterproof breathable membranes
Microporous ﬁlm fully impregnated with a hydrophilic polymer, Thintech, is
sandwiched between the outer and inner fabrics of a garment, followed by
lamination of Thintech to their Thinsulate Thermal Insulation.
It prevents rain, sleet or snow from penetrating a garment and stops the
build-up of moisture within the garment.
4.3.4 Antistatic and heat energy-absorbing coatings
The coating comprises 5—90% ultraﬁne Sb—Sn oxide particles (from : 0.1 m
Sb O ) and 10—90% binder resin.
Polyester cloth treated with aqueous acrylic emulsion (acrylic melamine
resin) containing 20% of 0.005 m ATO particles and baked to form a cloth
showing the half-life of an electric charge of one sec. The front and back
temperatures are 27 °C and 26 °C, respectively, after irradiating with 300 W
lamp at 20 °C and 60% RH.
Heat-insulating, moisture-permeable, and water-resistant nylon has been
produced by coating it with polyurethane containing 2—4% of inorganic ﬁne
powder (Sb oxide-doped SnO ) and Zr carbide having photoabsorption
thermal conversion capability. The coated nylon fabric showed water
resistance pressure (x) P 7000 g/m 24 h and moisture permeability
(y) P 0.6 kg/cm.
Bonding of IR-ray radiating ceramics has also been attempted for
producing thermal insulative textiles. Insulating fabrics were prepared by
immersing fabrics in emulsions containing IR ray-radiating ceramics and
polymers and adding trivalent metal salts to the emulsion to cause bonding of
the ceramic to the fabrics. Thus, a fabric was immersed in a dispersion
containing synthetic rubber latex (solids 15%) and 10% (on fabric) IR
ray-radiating ceramic, and stirred as 10% Al (SO ) was added dropwise,
Thermally sensitive materials 75
washed and dried to give an odour-absorbing insulating fabric with ceramic
content of 10%.
The thermal insulation capabilities of cold protective clothing materials
may be signiﬁcantly improved by the application of MicroPCM, that is
capsules containing small amounts of PCM (phase change materials). The
PCM have the ability to changing their state within a certain temperature
range, storing energy during the phase change and then releasing it at
crystallization temperature. It is shown that, by applying a coating of 50 g/m
onto a ﬁbrous batting of 180 g/m, the insulation capacity is comparable to a
batting of 360 g/m. Micro PCM may thus be used to increase the insulation
capabilities against the cold, with a resulting material which will be
signiﬁcantly thinner, allowing much larger freedom of movement.
4.4 Designing of fabric assemblies—
In colder environments, layered fabrics rather than a single fabric are used in
most cases (Table 4.7). Under such conditions, the two most important
characteristics of fabrics are water vapour and heat transport. In order to gain
insight into the transient states of such transport across a set of layers of
fabrics, Yasuda et al. developed an MU water vapour transport simulator
(MU—WVT simulator). They reported that water transport was not inﬂuenced
signiﬁcantly by surface characteristics — the hydrophilic or hydrophobic
nature of fabrics. On the other hand, when liquid water contacted a fabric,
such as in the case of sweating, the surface wettability of the fabric played a
dominant role in determining the water vapour transport rate through the
layered fabrics. In such a case, the wicking characteristic, which determines
how quickly and how widely liquid water spreads out laterally on the surface
of/or within the matrix of the fabric, determines the overall water vapour
transport rate through the layered fabrics.
The overall water vapour and heat transport characteristics of a fabric
should depend on other factors such as the water vapour absorbability of the
ﬁbres, the porosity, density and thickness of the fabric, etc. In this study, the
major emphasis was on the inﬂuence of the chemical nature of the ﬁbres that
constitute a woven fabric. Dynamic water vapour and heat transport in the
transient state were investigated for fabrics made of polyester, acrylic, cotton
and wool ﬁbres (Table 4.8). The overall dissipation rate of water vapour
depends on both the vapour transport rate and the vapour absorption by
ﬁbres, which are mutually interrelated. Water vapour transport is governed by
the vapour pressure gradient that develops across a fabric layer (Fig. 4.2).
When a fabric is subjected to given environmental conditions, the actual water
vapour transport rate diﬀers greatly depending on the nature of the ﬁbres, even
76 Smart ﬁbres, fabrics and clothing
Table 4.8 Characteristics of fabrics
Property Polyester Acrylic Cotton Wool
Fabric densitya (cm−1)
Ends 36.4 37.0 38.1 34.9
Picks 22.5 22.1 23.8 24.4
Thicknessa (mm ; 10) 2.7 2.9 3.1 3.2
Weighta (g/m2) 121.7 116.4 125.0 113.9
Porositya (%) 67.5 66.4 74.8 73.4
Air permeabilitya (cm3/cm2/s) 77.8 81.0 28.2 54.9
Advancing contact angle of water 116 b c
Water vapour absorption rate 3.3 6.1 10.1 15.0
(g/g/min ; 104)
aAccording to JIS (Japanese Industrial Standard) L 1096. bWater droplet was
absorbed by the fabric gradually. cWater droplet was absorbed by the fabric
Source: Ref. 49.
Water vapour pressure (mmHg)
0 5 10 15 20 25 30
4.2 Comparison of water vapour build-up curves in chamber 1 in the
sweat (liquid water) case. Source: ref. 49.
when other parameters are nearly identical, such as density, porosity and
Hong et al. have studied in-depth dynamic moisture vapour transfer
through clothing assemblies. Cotton, polyester and a blend in plain woven,
pure ﬁnish fabrics were studied to determine their inﬂuence on dynamic
surface wetness and moisture transfer through textiles. A simulated sweating
skin was used, over which were placed test fabrics incorporating a clothing
hygrometer to continuously measure dynamic surface wetness. Moisture
Thermally sensitive materials 77
vapour concentration and its rate of change at both inner and outer fabric
surfaces were determined. At the inner fabric surface facing the sweating skin,
all the cotton fabric exhibited the slowest build-up of moisture vapour
concentration, followed by cotton/polyester blend. The all-polyester fabric
showed the highest rate of change in moisture vapour concentration. The
newly modiﬁed clothing hygrometer provides a sensitive method for ascertaining
dynamic surface wetness on both fabrics and clothing as worn.
Dynamic moisture vapour transfer through textiles has also been investigated
by Kim. The inﬂuence of semipermeable functional ﬁlms on the surface
vapour pressure and temperature of fabric—ﬁlm—fabric assemblies has been
reported. The ﬁlm added between two fabric layers aﬀects vapour pressure and
temperature changes on both surfaces of the assembly under simulated
body-clothing conditions. The physical characteristics of ﬁlms greatly inﬂuence
the level of transient, comfort-related variables such as changes of inner
surface vapour pressure and temperature. Mixed cotton and polyester layers
of a ﬁlm reveal that the ﬁlm can negatively aﬀect the moisture sorption of the
assembly, not only by blocking the air spaces for moisture diﬀusion but, more
importantly, by ineﬀective heat dissipation from the cotton inner fabric for
continued moisture sorption. Using ﬁlm and fabric assemblies, this study
reinforces the interdependence of moisture sorption and temperature barrier
eﬀects during dynamic moisture transfer through the clothing assemblies. The
percentage increases of moisture uptake of C/P (inner/outer) and P/C
(inner/outer) without any ﬁlm (none) are the same throughout the experiment
(0.7, 1.6, 2.2 and 2.7%). The presence of ﬁlms, however, produces diﬀerent
moisture uptake behaviours in the C/P and P/C (Fig. 4.3).
The thermo-insulating properties of lofty non-woven fabrics, which have
been reported in several papers, depend on the nature of pore size and
distribution in a fabric, which are a function of ﬁbre ﬁneness and material
density. Jirsak et al. compared in a more comprehensive way the
thermo-insulating properties of both perpendicular-laid and conventional
cross-laid nonwoven fabrics. The total thermal resistance R of a textile fabric
as a function of the actual thickness of the material:
: ; [4.2]
where is the thermal conductivity (Wm K) as deﬁned in Eq. (4.2),
is the combined thermal conductivity of solid ﬁbre and air and L is the
thickness of the sample (m). The thickness of the material depends on the
L : L(P) [4.4]
78 Smart ﬁbres, fabrics and clothing
0 2 4 6 8 10 12 14 16 18 20
4.3 Dynamic moisture uptake, as a function of time, measured on
fabric–ﬁlm–fabric assemblies. Source: ref. 51. C/C = cotton/cotton
double-knit assembly, P/P = polyester/polyester assembly.
Thus, materials showing the same value, those with higher compressional
resistance, will exhibit better thermal resistance under the same compression.
The perpendicular-laid fabrics, due to their unique ﬁbre orientation, demonstrate
a higher degree of compressional resistance in the thickness direction than the
Farnworth also presented a theoretical model of the combined conductive
and radiative heat ﬂows through ﬁbrous insulating materials and compared
them with experimental values of the thermal resistances of several synthetic
ﬁbre battings and of a down and feather mixture (Table 4.9). No evidence of
convective heat transfer is found, even in very low-density battings. The
diﬀerences in resistance per unit thickness among the various materials may be
attributed to their diﬀerent absorption constants.
Crews et al. evaluated the use of milkweed ﬂoss as an insulative ﬁll
material and compared its performance to other insulators. Seven identical
jackets were constructed using diﬀerent ﬁll materials matched on a per unit
weight basis. The insulation (clo) values for the jackets were measured using a
standing, heated manikin as an environmental chamber. Thickness (loft),
compression, resiliency and hand were also measured. The results show (Table
4.10) that milkweed ﬂoss blended with down has insulative properties similar
to down. Down is superior to milkweed ﬂoss in loftiness and compressibility,
which inﬂuence product performance, but the properties of milkweed ﬂoss can
be enhanced by blending it with down.
Thermally sensitive materials 79
Table 4.9 Physical and thermal properties of all samples studied at minimal
compression (0.16 kPa)
Fibre Fibre Thermal
Fibre radius Thickness Mass volume resistance
Sample material ( m) (mm) (kg/m2) (%) m2K/W
Polarguard Polyester 11.7 26 0.270 0.76 0.48
Holloﬁl Polyester 13.2 28 0.350 0.94 0.59
Thinsulate Polypropylene 1 to 3 7.7 0.405 5.8 0.25
Thinsulate Polypropylene 1 to 3 5.2 0.175 ~ 3.0 0.16
C150 and polyester 20
Down and 40% and 60% — 42 0.545 ~ 1.3 1.22
Source: Ref. 53.
Table 4.10 Insulative value for ﬁlling material type before and after cleaning
Insulation value IT (clo)
Fill type Before cleaning After cleaning
50% Milkweed ﬂoss/50% down 2.36 2.26
100% Down 2.28 2.25
100% Qualloﬁl 2.26 2.19
100% Milkweed 2.24 2.16
50% Milkweed/50% feathers 2.24 2.06
100% Thinsulate 2.15 2.04
60% Milkweed/40% oleﬁn 2.04 1.97
Source: Ref. 54.
1 Bajaj P and Sengupta A K, ‘Protective clothing’, Textile Progr., 1992, 22(2/3/4), 1—110.
2 Ukponmwan J O, ‘The thermal insulation properties of fabrics’, Textile Progr., 1993,
3 Mathur G N, Hansraj and Kasturia N, ‘Protective clothing for extreme cold region’,
Indian J. Fibre Text. Res., 1997, 22, 292—6.
4 Godman R F, ‘Tolerance limits for military operations in hot and/or cold
environments’, paper presented in 12th Commonwealth Defence conference on
Operational Clothing and Combat Equipment, Ghana, 1978.
5 Jian R, ‘Thermal storage and thermal insulating ﬁbres and their manufacture and
applications’, CN 1,229, 153, 22 Sep 1999, Chem. Abstr., 2000, 133, 31770.
80 Smart ﬁbres, fabrics and clothing
6 Hongu T and Phillips Glen O, New Fibres, 2nd edition, Woodhead Publishing Ltd.,
UK, 1997, 63—5.
7 Unitika Ltd, Japan, ‘Self-stretchable heat-retentive polyester yarns containing gr.
IV transition metal carbides and mixture yarns containing them and wool like
fabrics therefrom: JP 11,21,720,26 Jan 1999, Chem. Abstr., 1999, 130, 140435y.
8 Mitsubishi Rayon Co. Ltd. Japan, ‘Heat-storageable and electrically conductive
ﬁbres and threads and clothes’ JP 2000 96,346, 4 April 2000, Chem. Abstr., 2000, 132,
9 Toyo Kogyo Co. Ltd., Osaka ‘Insulative antistatic ﬁbres and products thereof’, JP
03,193,970,23 Aug. 1991, Chem. Abstr., 1991, 115, 258198s.
10 Kuraray Co. Japan, ‘Heat-storing, heat-insulating ﬁbres with lasting thermal
properties’, JP 08,246,227, 24 Sep 1996, Chem. Abstr., 1996, 125, 331455m.
11 Unitika Ltd., Japan, ‘Insulative fabrics with improved heat retention properties’, JP
08,127,961, 21 May 1996, Chem. Abstr., 1996, 125, 117354j.
12 Unitika Ltd. ‘Thermally insulative fabrics for winter clothing and sportswear’ JP
07,300,741, 14 Nov 1995, Chem. Abstr., 1996, 124, 120007h.
13 Kuraray Co. Ltd. Japan, ‘Heat-ray radiating ﬁbres with high warming and heat
insulating properties’, JP 2000 154,419, 6 2000, Chem. Abstr., 2000, 133, 5794m.
14 Suwanii Kk, ‘Thermally insulative stockings from blends of metal containing
spandex ﬁbres and other ﬁbres’, JP 06,41,801, 15 Feb 1994, Chem. Abstr., 1994, 120,
15 Kuraray Co. ‘Heat-storing ﬁbres and their use in composite ﬁbres’, JP 06,158,419,
07 June 1994, Chem. Abstr., 1994, 121, 159320t.
16 Shimizu S, ‘Self-extinguishing far-IR radiating heat insulative ﬁbres containing
substances having high amount of water of crystallization’, JP 11,350,253, 21 Dec
1999, Chem. Abstr., 2000, 132, 51093j.
17 Beyreuther R, Schauer G and Hofmann H, ‘Melt spinning of hollow ﬁbres’. In
Progress in Textiles: Science Technology Vol. 2 Textile Fibres: Developments and
Innovations, IAFL publications, New Delhi, India, 2000, 299—353.
18 Kawabata S, ‘Measurement of anisotropic thermal conductivity of single ﬁbre’, J.
Textile Machin. Soc., Jpn, 1986, 39(12), 184.
19 Unitika Ltd. Japan, ‘Light weight hollow ﬁbre thermally insulating fabrics for
winter clothings and sportswear’, JP 08,60,486, 5 Mar 1996, Chem. Abstr., 1996, 124,
20 Unitika Ltd. Japan, ‘Thermally insulating heat-retentive hollow noncircular
synthetic conjugate ﬁbres containing zirconium carbide particles and exhibiting
heat retention properties’, JP 11,43,820, 16 Feb 1999, Chem. Abstr., 1999, 130, 183725k.
21 Toray Industries, ‘Hollow insulative lightweight polyester ﬁbres with good lustre’
JP 06,228,815, 16 Aug 1994, Chem. Abstr., 1994, 121, 302951g.
22 Kuraray Co., ‘Hollow hygroscopic insulative synthetic ﬁbres with good pilling
resistance’ JP 05, 279, 911, 26 Oct 1993, Chem. Abstr., 1994, 120, 166703c.
23 Teijin Ltd. Japan, ‘Heat-insulative hollow ﬁbres with hot spring bath eﬀect’, JP
09,111,664, 28 April 1997, Chem. Abstr., 1997, 127, 52176x.
24 Mitsubishi Rayon Co., ‘Porous insulative polypropylene ﬁbres and their manufacture’,
JP 04,300,318, 23 Oct 1992, Chem. Abstr., 1993, 118, 126420k.
25 Toray Industries Inc. Japan, ‘Thermally insulating hollow side-by-side bicomponent
polyester ﬁbres and their manufacture’, JP 09,250,028, 22 Sept. 1997, Chem. Abstr.,
Thermally sensitive materials 81
1997, 127, 249330z.
26 Bajaj P, ‘New developments in production of acrylic ﬁbres’. In Progress in Textiles:
Science Technology Vol. 2 Textile Fibres: Developments and Innovations, IAFL
publications, New Delhi, India, 2000, 534—614.
27 Hale D V, Hoover M J and O’Neil M J, Phase Change Materials Handbook,
Contract NAS 8-25183. Alabama: Marshall Space Flight Center (September 1971).
28 Pause B, ‘Development of heat and cold insulating membrane structures with phase
change material’, J. Coated Fabrics, July 1995, 25, 59—68.
29 Vigo T L and Frost C M, ‘Temperature adaptable fabrics’, Textile Res. J., 1985, 55,
30 Vigo T L and Bruno J S, ‘Temperature adaptable textiles’, Textile Res. J., 1987, 57,
427—9, September 1989, 34.
31 Kanebo Ltd., ‘Acrylic ﬁbres with increased latent heat retention and their
manufacture’, JP 06,220,721, 09 Aug 1994, Chem. Abstr., 1994, 121, 302948m.
32 Gateway Technologies Inc., High Performance Textiles, Aug 1995, 5—6.
33 Rupp J, ‘Interactive textiles regulate body temperature’, Intern. Textile Bull., 1999
34 Dusek K and Patterson D, ‘Transition in swollen polymer networks induced by
intramolecular condensation, J. Polym. Sci., Part A-2, 1968, 6, 1209.
35 Tanaka T, Nishio T, Sun S and Nishio S U, ‘Collapse of gels in an electric ﬁeld’,
Science, 1982, 218, 467.
36 Lee W F and Hsu C H, ‘Thermoreversible hydrogel V: synthesis and swelling
behaviour of the N-isopropylacrylamide-co-trimethyl methacryloyloxyethyl
ammonium iodide copolymeric hydrogels’, J. Appl. Polym. Sci., 1998, 69,
37 Zhang J and Peppas N A, ‘Synthesis and characterization of pH- and temperature-
sensitive Poly(methacrylic acid)/Poly(N-iso propyl acryl amide) interpenetrating
polymeric networks’, Macromolecules, 2000, 33, 102—7.
38 Kim Y H, Kwan I C, Bae Y H and Kim S W, ‘Saccharide eﬀect on the lower critical
solution temperature of thermo-sensitive polymers’, Macromolecules, 1995, 28(4),
39 Suzuki A and Tanaka T, ‘Phase transition in polymer gels induced by visible light’,
Nature, 26 July 1990, 346, 345—7.
40 Sarkar R K, Gurudatt K and De P, ‘Coated textiles as thermal insulators — Part II’,
Man-made Textiles in India, 2000, XLIII, 279—85.
41 Davies S and Owen P, ‘Staying dry and keeping your cool’, Textile Month, Aug
42 Tanner J C, ‘Breathability, comfort and Gore-Tex laminates’, J. Coated Fabrics,
1979, 8, 312—22.
43 Reischl U and Stransky A, ‘Comparative assessment of Gore-tex and Neoprene
vapor barriers in a ﬁreﬁghter turn-out coat’, Textile Res. J., 1980, 50, 643—7.
44 Pause B, ‘Measuring water vapor permeability of coated fabrics and laminates’, J.
Coated Fabrics, 1996, 25, 311—20.
45 Sumitomo Osaka Semento Kk Japan, ‘Antistatic and heat-energy absorbing
coating, ﬁbres and wearing apparels therewith’, JP 08,325,478, 10 Dec 1996, Chem
Abstr., 1997, 126, 105406k.
46 Unitika Ltd, Japan, ‘Heat insulating, moisture permeable and water resistant
82 Smart ﬁbres, fabrics and clothing
fabrics having polyurethane coatings’, JP 08,246,339, 24 Sept 1996, Chem. Abstr.,
1997, 126, 9259u.
47 Yamane, Sachiko, ‘Bonding IR-ray radiating ceramics to textiles’, JP 03,27,176, 5
Feb 1991, Chem. Abstr., 1991, 114, 187500a.
48 Fan J and Keighley J H, ‘An investigation on the eﬀects of: body motion, clothing
design and environmental conditions on the clothing thermal insulation by using a
fabric manikin’, Intern. J. Clothing Sci. Technol., 1991, 3(5), 6—13.
49 Yasuda T, Miyama M and Yasuda H, ‘Dynamic water vapor and heat transport
through layered fabrics Part II: Eﬀect of chemical nature of ﬁbres’, Textile Res. J.,
1992, 62(4), 227—35.
50 Hong K, Hollies N R S and Spivak S M, ‘Dynamic moisture vapor transfer through
textiles, Part I: Clothing hygrometry and the inﬂuence of ﬁbre type’, Textile Res. J.,
1988, 58, 697—706.
51 Kim J O, ‘Dynamic moisture vapor transfer through textiles, Part III: Eﬀect of ﬁlm
characteristics on microclimate moisture and temperature changes’, Textile Res. J.,
1999, 69(3), 193—202.
52 Jirsak O, Sadikoglu T G, Ozipek B and Pan N, ‘Thermo-insulating properties of
perpendicular-laid versus cross-laid lofty nonwoven fabrics’, Textile Res. J., 2000,
53 Farnworth B, ‘Mechanisms of heat ﬂow through clothing insulation’, Textile Res.
J., 1983, 53, 717—24.
54 Crews P C, Sievert S A, Woeppel L T and McCullough E A, ‘Evaluation of
Milkweed Floss as an insulative ﬁll material’, Textile Res. J., 1991, 61, 203—10.
55 Hansraj, Nishkam A, Subbulakshmi M S, Batra B S and Kasturia N, Proc.
‘Technical Textiles’, organized by SASMIRA, Mumbai, India, 31 Jan 1998, 24—32.
Cross-linked polyol ﬁbrous substrates
as multifunctional and multi-use
TYRONE L. VIGO AND
DEVRON P. THIBODEAUX
The concept of ‘intelligent’ or ‘smart’ materials was critically reviewed within
the context of ﬁbrous materials having these attributes. It is generally agreed
that the development of such materials occurred ﬁrst with shape memory
metal alloys (in the 1960s), followed by studies on polymeric intelligent gels
(1970s). Also, a few studies were initiated in the late 1970s and early 1980s on
intelligent ﬁbrous materials. This study will brieﬂy review ﬁbrous materials
that possess this special attribute, which is usually deﬁned as a profound
change caused by an external stimulus that may or may not be reversible. Also
examined in detail are our recent investigations on ﬁbrous materials
containing bound polyols that have at least two intelligent attributes: thermal
and dimensional memories. Particular attention is focused on the techniques
for measurement and characterization of load and pressure development in
modiﬁed fabrics wet with polar solvents, and possible applications for these
5.2 Fibrous intelligent materials
Although intelligent ﬁbrous substrates were ﬁrst described and demonstrated
in Japan in 1979 with shape memory silk yarn, it is our opinion that the
discovery of crease recovery in cellulosic fabrics in the wet and dry state by
Marsh and coworkers in 1929 was actually the ﬁrst example of intelligent
materials that even preceded intelligent shape memory alloys. However, this
discovery, which later led to the commercialization of durable press fabrics,
was never identiﬁed or promoted as an intelligent textile concept.
The shape memory silk yarn was modiﬁed by immersion in a hydrolysed
protein solution, followed by subsequent drying, crimping, immersion in water
and heat setting at high pressure in the wet state. On subsequent heating at
60 °C, the yarn becomes bulky and crimped, but it reverts to the untwisted and
84 Smart ﬁbres, fabrics and clothing
uncured state upon drying. Two other important developments that were
patented in the late 1980s can be classiﬁed as intelligent ﬁbrous materials. The
ﬁrst was polyester or polyamide fabrics, which absorbed visible solar radiation
and converted it into heat as infra-red radiation released inside the garment
due to the microencapsulation of zirconium carbide; it was irreversible since it
did not reverse at high temperatures to provide cooling. The second was
thermochromic garments (colour change induced by incorporation of
compounds that respond to changes in environmental temperature) produced
by Toray Industries called SWAY, which have reversible colour changes at
temperature diﬀerences greater than 5 °C and are operable from 9 40 °C to
; 80 °C.
Most of the other recent investigations on intelligent ﬁbrous materials have
been primarily concerned with shape memory eﬀects. Some relevant examples
are polyester fabrics with durable press properties produced by high energy
radiation cross-linking with polycaprolactone and acrylate monomers and
temperature-sensitive polyurethanes prepared by copolymerization of poly-
tetramethylene glycol and methylene diisocyanate, 1,4-butanediol. More
novel intelligent ﬁbre applications and responses to external stimuli were
described in a 1995 American Chemical Society symposium. These polymeric
smart materials included ﬁbre optic sensors with intelligent dyes and enzymes
whose ﬂuorescence changes with changes in glucose, sodium ion and pH, and
elastomeric composites embedded with magnetic particles, which undergo
changes in their moduli when exposed to external magnetic ﬁelds and thus can
be used for vibration or noise reduction in transportation and machinery.
Smart ﬁbrous composite sensors made of carbon and glass have also been
described for prevention of fatal fracture by changes in their insulating and
Fibrous materials containing bound or cross-linked polyols were patented
and initially characterized by multifunctional properties imparted to the
modiﬁed materials by a single process. Major property improvements
include thermal adaptability, high absorbency and exsorbency, enhanced
resistance to static charge, oily soils and ﬂex abrasion, and antimicrobial
activity. The most notable of these property improvements was temperature
adaptability and reversibility due to the phase change material (PCM)
characteristics of the cross-linked polyol bound to the ﬁbres. However, this
unique and new ﬁbre property was not initially deﬁned as an intelligent
material attribute. Moreover, a related invention, the disclosure of ﬁbres with
thermal adaptability due to attachment by microencapsulation of hexadecane
and n-eicosane (PCMs with high latent heat and thermal reversibility), was
also not characterized as an intelligent ﬁbrous material.
Cross-linked polyol ﬁbrous substrates 85
The modiﬁed fabrics containing the bound polyols, derived from using
formulations with diﬀerent molecular weight, acid catalysts and cross-linking
resins as previously described, were woven cotton and 65/35 cotton
polyester printcloth or sheeting (125—135 g/m). The surface temperatures
were measured with a Hughes Probeye Thermal Video System 3000 with an
image processor, infra-red camera head, argon gas cylinder and colour screen
monitor. Untreated and modiﬁed fabrics (6 in or 150 mm) were mounted on
a pin frame surrounded by a wooden enclosure containing a 150 watt light
bulb whose heat output was controlled by a voltage regulator device (Variac)
with the camera sensitivity set at 2.0 and emissivity value set at 0.95, which was
appropriate for fabric surfaces. Surface temperatures (°F) were measured every
10 min and for up to 30 min with the infra-red camera 1 m from the fabric by
positioning the cross-hairs of the camera in the centre of the fabric with the
untreated control value at 147 °F (64 °C).
For the work and power measurements previously described, a 65/35
cotton/polyester cross-tuck knit (177 g/m), woven cotton printcloth (125 g/m),
and 50/50 hydroentangled pulp/polyester non-woven (80 g/m) containing
40—60% bound polyol were evaluated. Each of the fabrics was attached to a
metal alligator clip, suspended vertically. The amount of shrinkage, work (W)
performed, and power (P) generated were determined with weights attached
after wetting with various solvents (water, acetone and ethanol). The amount
of shrinkage was also determined without weights attached for each of the
diﬀerent types of fabrics for each solvent.
For the tension and pressure measurements, a desized, scoured and
bleached 100% cotton interlock knit fabric (205 g/m) was treated with 50%
PEG-1450—11% DMDHEU (Fixapret ECO)—5.1% citric acid—5.1%
MgCl .6H O to a wet pickup of 110%, then cured for 3 min at 110 °C, washed
in warm water to a pH of 8.5 to neutralize acid catalyst, excess water removed,
then oven-dried for 7 min at 85 °C. The resultant fabric had a wt. gain of 65%
and had shrinkage in one direction (longitudinal) when wet with various polar
solvents (28% with water; 25% with 1% aq. NaCl; 10% with 95% ethanol; and
7% with acetone). Three inches of a 1 ; 6 inch strip of the treated fabric was
clamped between the jaws of an Instron (Model 4201) having a 10 lb load cell,
completely wet with each of the four solvents and tension load/stress measured
after initial wetting to a maximum time of 15 min.
86 Smart ﬁbres, fabrics and clothing
5.4 Results and discussion
5.4.1 Thermal memory
The characterization of ﬁbrous materials containing cross-linked polyols as
smart materials with a thermal memory was ﬁrst discussed by Vigo in an
American Chemical Symposium which he co-organized in 1995 and later
described in more detail in conference proceedings and in refereed journals.
This thermal memory or thermal reversibility is unique and has been
determined and documented by diﬀerential scanning calorimetry and infra-red
thermography. The latter measures changes in surface temperature on
exposure to a heat source. As shown in Fig. 5.1, cotton fabrics containing
bound polyol had substantial reduction in surface temperature relative to an
untreated control fabric (surface temperature 147 °F or 64 °C) after all fabrics
were exposed to a heat source for a minimum of 30 minutes. Even more
impressive is that the lowest amounts of bound polyol in the fabric gave the
greatest decrease in surface temperature. Weight gains were 34% for fabrics
containing bound PEG-1000, 37% for fabrics containing bound PEG-2000,
28% for fabrics containing bound PEG-4000 and only 25% for fabrics
containing bound PEG-6000.
The decrease in surface temperature in all treated fabrics usually occurred
within 30 seconds and was greater with higher molecular weight cross-linked
polyols bound to the fabric, due to the increasing crystallinity of the polyol
with increasing molecular weight. Surface temperature decrease on the
modiﬁed fabrics was 17—28%. Thermal memory and reversibility have been
documented in commercial skiwear marketed in Japan, with the crosslinked
polyol as one of the fabric components; thermocouples in this component
demonstrated that the skiers had optimum thermal comfort by an increase in
fabric surface temperature when idle and lowering of the surface temperature
after skiing, thereby preventing discomfort due to perspiration and body heat.
5.1 Change in surface temperature of untreated and cross-linked
polyol-treated fabrics after 30 min exposure to a heat source.
Cross-linked polyol ﬁbrous substrates 87
Applications for thermally adaptable fabrics containing cross-linked polyols
have been previously described, primarily with regard to apparel and
insulation. However, there are many other applications that could evolve
based on the ‘intelligent’ thermal memory of these modiﬁed ﬁbrous materials.
The wear life of many automotive and aerospace components could be
extended by the moderation of temperature ﬂuctuations during their use.
Camouﬂage uniforms made of this material would be useful for the military
because the wearer would have a diﬀerent surface temperature on garments
normally detected by infra-red sensors. The thermal buﬀering capacity of the
modiﬁed fabrics could be used advantageously in various healthcare applications,
such as in burn therapy and to improve skin temperature and circulation in
patients with maladies such as arthritis and diabetes. Changes in the fabric
surface temperature could also be used to fabricate remote sensing devices for
detection in industrial, residential, horticultural, agricultural and other
environments where temperature change detection would be useful. These
modiﬁed fabrics could be used to minimize plant stress due to temperature
changes and ﬂuctuations as well as protection of livestock and other animals.
Many other ‘thermal memory’ applications for these modiﬁed materials as
sensors and/or actuators are envisioned with the molecular weight of the
bound polyol deﬁning the magnitude and temperature range desired.
5.4.2 Dimensional memory
It was known from our earlier studies that certain types of fabric constructions
containing bound polyol were more prone to wet shrinkage. The magnitude of
this eﬀect with various solvents such as hexane, ethanol, acetone and water,
was investigated with three diﬀerent fabric constructions: knit, woven and
non-woven. An increase in the polarity of the solvent resulted in increasing
reversible wet shrinkage (highest with water, no shrinkage with hexane) that
was most pronounced with knit fabric constructions. To demonstrate the
potential for converting chemical into mechanical energy, diﬀerent quantities
of weights were aﬃxed to modiﬁed knit, woven and non-woven fabrics that
were subsequently wet with water. The work performed (W) and power
generated (P) were determined. As shown in Fig. 5.2, knit fabrics are far
superior to woven and non-woven fabrics in this characteristic, due to its
optimum wet shrinkage in the presence of an applied force. Work performed
by the wet knit fabric was 30—50 times greater than that of the non-woven and
woven fabrics when each had the same amount of weight attached (50 g). It was
even an order of magnitude greater when the knit fabric had twice the weight
attached compared to the other two fabrics. Similar results were obtained for
power generated (P). These results were used to present the concept and design
of an intelligent medical bandage that would contain a removable and
88 Smart ﬁbres, fabrics and clothing
5.2 Work (W) performed by fabrics of different constructions containing
cross-linked polyol by lifting attached weights after wet with water for 30 s.
— + 50 g, - - - + 100 g, . . . + 200 g (from ref. 13).
disposable component of knit cross-linked polyol fabric aﬃxed to a
non-disposable component by metal fasteners or other methods. However,
no pressure or tension measurements were made to determine the amount of
tension or force developed for these types of intelligent fabrics with dimensional
memories activated by wetting with polar solvents.
The tensile load (lb) and stress developed (psi) were measured for untreated
and treated fabric strips after wetting with deionized water (Table 5.1). The
tension developed for the untreated fabric was negligible, but it was very
signiﬁcant for the treated fabric. Multiple measurements were made and there
was some detectable variability (a range of 4.5—5.6 lb and corresponding
values of 130—196 psi). In addition to the development of high tensile stress, the
modiﬁed fabrics wet with water achieved these values rapidly (within 90
seconds of wetting) and maintained them over the measurement period of 5
min (Fig. 5.3). Although there was somewhat more variability for treated
fabrics that were wet with 1% aq. NaCl with regard to load and tensile stress
developed (3.5—6.2 lb and 120—217 psi), these fabrics also developed such
tension rapidly (Fig. 5.4). Thus, tension developed rapidly in treated fabrics
wet with water and aqueous salt solution and was generally proportional in
Cross-linked polyol ﬁbrous substrates 89
Table 5.1 Maximum load and tension developed in fabrics after wetting with
Max. load Max. tension
Fabric Solvent/solution (lb) (psi)
Untreated control H2O — —
Treated H2O 5.6 196
Treated 1% aq. NaCl 6.2 217
All fabrics were clamped between jaws of Instron (1 ; 3 in length) that were wet
within 30 s and tension developed measured from initial wetting up to 5 min.
5.3 Development of tension over time with modiﬁed fabric after wetting
5.4 Development of tension over time in untreated control fabric after
wetting with water.
90 Smart ﬁbres, fabrics and clothing
magnitude to the wet shrinkage that these fabrics experienced when they were
The behaviour of the modiﬁed fabrics when wet with the two organic
solvents shown in Table 5.2 and Fig. 5.5 and 5.6 (95% ethanol and acetone,
respectively) diﬀered from those wet with aqueous media in three fundamental
aspects: (1) maximum tension took longer to achieve with these solvents than
those wet with aqueous media; (2) the tension developed was also less than
those exposed to aqueous media; and (3) the reversal of load and pressure
occurred over relatively short time periods due to the high vapour pressure
and accompanying evaporation of solvent. Fabrics wet with ethanol took
about 450—550 seconds to reach maximum stress (138 psi generated), then
reversed this eﬀect due to slow solvent evaporation (Fig. 5.5). Fabrics wet with
acetone reach maximum tension more rapidly (150 seconds with a corresponding
load of 1.6 lb and 56 psi), but rapidly reversed back to zero load after 250
seconds due to the complete evaporation of the solvent (Fig. 5.6).
Table 5.2 Maximum load and tension developed in fabrics after wetting with
polar organic solventsa
Max. load Max. tension
Fabric Solvent (lb) (psi)
Treated 95% ethanol 3.9 138
Treated Acetone 1.6 56
aAll fabrics were clamped between jaws of Instron (1 ; 3 in length) that were wet
within 30 s and tension developed measured from initial wetting up to 15 min.
5.5 Development of tension over time in modiﬁed fabric after wetting with
Cross-linked polyol ﬁbrous substrates 91
5.6 Development of tension over time in modiﬁed fabric after wetting with
Intelligent fabrics containing cross-linked polyols that have reversible
dimensional memories on exposure to polar solvents can serve in a variety of
applications. A variety of sensors could be developed that detect diﬀerent
types of polar solvents and solutions related to the amount of wet shrinkage
and/or tension developed. Alternatively, fabric sensors could be fabricated to
detect varying amounts of water vapour and liquid water by wet shrinkage
and/or accompanying tension developed on wetting. Several types of actuator
systems based on these modiﬁed fabrics are also envisioned. In the biomedical
and healthcare area, wetting with solvents such as sterilized water, salt
solutions and alcohol could be used to activate medical pressure bandages and
possibly tourniquets; alternatively, blood (plasma) could activate pressure
development and thus stop undesirable bleeding. These fabrics could be used
to produce micromotors and a variety of valves or other mechanical devices
that are activated by the reversible wet shrinkage that occurs with a variety of
Fabrics of woven, non-woven and knit constructions containing cross-linked
polyols have been shown to have thermal memories over a wide temperature
range and can be adapted to various thermal environments by the molecular
weight of the bound polyol and the degree of cross-linking on the ﬁbrous
substrate. In contrast, only speciﬁc fabric constructions (cross-tuck and
interlock knits) containing the cross-linked polyols are able to generate
substantial tensile load when wet with polar solvents. The load and stress
generated are usually proportional to the degree of wet shrinkage when the
fabrics are not constrained. Maximum and rapid tension development occurs
92 Smart ﬁbres, fabrics and clothing
with water and aqueous salt solutions, while ethanol and acetone are
somewhat less eﬀective with faster reversibility due to rapid evaporation of
these low-boiling, high vapour pressure solvents. Numerous applications for
the cross-linked polyol fabrics with thermal and dimensional memories are
envisioned with two major areas of use as sensors and actuators.
1 Vigo T, Intelligent ﬁbrous materials, J. Textile Inst. 1999, 90(3), 1—13.
2 Hongu T and Philips G O, New Fibers, New York, Ellis Horwood, 1990.
3 Vigo T, Textile Processing and Properties: Preparation, Dyeing, Finishing and
Performance, Amsterdam, Elsevier, 1997.
4 Toray Industries, Spiro-oxazine compounds and preparation thereof and photo-
chromic article shaped, US Pat 4 784 474, Nov. 15, 1988.
5 Wantabe I, Fabrics with shape memory, Japan Kokai Tokkyo Koho JP 09,95,866,
April 8, 1997.
6 Lin J R and Chen L W, Study on shape-memory behavior of polyether-based
polyurethanes, Appl. Poly. Sci., 1998, 69, 1563—74.
7 Dagani R, Polymeric ‘smart’ materials respond to changes in their environment,
Chem. Eng. News, 1995, 73(38), 30—3.
8 Muto N, Yanagida H, Nakatsju T, Sugita M, Ohtsuka Y and Arai Y, Design of
intelligent materials with self-diagnosing function to prevent fatal fracture, Smart
Mater. Struct., 1992, 1(4), 324—9.
9 Vigo T L, Frost C M, Bruno, J S and Danna, G F, Temperature adaptable textile
ﬁbers and method of preparing same, US Pat 4 851 291, July 25, 1989.
10 Vigo T L and Bruno J S, Handbook of Fiber Science and Technology, Vol. III, High
Technology Fibers, Part C, New York, Marcel Dekker, 1993.
11 Triangle Research and Development Corp., Bryant Y G and Colvin, D P, Fibre
with reversible enhanced thermal storage properties and fabrics made therefrom,
US Pat 4 756 958, July 12, 1988.
12 Vigo T L, Intelligent ﬁbrous ﬂexible composites containing crosslinked polyethylene
glycols, 4th Int. Conf. Composites Engineering, New Orleans, U. of New Orleans, 1996.
13 Vigo T L, Intelligent ﬁbrous substrates with thermal and dimensional memories,
Poly. Adv. Technol., 1997, 8, 281—8.
14 Private communication, Mitsui Co. and Phenix Co., Tokyo, Japan, 1991.
15 Vigo T L, 6th Int. Conf. Composites Engineering, Las Vegas, 1998.
Stimuli-responsive interpenetrating polymer
network hydrogels composed of
poly(vinyl alcohol) and poly(acrylic acid)
YOUNG MOO LEE AND SO YEON KIM
Recently, there have been many investigations of stimuli-responsive hydrogels,
which are three-dimensional polymer networks exhibiting sensitive swelling
transitions dependent on various stimuli, e.g. electric ﬁeld, pH,—
temperature, ionic strength or other chemicals. They have been
considered to be useful in separation and medical applications, especially in
drug delivery systems.
The schematic diagram illustrating the diﬀusion of bioactive materials
through stimuli-sensitive hydrogels is shown in Fig. 6.1. Among these, pH
and/or temperature-responsive systems have been potential candidates because
these factors could be the most widely available in the environment of the
human body. In an aqueous system, the temperature dependence of the
swelling of a polymer gel is closely related to the temperature dependence of
polymer—water and polymer—polymer interaction. Katono et al. investigated
thermal collapse from interpenetrating polymer networks (IPNs) composed of
poly(acrylamide-co-butyl-methacrylate) and PAAc, and obtained on—oﬀ
release proﬁles as a function of temperature. Poly(N-isopropylacrylamide)
(PNIPAAm) hydrogels demonstrated negative temperature sensitivity with
lower critical solution temperature (LCST) in aqueous solution, which showed
the decrease of swelling with an increase of the temperature above 30—32 °C.
In the case of pH-dependent drug delivery systems, many researchers have
focused on the swelling properties of hydrogels. The acidic or basic components
in the hydrogels led to reversible swelling/deswelling because they changed
from neutral state to ionized state and vice versa in response to the change of
pH. Brannon and Peppas reported a pH-sensitive drug release system
composed of a copolymer of hydroxyethyl methacrylate (HEMA) and
methacrylic acid (MAAc) or maleic anhydride. The poly(NIPAAm-co-vinyl
terminated poly(dimethylsiloxane)-co-AAc) hydrogel synthesized by Hoﬀman
and Dong permitted the release of drugs at pH 7.4 and showed release-oﬀ at
94 Smart ﬁbres, fabrics and clothing
6.1 The diffusion of bioactive materials through stimuli-sensitive IPN
pH 1.4, and was proved to be a suitable carrier for indomethacin through the
gastrointestinal (GI) tract.
In addition, electric current-sensitive hydrogels actuated by electric stimulus
are particularly interesting in connection with the mechanical energy triggered
by an electric signal.— Electric current-sensitive hydrogels are usually
made of polyelectrolytes and an insoluble but swellable polymer network
which carries cations or anions. This system can transform chemical free
energy directly into mechanical work to give isothermal energy conversion. A
typical function of a gel containing ionic groups is to bend reversibly under the
inﬂuence of an electric ﬁeld, making it useful in some actuators driven by an
electric ﬁeld. From the viewpoint of mechanical engineering, great hopes are
set on these materials as new actuators,— especially in the ﬁelds of robotics
and medical welfare instruments.
The present chapter will review the pH/temperature-sensitive properties of
novel PVA/PAAc IPN hydrogels synthesized by a unique sequential method
through UV irradiation and a freezing—thawing process.
Stimuli-responsive interpenetrating polymer network hydrogels 95
Acrylic acid monomer (AAc) obtained from Junsei Chemical Co. was puriﬁed
by inhibitor remove column (Aldrich Chem. Co.) Poly(vinyl alcohol) (PVA;
DP : 2500, degree of deacetylation : 99%) was purchased from Shinetsu Co.
Methylenbisacrylamide (MBAAm) as a cross-linking agent and 2,2-dimethoxy-2-
phenylacetophenone (DMPAP) as a photoinitiator were purchased from
Aldrich Chem. Co. Indomethacin (anhydrous, MW : 357.8), used as a model
drug, was obtained from Sigma Chem. Co. As ﬁve representative solutes,
theophylline (99%, Aldrich Chem. Co.), vitamin B (Sigma Chem. Co.),
riboﬂavin (Junsei Chem. Co.), bovine serum albumin (Young Science Inc.) and
cefazolin sodium were used. Cefazolin sodium was kindly donated by
Chongkeundang RD Center in Seoul, Korea.
6.2.2 Synthesis of PVA/PAAc IPN hydrogels
The PVA/PAAc IPNs were prepared by sequential method. PAAc as an initial
network was synthesized inside a PVA solution using UV irradiation. PVA as
a secondary network was then formed by repetitive freezing—thawing process.
The whole reaction scheme of PVA/PAAc IPNs is described in Fig. 6.2. PVA
was dissolved in deionized water and heated at 80 °C for 2 h to make 10 wt%
aqueous solution. AAc monomers were mixed with 0.2 wt % DMPAP as a
photoinitiator and 0.5 mol% MBAAm as a cross-linking agent. The mixture
was combined with PVA solution to yield PVA—PAAc. The feed composition
and designation of each sample are listed in Table 6.1.
The mixed solutions were poured onto Petri dishes and irradiated using a
450 W UV lamp (Ace Glass Co.) for 1 h under N atmosphere. The irradiated
samples were placed at 9 50 °C for 6 h and at room temperature for 2 h. These
freeze—thawing cycles were repeated eight times.
Table 6.1 Designation and feed contents of PVA/PAAc IPN
Sample PAAc AAc MBAAm DMPAP
name (mol %) (g) (g) (g)
IPN37 70 5.70 0.061 0.0084
IPN46 60 4.89 0.052 0.0098
IPN55 50 3.26 0.035 0.0065
IPN64 40 2.16 0.023 0.0043
IPN73 30 1.62 0.017 0.0032
96 Smart ﬁbres, fabrics and clothing
6.2 The preparation of PVA/PAAc IPN hydrogels by UV irradiation and
Fourier transform-infra-red (FTIR) spectroscopy (Nicolet Model Magna
IR550) and diﬀerential scanning calorimetry (DSC, Du Pont Instruments
DSC 910) were used to conﬁrm the structure of the IPNs. The equilibrium
water content (EWC) was measured in pH 4 and pH 7 buﬀer solution. The
EWC was calculated using the equation in reference. In addition, the
swelling ratio of each sample was evaluated as EWC/100.
6.2.4 Loading and releasing of drug
The indomethacin, as a model drug, was loaded into IPN disks by the solvent
sorption method. The indomethacin release experiment was conducted in
various conditions, changing the pH and/or the temperature of the release
Stimuli-responsive interpenetrating polymer network hydrogels 97
medium, as described elsewhere. The permeation studies were carried out
using a two-chamber diﬀusion cell.
6.3 Results and discussion
6.3.1 Synthesis of PVA/PAAc IPNs
The sequential method by UV irradiation, followed by freezing and thawing,
would be a novel method of preparing the stimuli-sensitive polymer hydrogel.
The structure of the IPN samples prepared was conﬁrmed by FTIR spectra.
6.3.2 Swelling measurement of PVA/PAAc IPNs
The swelling ratios of all PVA/PAAc IPNs were relatively high, and they
showed reasonable sensitivity to both pH and temperature. Temperature-
dependent swelling behaviours at pH 7 are shown in Fig. 6.3(a) and (b).
Measurements were carried out with hydrogels after immersing the samples
for 20 h at 25 °C. The IPN hydrogels showed diﬀerent kinds of thermo-sensitivity.
All IPN samples showed positive temperature-sensitive systems before
reaching their equilibrated state as illustrated in Fig. 6.3(a). After equilibrium
swelling, however, the swelling ratio of IPN46 increased with temperature,
showing a positive temperature-sensitive system, while IPN64 and IPN55
exhibited negative temperature-sensitive systems. The swelling behaviours of
IPN64 and IPN55 are similar to that of virgin PVA homopolymer. This is
ascribable mainly to the swelling tendency of PVA itself, rather than to
polymer—polymer interactions between PVA and PAAc, such as hydrogen
bonding and ionic repulsion in PAAc. The PVA content, even in IPN55
hydrogels, is supposed to be greater than the PAAc content because the
6.3 Temperature/pH-dependent swelling behaviours of PVA–PAAc IPN: (a)
temperature-dependent swelling behaviour before equilibrium (6 h) at
25 °C, (b) temperature-dependent swelling behaviour after equilbrium
(24 h) at 25 °C, (c) pH-dependent swelling behaviours at 25 °C; () IPN 46,
98 Smart ﬁbres, fabrics and clothing
residual acrylic acid monomer, which did not take part in polymerization
during the synthesis of the IPNs, was removed from the IPNs by washing after
the whole procedure. Accordingly, the swelling changes in IPN46 must be
related to the hydrogen bonding between two polymers and the ionic
repulsion of carboxylate ion produced due to the breakage of hydrogen
bondings, while those in IPN64 and IPN55 depend mainly on the swelling
tendencies of PVA composition.
As shown in Fig. 6.3(c), pH-dependent swelling behaviour was observed at
35 °C with changes in pH. The pK value of PAAc is known to be 4.8.
Therefore, at pH 2 and pH 4 buﬀer solutions, carboxyl groups in PAAc
associate and form hydrogen bonding with PVA chains; thus, the swelling
ratios are small. Carboxylate ions formed at pH greater than 4, however,
induce the repulsion between them, and the hydrogen bondings between PVA
and PAAc should decrease, resulting in the increase of free volume in the
matrix and, therefore, a rapid increase in swelling ratios. The small deswelling
that occurred at pH 9 is considered to be due to an increase of ionic strength in
the buﬀer solution at pH 9, which might inhibit the polymer—water interactions
inside the hydrogel matrix. The swelling ratio increased with the PAAc
content within the PVA/PAAc IPNs.
The relationship between the changes in molecular structure in the IPN
hydrogel and electrolytes in the buﬀer solution is shown in Table 6.2. The
ionization of carboxylic acid in the IPN hydrogel was an important factor in
the pH-dependent swelling. However, the interaction between ionic groups in
the IPN chains and electrolytes in the buﬀer solution became more intense
when the pH of the buﬀer solution changed from 4 to 7; therefore, when a pH
was below the pK value of the PAAc (at pH 4) in which the carboxylic acid
group in the IPN hydrogel was in a hydrogenated state, the eﬀect of the ionic
strength on the swelling was less than a pH above the pK value of PAAc (at
pH 7) in which the carboxylic group in the IPN hydrogel was in an ionized
state. For the buﬀer solution at pH 7, in which the ionic strength was adjusted
to 0.01, the swelling ratio of each IPN sample became high, ranging from 15.2
to 33.4, while the increase of electrolyte concentration to 0.1 in the medium
produced a drastic collapse of all the IPN hydrogels. However, the swelling of
all IPN hydrogels at pH 4 was not dependent on ionic strength, as can be seen
in Table 6.2.
6.3.3 Release experiment of drug from PVA/PAAc IPNs
All the samples exhibited higher release rates at higher temperatures. These
results are in correspondence with the temperature-dependent swelling
behaviours of PVA/PAAc IPN hydrogels. All IPN samples showed positive
temperature-sensitive systems before they reached the equilibrated state. The
Stimuli-responsive interpenetrating polymer network hydrogels 99
Table 6.2 Effect of pH and ionic strength in the swelling medium on the
equilibrium swelling ratio of IPN hydrogels
Sample pH Ionic strength Swelling ratio
IPN37 7 0.01 32.3 ± 0.92
IPN46 4 0.1 6.8 ± 0.44
0.01 6.0 ± 0.91
7 0.1 16.3 ± 1.80
0.01 28.0 ± 0.36
IPN55 4 0.1 4.2 ± 0.47
0.01 4.4 ± 0.30
7 0.1 11.9 ± 1.80
0.01 21.5 ± 1.50
IPN64 4 0.1 5.5 ± 1.32
0.01 4.9 ± 1.20
7 0.1 10.1 ± 0.67
0.01 17.4 ± 0.58
IPN73 7 0.01 14.5 ± 1.13
release of the incorporated drugs within IPN hydrogels was delayed for about
10—15 hours, which was not enough time for all the samples to be fully
equilibrated. The release proﬁles indicated positive temperature-sensitive
release behaviours, and thus the composition of IPN was negligible in the
temperature-dependent release system.
The changes of release rate for IPN46, IPN55, IPN64 hydrogels in response
to stepwise temperature changes between 25 and 45 °C are shown in Fig. 6.4.
High release rates are obtained at 45 °C, while low release rates are observed
during the lower temperature period, as mentioned above. The released
amounts from IPN46 and IPN55 are almost the same, while the released
amount from IPN64 is small due to the low swelling. In the case of IPN64, the
fact that the hydroxyl groups in PVA formed hydrogen bonding and had little
chance to experience the ionic repulsion from carboxylate groups was proved.
The pH-sensitive release behaviours of indomethacin were observed at
25 °C with change in pH. Indomethacin is expected to diﬀuse through the
water-swelling region in the polymer gel. At pH 4, PAAc is in the form of
carboxylic acid, which produces hydrogen bonding with the hydroxyl group of
PVA, resulting in the decrease of drug release. However, at pH 7, carboxylate
ions formed in PAAc induced the drastic increase of swelling which exhibited
high release rate. The release amounts from IPN46 and IPN55 were almost
identical, and IPN64 gave lower values due to signiﬁcant low swelling
compared to the others at pH 4. It is considered that the release rate from IPN
hydrogels is nearly independent of the composition of samples at pH 4. In the
100 Smart ﬁbres, fabrics and clothing
6.4 Release change of indomethacin from IPN hydrogels in response
to stepwise temperature change between 25 °C and 45 °C; (*) IPN46,
() IPN55, (
case of the drug release experiment at pH 7, more PAAc contents in IPN
contributed to the higher release amount.
Oscillatory release proﬁles at 25 °C with changing pH levels between 4 and 7
are shown in Fig. 6.5. The plot gives the reversible change of release rate with
pH ﬂuctuation. IPN46 and IPN55 showed lower release at pH 4 and higher at
pH 7, and continued reversible behaviour during the experiment. However,
IPN64 did not show sharp reversible change because it did not have enough
6.3.4 Solute permeation through PVA/PAAc IPNs
Solute permeation experiments were performed using ﬁve representative
solutes with diﬀerent molecular weights and hydrodynamic sizes. The
characteristics of selected solutes are listed in Table 6.3. In the experimental
buﬀer solution in which pH was adjusted to 4 or 7, theophylline, vitamin
B and BSA were in a neutral state, and riboﬂavin and cefazolin
showed ionized structures.
Table 6.4 shows the results of solute permeation experiment measured at 25
and 45 °C, respectively. The permeation of solutes through IPN hydrogels as a
Stimuli-responsive interpenetrating polymer network hydrogels 101
Table 6.3 Characteristics of permeating solutes
Hydrodynamic Ionic property
Solutes MW radius (Å) at pH 7
Theophylline 180 3.5 Neutral
Riboﬂavin 376 5.8 Ionic
Cefazolin 476 6.5 Ionic
Vitamin B12 1355 8.5 Neutral
BSA 65 000 36.1 Neutral
6.5 Release change of indomethacin from IPN hydrogels in response to
stepwise pH change between pH 4 and 7; (*) IPN46, () IPN55, (
function of temperature was in accordance with the swelling behaviours of the
IPNs. IPN46 exhibited a positive swelling change with temperature, as
described in the swelling experiments. Therefore, all the solutes showed higher
diﬀusion coeﬃcients at high temperature. This is explained by the fact that the
increase of diﬀusion coeﬃcients at high temperature does not alter the
interaction between solutes and IPN structure, but only causes an expansion
102 Smart ﬁbres, fabrics and clothing
Table 6.4 The permeation studies of various solutes through IPN46 hydrogel at
pH 7 buffer solution (I = 0.01)
Temp. Pa Dc
Solute (°C) (;106 cm2/s) Kd b (;106 cm2/s)
Theophylline 25 7.63 ± 0.127 1.55 ± 0.035 4.94 ± 0.195
Riboﬂavin 25 0.99 ± 0.007 2.97 ± 0.028 0.33 ± 0.001
Cefazolin 25 0.42 ± 0.007 5.67 ± 0.064 0.07 ± 0.003
Vitamin B12 25 1.80 ± 0.099 1.20 ± 0.064 1.51 ± 0.163
BSA 25 1.03 ± 0.134 2.75 ± 0.043 0.41 ± 0.052
Theophylline 45 9.90 ± 0.141 0.81 ± 0.014 12.22 ± 0.039
Riboﬂavin 45 1.52 ± 0.028 2.35 ± 0.014 0.65 ± 0.016
Cefazolin 45 1.38 ± 0.092 9.14 ± 0.042 0.15 ± 0.011
Vitamin B12 45 4.06 ± 0.170 1.89 ± 0.099 2.15 ± 0.023
BSA 45 3.86 ± 0.134 4.74 ± 0.031 0.81 ± 0.034
P: permeability coefﬁcient, bKd : partition coefﬁcient, cD: diffusion coefﬁcient
n = 3 for each sample.
of IPN networks. Higher swelling in IPN at high temperature increases the
free volume through which the solutes permeate more freely.
The partition coeﬃcients (K ) of solutes between hydrogel membranes and
surrounding solutions are also shown in Table 6.4. The value of K is driven by
interactions between the solutes and the polymer molecular structure. Due to
the hydrophilicity of PVA/PAAc IPN hydrogels, it is predicted that more
hydrophilic solutes are well distributed throughout the entire hydrogel
membranes. As can be seen in Table 6.4, the K values of ionic solutes such as
riboﬂavin and cefazolin are greater than those of non-ionic solutes, obviously
due to induced ionic interaction between ionic solutes and the carboxylic acid
group. BSA showed the largest K value among non-ionic solutes. This is
believed to be caused by the protein adsorption to the polymer surfaces.
However, further study is needed to verify the interaction, which aﬀects and
determines the partition coeﬃcients of solutes within the swollen hydrogels.
The size of the solute was an important factor in determining the diﬀusion
and thus permeation through IPN hydrogels. The hydrodynamic sizes of three
solutes is in the range from 3.5 Å to 36.1 Å, as seen in Table 6.3. For non-ionic
solutes which had no ionic interaction with ionizable hydrogel membranes,
theophylline, having the smallest molecular size of 3.5 Å, showed the most
rapid diﬀusion through the hydrogel. The diﬀusion of vitamin B (hydrodynamic
radius : 8.5 Å) was faster than that of BSA (hydrodynamic radius : 36.1 Å).
The free volume caused by hydration may allow the pathway of solutes
through which the larger molecules were excluded in the permeation.
However, the diﬀusion of ionic solutes such as riboﬂavin and cefazolin were
independent of their hydrodynamic size. Riboﬂavin and cefazolin, which are
Stimuli-responsive interpenetrating polymer network hydrogels 103
smaller in size than vitamin B and BSA, gave a drastic reduction of diﬀusion
coeﬃcients. The permeability of solutes through IPN46 exhibited a similar
tendency with diﬀusion coeﬃcients. These results are indicative of the fact that,
in the ionizable hydrogel membranes, the solute diﬀusion is much aﬀected by
solute size, as well as by ionic interaction between solutes and membranes.
6.3.5 Electro-responsive properties of PVA/PAAc IPNs
To investigate the electric-responsive behaviour of PVA/PAAc IPN hydrogel
under electric stimulus, we measured the bending degree of IPN by varying
several factors. When PVA/PAAc IPN hydrogel in NaCl electrolyte solution
is subjected to an electric ﬁeld, the IPN bends toward the anode. The gradient
slope in the plot of the bending angle vs. time became steeper with increasing
applied voltage, and then levelled oﬀ at steady state. Note that the equilibrium
bending angle (EBA) and the bending speed increase with applied voltage.
This could be explained by the fact that there was an enhancement in the
transfer rate of the counter ions of the immobile carboxylate groups of PAAc
within PVA/PAAc IPN from IPN to external solution and free ion moved
from external solution into IPN, as the potential gradient in the electric ﬁeld
We investigated the eﬀect of PAAc content on the EBA of IPN in 0.1 M
NaCl solution at 10 V. As the content of the PAAc network increased, the EBA
increased linearly. The bending speed also increased in proportion to the
content of PAAc in the IPN. This may indicate that the EBA is not a
rate-limiting step for bending in an equilibrated state.
In addition, the EBA and bending kinetics of IPN37 were measured in NaCl
solution with diﬀerent ionic strength. There was a critical ionic strength for the
bending of PVA/PAAc IPN. The bending degree increased with ionic strength
when the latter was less than 0.1, while it decreased at ionic strength of greater
than 0.1. Furthermore, when the ionic strength of NaCl solution was 1.0, we
could not observe the bending behaviour of PVA/PAAc IPN under the 10 V of
applied voltage. As described above, an increase of electrolyte concentration in
the solution induces the increase of free ions moving from the surrounding
solution toward their counter electrode or into the IPN. As a result, the
bending degree and speed of the IPN could increase. However, if the ionic
strength of the solution is greater than a critical concentration, the shielding
eﬀect of polyions by the ions in the electrolytic solute occurred, leading to a
reduction in the electrostatic repulsion of polyions and a decrease in the degree
of bending. As already shown in Table 6.2, the swelling ratio of PVA/PAAc
IPN in solution with the lower concentration of electrolyte (ionic strength : 0.01)
was greater than that of higher electrolyte concentration (ionic strength : 0.1).
Therefore, if it is compared with the bending results depending on the ionic
104 Smart ﬁbres, fabrics and clothing
6.6 Reversible bending behaviour of IPN37 in NaCl solution (ionic
strength = 0.1) with changes in applied voltage 10 volts every 10 min.
strength of the solution, we could consider that the swelling of PVA/PAAc
IPN by ionic strength does not signiﬁcantly aﬀect the bending behaviours of
the IPN. In addition, stepwise bending behaviour of PVA/PAAc IPN
depending on electric stimulus was observed for IPN in 0.1 M NaCl solution,
with changes in the applied voltage of 10 V every 10 minutes. When the electric
stimulus was removed, the IPN displaced to its original position. Also, if the
polarity of the electric ﬁeld was altered, IPN bent in the opposite direction. As
shown in Fig. 6.6, PVA/PAAc IPN exhibited reversible bending behaviour
according to the application of the electric ﬁeld.
6.3.6 Drug release behaviour under electric ﬁelds
To investigate the electrically induced release behaviours of drugs, we
determined the amount of released drug from PVA/PAAc IPN into a release
medium under various conditions by UV-spectrophotometer. The drug-loaded
IPN disk was placed between two carbon electrodes in a release chamber ﬁlled
with a release medium. Applied voltage was then altered every 30 min.
Figure 6.7 exhibits the release behaviours of drugs from IPN37 as a function
of time and the voltage of applied electric ﬁeld in 0.9 wt % NaCl solution at
37 °C. The release behaviours of drugs from IPN37 as a function of time and
the voltage of applied electric ﬁeld in 0.9 wt % NaCl solution at 37 °C were
investigated. Figure 6.7 shows the plot of M /M vs. time (min) while altering
electric stimulus. Here, M is the amount of drug released up to time t, and M
is the amount of drug present in the IPN at time t : 0. Depending on the
electric stimulus being turned on and oﬀ, the release of drug molecules loaded
Stimuli-responsive interpenetrating polymer network hydrogels 105
6.7 Release behaviours of cefazoline and theophylline from PVA–PAAc
IPN55 as a function of applied voltage in 0.9% NaCl solution at 37 °C.
Electric potential was altered every 30 min. —*— IPN55C, 10 V, ——
IPN55C, 5 V, —
— IPN55C, 0 V, —
— IPN55T, 5 V.
within PVA/PAAc IPN was switched on and oﬀ in a pulsatile fashion. A
possible reason for this switching pattern of the release of drug molecules was
that the electrically induced changes in osmotic pressure within the gel and
local pH gradient attributed to water electrolysis could aﬀect the swelling of
IPN with charged groups.
In the case of theophylline (non-ionic solute), however, the magnitude of the
‘ON—OFF’ release pattern induced by the electrical stimulus was not so large
as that of cefazolin (ionic solute). Particularly, the release rate of theophylline
from IPN55T (theophylline-loaded IPN55) under 5 volts of electric potential
was even smaller than that of cefazolin from IPN55C (cefazolin-loaded
IPN55) without electric stimulus.
We conducted the release experiment of a drug from cefazolin- or
theophylline-loaded IPN46 in NaCl solution with diﬀerent ionic strength to
examine the eﬀect of the ionic strength of the release medium. Figure 6.8 shows
the release behaviours of cefazolin and theophylline as a function of ionic
strength in release medium at 5 V. In the case of IPN46C, the release rate of
cefazolin increased in inverse proportion to the ionic strength of the release
medium. Therefore, an increase of electrolyte concentration in the solution
induces the movement of free ions from the surrounding solution toward their
counter electrode or into IPN, resulting in an increase in release rate of
cefazolin from charged PVA/PAAc IPN. The change of swelling in the
PVA/PAAc IPN due to the ionic strength of the surrounding medium does not
106 Smart ﬁbres, fabrics and clothing
6.8 Effect of ionic strength in release medium on release behaviours of
cefazoline and theophylline from IPN46 under 5 V applied voltage. —*—
IPN46C, 0.01 M NaCl, —— IPN46C, 0.1 M NaCl, —
— IPN46C, 0.2 M
— IPN46T, 0.1 M NaCl.
signiﬁcantly aﬀect the release behaviours of the drug. It rather indicates that
the electrically induced changes of osmotic pressure within the gel, the local
pH gradient attributed to water electrolysis, and the squeezing eﬀect of IPN
gel were more important than the decrease of the swelling ratio due to the ionic
strength of the release medium. However, in view of the ionic property of
drugs, we can see that the release rate of ionic drugs is much faster than that of
non-ionic drugs. An IPN46T sample containing a non-ionic drug, theophylline,
exhibited a slower release rate in 0.1 M NaCl at 5 V than the ionic drug,
cefazolin, in 0.01 M NaCl. This could be attributed to the enhancement of the
release by electrophoresis of charged drug molecules.
PVA/PAAc IPNs with various compositions were prepared by a sequential
synthetic method composed of UV polymerization and freeze—thawing
process. A PVA/PAAc IPN exhibited diﬀerent swelling patterns as a function
of pH, temperature, ionic strength of external solution, and the content of ionic
group in IPN. The release of indomethacin from these IPN hydrogels was
dominated by the magnitude of swelling in the IPN hydrogels. In the
temperature-sensitive system, the positive release of drugs caused by the
hydrogen bonding between PVA and PAAc was observed, showing an
increase of the released amount with higher temperature. In the case of
Stimuli-responsive interpenetrating polymer network hydrogels 107
pH-dependent release, changing the pH controlled the release rate. At pH 7,
higher release amounts were observed, since the water contents after swelling
increased signiﬁcantly. The permeability of non-ionic solutes changed according
to the variation in swelling in the IPN hydrogel. Smaller solutes and higher
swelling of the IPN hydrogel produced higher diﬀusion coeﬃcients. However,
the permeability of ionic solutes at pH 7 through IPN decreased, while the
swelling of the IPN hydrogel increased. When a swollen PVA/PAAc IPN was
placed between a pair of electrodes, the IPN exhibited bending behaviours
upon the application of an electric ﬁeld. The release behaviours of drug
molecules from negatively charged PVA/PAAc IPN were switched on and oﬀ
in a pulsatile pattern depending on the applied electrical stimulus. The release
amount and the release rate of the drug were inﬂuenced by the applied voltage,
the ionic group contents of the IPN, the ionic properties of the drug, and the
ionic strength of the release medium. Therefore, the present IPN system was
valid in pH/temperature/electrical-responsive drug delivery.
1 Kwon C, Bae Y H and Kim S W, ‘Heparin release from polymer complex’, J.
Controlled Release, 1994, 30, 155.
2 Yuk S H, Cho S H and Lee H B, ‘Electric current-sensitive drug delivery systems
using sodium alginate/polyacrylic acid composites’, Pharm. Res., 1992, 9, 955.
3 Okahata Y and Seki T, ‘pH-sensitive permeation of ionic ﬂuorescent probes nylon
capsule membranes’, Macromolecules, 1984, 17, 1880.
4 Okahata Y, Noguchi H and Seki T, ‘Functional capsule membrane. 26. Permeability
control of polymer-grafted capsule membrane responding to ambient pH changes’,
Macromolecules, 1987, 20, 15.
5 Gudeman L F and Peppas N A, ‘pH-sensitive membranes from poly(vinyl
alcohol)/poly(acrylic acid) interpenetrating networks’, J. Mem. Sci., 1995, 107, 239.
6 Feil H, Bae Y H, Feijen T and Kim S W, ‘Mutual inﬂuence of pH and temperature
on the swelling of ionizable and thermosensitive hydrogels’, Macromolecules, 1992,
7 Yoshida M, Yang J S, Kumakaru M, Hagiwara M and Katakai R, ‘Artiﬁcially
intelligent hydrogels: responding to external stimuli such as temperature and pH’,
Eur. Polym. J., 1991, 27, 997.
8 Gutowska A, Bae Y H, Jacobs H, Feijen J and Kim S W, ‘Thermosensitive
interpenetrating polymer network: synthesis, characterisation, and macromolecular
release’, Macromolecules, 1994, 27, 4167.
9 Okano T, Bae Y H, Jacobs H and Kim S W, ‘Thermally on—oﬀ switching polymers
for drug permeation and release’, J. Controlled Release, 1990, 11, 255.
10 Siegal R A and Firestone B A, ‘pH-dependent equilibrium swelling properties of
hydrophobic polyelectrolyte copolymer gels’, Macromolecules, 1988, 21, 3254.
11 Kim J H, Kim J Y, Lee Y M and Kim K Y, ‘Properties and swelling characteristics
of crosslinked poly(vinyl alcohol)/chitosan blend membrane’, J. Appl. Polym. Sci.,
1992, 45, 1711.
108 Smart ﬁbres, fabrics and clothing
12 Kim J H, Kim J Y, Lee Y M and Kim K Y, ‘Controlled release of riboﬂavin and
insulin through crosslinked poly(vinyl alcohol)/chitosan blend membrane’, J. Appl.
Polym. Sci., 1992, 44, 1823.
13 Katono H, Maruyama A, Sanui K, Ogata N, Okano T and Sakurai Y,
‘Thermo-responsive swelling and drug release switching of interpenetrating
polymer networks composed of polycylamide-co-butyl methacrylate) and poly(acrylic
acid)’, J. Controlled Release, 1991, 16, 215.
14 Schilld H G, ‘Poly(N-isopropyl acrylamide): experiment, theory and application’,
Prog. Polym. Sci., 1992, 17, 163.
15 Brannon L and Peppas N A, ‘Solute and penetrant deﬀusion in swellable polymers.
IX. The mechanisms of drug release from pH-sensitive swelling-controlled systems’,
J. Controlled Release, 1989, 8, 267.
16 Hoﬀman A S and Dong L C, ‘A novel approach for preparation of pH-sensitive
hydrogels for enteric drug delivery’, J. Controlled Release, 1991, 15, 141.
17 Kishi R, Hara M, Sawahata K and Osada Y, Polymer Gels: Fundamentals and
Biomedical Applications, Plenum Press, New York, 1991, p. 205.
18 Osada Y, Okuzaki H and Hori H, ‘A polymer gel with electrically driven motility’,
Nature, 1992, 355, 242.
19 Chiarelli P, Umezawa K and Rossi D D, Fundamentals and Biomedical Applications,
Plenum Press, New York, 1991, p. 195.
20 Ma J T, Liu L R, Yang X J and Yao K D, ‘Blending behavior of gela-
tin/poly(hydroxyethyl methacrylate) IPN hydrogel under electric stimulus’, J. Appl.
Polym. Sci., 1995, 56, 73.
21 Kim S S and Lee Y M, ‘Synthesis and properties of semi-interpenetrating polymer
networks composed of -chitin and poly(ethylene glycol) macromer’, Polymer,
1995, 36, 4497.
22 Lee Y M, Kim S H and Cho C S, ‘Synthesis and swelling characteristics of pH and
thermo-responsive interpenetrating polymer network hydrogel composed of
poly(vinyl alcohol) and poly(acrylic acid)’, J. Appl. Polym. Sci., 1996, 62, 301.
23 O’Neil M J, Smith A, Heckelman P E and Budavari S, in The Merck Index, 11th ed.,
Merck Co., Rahway, NJ, 1989.
24 Florey K, Analytical Proﬁles of Drug Substances, Vol. 4, Academic Press, New York,
Permeation control through stimuli-responsive
polymer membrane prepared by plasma and
radiation grafting techniques
YOUNG MOO LEE AND JIN KIE SHIM
Stimuli-sensitive polymer drug delivery, especially using temperature and
pH-sensitive hydrogels and polymeric membranes, may be applied to enhance
environment-sensitive properties. Temperature-sensitive polymers demonstrate
lower critical solution temperatures (LCST), which provide reversible high
swelling at low temperatures and low swelling at high temperatures.—
Similarly, pH-sensitive polymers synthesized with either acidic or basic
components demonstrate reversible swelling/deswelling in an acidic or basic
Hoﬀman and Dong combined these two properties by synthesizing
cross-linked pH/temperature-sensitive hydrogels. Positively charged hydrogels
were prepared by copolymerizing in varying ratios of N-isopropylacrylamide
and N,N-dimethylaminopropylmethacrylamide. Kim et al. made beads
formed from linear pH/temperature polymers, poly(N-isopropylacrylamide-co-
butylmethacrylate-co-acrylic acid) and reported on the release of insulin
through the polymeric system.
There have been several studies reported on the surface modiﬁcation of
porous membranes by grafting acrylic monomers utilizing corona discharge,
glow discharge and UV techniques.— Iwata et al. reported on the graft
polymerization of acrylamide onto a polyethylene using corona discharge
and of N-isopropylacrylamide onto a poly(vinylidene ﬂuoride) using the
glow discharge technique. Osada et al. grafted poly(methacrylic acid) onto a
porous poly(vinyl alcohol) membrane using plasma treatment, and their ion
transport, albumin and poly(ethylene glycol) permeation behaviours were
studied. X-ray photoelectronspectroscopy (XPS) was utilized to conﬁrm the
graft reaction.— Recently, Ito et al. reported on the water permeation
through porous polycarbonate membrane having poly(carboxylic acid) on the
membrane surface by pH and ionic strength.
It is our objective to review the intelligent pH/temperature-sensitive
membrane by grafting acrylic acid (AAc) and N-isopropylacrylamide (NIPAAm)
110 Smart ﬁbres, fabrics and clothing
onto the porous polymer membrane, which was prepared by the plasma or UV
Acrylic acid (AAc) was obtained from Junsei Chemical Co. and used as a
grafting monomer. It was puriﬁed by using a glass column ﬁlled with an
inhibitor remover (Aldrich Co., Milwaukee, WI) and stored in a dark and cold
place. N-isopropylacrylamide (NIPAAm; Tokyo Kasei Chemical Co., Japan)
was used after recrystallization in hexane and toluene (40 : 60 in vol %).
Riboﬂavin was purchased from Junsei Chemical Co. and used without any
further treatment. Porous polyamide membrane from Gelman Science Co.
with 127 m in thickness, 0.45 m pores and 1,1-dimethyl-2-picrylhydrazyl
(DPPH) (Aldrich Co.) was used for the determination of peroxides produced
by UV irradiation.
7.2.2 Determination of peroxide produced by UV
The PSF membrane was irradiated by a medium-pressure mercury lamp
(450 W, Ace Glass Inc.) at room temperature in air for a predetermined time.
The membrane samples were prepared to an area of 8.675 cm and irradiated
at a distance of 5 cm below the UV lamp for all samples. Peroxides produced
on the membrane surface were determined by DPPH. The DPPH
(1 ; 10 mol/l) solution in toluene was degassed by nitrogen blowing for
60 min. The UV-treated PSF membrane was quickly dipped into the DPPH
solution at 60 °C for 2 hours in a shaking water bath. Using the reacted
solutions, a consumed amount of DPPH due to peroxides produced on the
surface was measured by a UV spectrophotometer (UV-2101PC, Shimadzu,
Kyoto, Japan) at 520 nm. A calibration curve was obtained by using a DPPH
solution of a known concentration.
7.2.3 Preparation of stimuli-responsive polymeric membranes
126.96.36.199 Preparation of poly(amide-g-NIPAAm) and
For the plasma polymerization, a bell jar type plasma reaction apparatus was
used to accommodate the AAc and NIPAAm monomers. This low pressure
glow discharge apparatus has a radio-frequency generator (13.56 MHz, 0—300 W
Permeation control through stimuli-responsive polymer membrane 111
Table 7.1 Effect of feed composition on the graft yield of surface modiﬁed
polyamide membranes using plasma polymerization method at 60 °C for 2
Feed composition Concentration Graft yield
Sample NIPPAm/AAc (w/w) (wt %) ( g/cm2)
PA — 20 —
PNA1 100: 0 20 202
PNA2 95: 5 20 222
PNA3 90: 10 20 297
PNA4 85: 15 20 197
power) and an impedance matching circuit. After washing and drying, the
porous polyamide membrane was applied to 50 mtorr and 30 W argon plasma
for 30 seconds. The sample was exposed immediately to the air and immersed
in the monomer solution. The AAc and NIPAAm monomer solutions were
prepared by dissolving each monomer in deionized water (see Table 7.1) for
sample designation. To remove the oxygen remaining in the solution, nitrogen
gas was bubbled into the solution at room temperature for 30 min. The graft
polymerization of AAc and NIPAAm onto the plasma-treated polyamide was
performed for 2 h at 60 °C.
The grafting amount of treated polyamide membranes was calculated as
(W 9 W )
Graft yield ( g/cm) : R ; 100,
where W , W and A represent the weight of the membrane before and after
the graft reaction and membrane area, respectively.
188.8.131.52 Preparation of PSF-g-AAc membrane
The PSF membrane (17.35 cm) was weighed precisely and irradiated at the
same conditions as in the peroxide-determination experiments. 20 wt. % AAc
aqueous solution was degassed by nitrogen blowing for 60 min. UV-treated
PSF was quickly dipped into the solution at 60 °C for 2 h in a shaking water
bath. The grafted membranes were washed with deionized water at 70 °C for
24 h and dried in a vacuum oven at 40 °C for 48 h. Details on analytical
equipment and methods and the solute permeation experiments can be found
in the references.
112 Smart ﬁbres, fabrics and clothing
7.3 Results and discussion
7.3.1 Characterization of stimuli-responsive polymeric
184.108.40.206 Poly(amide-g-NIPAAm) and poly(amide-g-(AAc-NIPAAm)) membranes
The surface of AAc and NIPAAm grafted polyamide membrane was analysed
by XPS— as shown in Fig. 7.1 and 7.2. The PNA membrane surface
showed new peaks resulting from the incorporation of —C—O— at : 286.6 eV
and ester carbon atoms at : 289.1 eV (O C—O—). The poly(amide-g-NIPAAm)
(PNA1) surface showed a new peak : 288.0 eV as O C—N, indicating the
presence of N-isopropyl groups on the polyamide surface. The oxygen peak in
the C O groups appeared at 529 eV for membranes. The peak at high binding
energy region (533.5 eV) is a peak for the oxygen in the —OH groups, indicating
the presence of —COOH groups on the grafted PNA membrane surface. As the
AAc content increases, the —OH peak becomes larger relative to the peak of
the C O bond.
290 286 282 278
Binding energy (eV)
7.1 XPS carbon 1S core level spectra of polyamide and grafted polyamide
Permeation control through stimuli-responsive polymer membrane 113
In the present study, the graft yields of the polymer range between
197—297 g/cm (see Table 7.1) and increase with increasing AAc content,
except for the PNA4 sample. When the AAc content was more than 10 wt %
of the feed composition, the graft yield of the membrane decreased. These
results also showed that upon increasing the pH, the reactivity ratio decreased
and increased for acrylic acid and acrylamide, respectively. The pH of the feed
solution in Table 7.1 decreased from 4.7 to 2.7 as acrylic acid increased.
Therefore, the lower graft yield in PNA4 is probably due to the low reactivity
of NIPAAm at above 10 wt % of acrylic acid in the feed composition because
of the low pH.
220.127.116.11 PSF-g-AAc membranes
It is known that PSF and poly(ether sulfone) show strong absorption bands in
the wavelength range between 250 and 300 nm. During UV irradiation,
chain scission, cross-linking and extensive yellowing occur. UV irradiation in
a vacuum or in air yields several degraded products, such as gaseous products,
oligomeric or polymeric sulfonic acids, and polymeric peroxides.
536 532 528 524
Binding energy (eV)
7.2 XPS carbon 1S core level spectra of polyanide and grafted polyamide
114 Smart ﬁbres, fabrics and clothing
Radical density + 10 8 (mol/ cm 2 ) 20
0 50 100 150 200
Irradiation time (s)
7.3 Effect of radical density as a function of UV irradiation time as
determined by the DPPH method.
Kuroda et al. reported the tendency of chain scission and cross-linking of
poly(ether sulfone) ﬁlms below and above the glass transition temperature
(T ). Chain scission and cross-linking occur simultaneously in all ranges of
experimental temperatures. Cross-linking is dominant at above 170 °C, while
chain scission is more important at room temperature. Yamashita et al.
reported on the photodegradation of poly(ether sulfone) and PSF in the
presence and absence of oxygen over the temperature range from room
temperature to 225 °C, and investigated the quantum yields for cross-linking
and chain scission by gel permeation chromatography (GPC) measurements.
They showed similar results on the temperature eﬀect of chain scission and
cross-linking from the degradation of poly(ether sulfone). However, in the
case of PSF, chain scission occurs even at higher temperatures.
Figure 7.3 shows the radical density of a UV-irradiated PSF membrane
with varying irradiation times. The radical density increased with increasing
irradiation time up to 150 seconds, but decreased slightly with further irradiation.
This indicates that the produced peroxides are partially converted into inactive
species, which cannot generate radicals.
Table 7.2 summarizes the amount of PAAc grafted onto the surface of the
PSF membrane. The graft amount of PAAc increased with irradiation time up
to 150 s, exhibiting the same tendency as did the result from the radical density
data. When we further irradiated the PSF samples, the graft amount and
radical density of the modiﬁed PSF membrane decreased slightly. This means
that long irradiation times do not always provide a merit in the amount of
PAAc grafted onto the PSF membranes. Characterization and permeation
experiments were done for grafted membranes irradiated up to 150 s.
Permeation control through stimuli-responsive polymer membrane 115
Table 7.2 Effect of UV irradiation time on the amount of grafting of
surface-modiﬁed PSF membranes
Irradiation time Amount of grafting
Samplea (s) ( g/cm2)
PSF — —
UA1 10 53
UA2 30 57
UA3 90 62
UA4 120 71
UA5 150 104
UA6 180 98
A 20 wt % aqueous solution of AAc was used.
Table 7.3 XPS surface analysis of surface-modiﬁed PSF membranes by UV
Sample C1S O1S S2P O1S/S2P
PSF 90.70 3.92 5.37 0.73
UA1 90.81 4.18 5.01 0.83
UA2 91.69 4.00 4.11 0.97
UA3 87.93 6.28 5.60 1.08
UA4 90.20 5.43 4.37 1.24
UA5 91.08 5.08 3.85 1.32
To investigate the chemical composition of the membrane surface, XPS
analyses of the PSF and PSF-g-AAc membranes were performed and are
summarized in Table 7.3. The atomic concentration of S for the unmodiﬁed
PSF membrane is 5.37% and can be used as a reference on the basis that it
does not change after UV irradiation. The atomic concentration of grafted
membranes, the ratio of O to S , gradually increases upon prolonging the
UV irradiation time up to 150 s (UA5). This indicates that the atomic
concentration of O in the surface region increases as AAc is grafted further.
An inert gas ion beam was used to ablate the sample surface, and the
chemical composition of the new surface was determined by XPS surface
analysis. XPS ion-sputter depth proﬁling is a valuable means of determining
the thickness of the graft layer. The eﬀective thickness of the graft layer was
calculated and the thickness of the PAAc grafted onto the PSF membrane
surface in UA1 and UA3 was determined to be around 80—100 nm. Moreover,
we can also determine the thickness of the graft layer from the relation
116 Smart ﬁbres, fabrics and clothing
Permeability coefficient + 10 6 (cm 3 cm/cm 2 s)
3 4 5 6 7 8
7.4 Effect of pH on the permeation of riboﬂavin through PA and PNA
membranes measured at 37 °C. —*— PA, —— PNA1, —
— PNA3, —s— PNA4.
l : m/ A, where l is the thickness of the graft layer, m the amount of grafting,
the density of the graft PAAc and A the unit area. Here, the PAAc density is
approximately 1. The thickness of the UA1 and UA3 samples can be calculated
to be approximately 530—620 nm, indicating a large discrepancy between the
thickness values determined by the two methods. The thickness determined
by an XPS method is much smaller than that by the amount of grafting. This
result suggests that PAAc was grafted not only onto the surface of the PSF
membrane but also onto the inside of the PSF membrane. In this case, an
aqueous AAc solution was expected to diﬀuse into the PSF membrane, and
the vinyl monomer was grafted not only at the surface but also within the
membrane. Tazuke reported that acrylamide was grafted more from the
bulk of the hydrophobic-oriented polypropylene membranes than on the
surface of the membranes when the solvent had strong interactions with the
7.3.2 Riboﬂavin permeation through stimuli-responsive
18.104.22.168 Poly(amide-g-NIPAAm) and poly(amide-g-(AAc-NIPAAm)) membranes
The riboﬂavin release patterns of PA and PNA membranes at diﬀerent pH
regions and at 37 °C are demonstrated in Fig. 7.4. The permeation of riboﬂavin
was also measured at various temperatures and at neutral pH, as shown in
Permeation control through stimuli-responsive polymer membrane 117
7.5 Effect of temperature on the permeation of riboﬂavin through PA and
PNA membranes measured at pH 7. —*— PNA1, —— PNA2, —
Fig. 7.5. In PA and PNA1 membranes that did not have acrylic acid on the
polyamide surface, the release proﬁle of riboﬂavin was constant as pH varied.
However, the PNA2, PNA3 and PNA4 membranes showed a pH-dependent
release of riboﬂavin. The permeability of riboﬂavin decreased from
6.3 ; 10 cm cm/cm s at pH 4 to around 5.7 ; 10 cm cm/cm s at pH 7.
The absolute permeability value was one order of magnitude higher than that
of the PVDF membrane in our previous study due to the larger pore radius
of the PA membrane.
However, the magnitude of the decrease of permeability at pH 4 to pH 7
was somewhat lower than that of the PVDF membrane. This may be caused
by two possible factors: the large pore size of the PA membrane and the lower
acrylic acid content in the feed solution.
The eﬀective graft chain for permeation is present on the inner pore or on
the edge of the pore, and may shrink or enlarge upon pH changes. Large pore
size may reduce the eﬀectiveness of the pH-dependent permeation of small
solutes unless the graft chain is long enough to cover the pores. Competitive
AAc and NIPAAm reaction reduced the number of the AAc content in the
chain and lowered the pH sensitivity, which is deﬁned as the ratio of permeability
at pH 4 and pH 7.
The eﬀective pore size of the PNA membranes at any pH and temperature
can be calculated using a simple Hagen—Poiseuille’s law and the ratio of ﬂux
or permeability coeﬃcient of the virgin and graft membrane.
118 Smart ﬁbres, fabrics and clothing
Table 7.4 Determination of effective pore radii and effective areas for permeation
at pH 4 and 7 through pH-sensitive polyamide membranes estimated by Eq. (7.1)
pH 4 pH 7
Sample r (Å) A* ( ; 106 Å2) r (Å) A* ( ; 106 Å2) ApH 7
PA 2250 15.90 2250 15.90 100.0
PNA1 2176 14.88 2176 14.88 100.0
PNA2 2147 14.48 2115 14.05 103.1
PNA3 2167 13.75 2103 13.89 106.2
PNA4 2172 14.82 2121 14.13 104.9
*A = Effective membrane area for permeation of solute.
r /r : [J /J ] [7.1]
Here, J and J are the ﬂuxes of solute through the PA and PNA membranes
respectively, at 37 °C in varying pH ranges.
The eﬀective pore radius was reduced from 2250 Å to 2103 Å upon grafting
and expansion of the graft chain at pH 7 (Table 7.4). The above results show
the possibility of controlling the pH region, in which the riboﬂavin permeability
changes most sensitively with pH, by choosing the nature of the polymers to
As NIPAAm is grafted on the porous polyamide membrane using the
plasma grafting technique, the permeability changes with temperature.
Poly(NIPAAm) is known to have LCST at around 31—33 °C. Below LCST,
poly(NIPAAm) forms hydrogen bonds with water and exists in solution form.
However, above LCST, inter- and intramolecular interaction in poly(NIPAAm)
is much stronger, resulting in an undissolved state. In this state, the hydrogen
bonding between grafted poly(NIPAAm) (PNA1) and water breaks down and
the mobility of the polymer chain, inter- and intramolecular interactions, and
the hydrophobic interaction due to the presence of the alkyl groups in the
polymer chain increase. The grafted poly(NIPAAm) chain shrinks, leading
to an enlargement of the eﬀective pore size in the porous polyamide membrane.
Using the same Hagen—Poiseuille’s equation and Eq. (7.1), the eﬀective pore
radius was calculated to be 2113 Å at 30 °C and the graft chains shrink to
2175 Å at 50 °C for PNA2 membrane, resulting in an expansion of the eﬀective
area for permeation, as indicated in increase in A ° /A ° in Table 7.5.
PNA2, PNA3 and PNA4 used the acrylic acid as a comonomer with
NIPAAm. In this case, the transition temperatures of riboﬂavin permeation
change from 35 °C to 50 °C, as illustrated in Fig. 7.5.
Permeation control through stimuli-responsive polymer membrane 119
Table 7.5 Determination of effective pore radii and effective areas for permeation
at 30 °C and 50 °C through temperature-sensitive polyamide membranes estimated
by Eq. (7.1)
Temperature 30 °C Temperature 50 °C
Sample r (Å) A* ( ; 106 Å2) r (Å) A* ( ; 106 Å2) A30 °C
PA 2250 15.90 2250 15.90 100.0
PNA1 2126 14.20 2182 14.96 100.3
PNA2 2113 14.03 2175 14.86 105.9
PNA3 2102 13.88 2162 14.69 105.9
PNA4 2118 14.09 2147 14.48 102.8
*A = Effective membrane area for permeation of solute.
Released amount of riboflavin (mg/h)
1 pH 7 pH 7
0 2 4 6 8 10 12 14 16
7.6 Reversible release pattern of riboﬂavin from PNA3 membrane with
step-wise changing of the pH between 7 and 4 measured at 37 °C. —*—
In order to study the pH/temperature-dependent change of the permeability
of riboﬂavin, the permeation of riboﬂavin through the PNA3 membrane was
investigated by alternating pH from 7 to 4 (Fig. 7.6), and temperature from 30
to 50 °C (Fig. 7.7). It was observed that a discontinuous change in concentration
of riboﬂavin was brought about by stepwise changing of the temperature or
pH. When the permeation experiment of riboﬂavin through the PNA3
membrane was conducted by changing pH or temperature, the riboﬂavin
release increased rapidly but reverted to the same permeability within an hour.
120 Smart ﬁbres, fabrics and clothing
7.7 Reversible concentration control of riboﬂavin from PNA3 membrane
with step-wise changing of the temperature between 30 °C and 50 °C
measured at pH 7. —*— PNA3.
22.214.171.124 PSF-g-AAc membranes
Riboﬂavin permeability through the original PSF membrane and the PSF-g-
AAc membranes is shown in Fig. 7.8, measured at diﬀerent pH values. Note
that the virgin PSF membrane exhibits no response to the change in pH,
whereas PSF-g-AAc membranes are responsive to the pH change. A remarkable
decline in permeability is noted in the range of pH 4—5. From these data, it is
clear that the grafted PAAc is responsible for the permeability decline in
It has been reported that the pK value of poly(acrylic acid) (PAAc) is
4.8. Above pH 4.8, the carboxylic acid groups of the grafted PAAc chains
are dissociated into carboxylate ions and have an extended conformation
because of the electrostatic repulsion forces between the chains. Extended
chains block the pores of the PSF membrane, causing a decrease in the
permeability. At below pH 4.8, carboxylic acid groups do not dissociate: the
grafted PAAc chains will shrink and be precipitated on the surface. Thus, the
pores become open and permeability increases sharply. These conformational
changes are obviously due to both intra- and intermolecular interactions
between the grafted PAAc chains.
As the amount of grafted PAAc increases further, pore blocking overwhelms
the conformational changes of the grafted chains due to the interactions of the
polymer chains, causing only small changes in the permeability of riboﬂavin
in response to the pH. Therefore, for a UA5 sample, the extension and
Permeation control through stimuli-responsive polymer membrane 121
Permeability coefficient + 10 6 (cm 3 cm/cm 2 s)
3 4 5 6 7
7.8 Effect of pH on the riboﬂavin permeation through (a) PSF (*), (b) UA1
(), (c) UA2 (
), (d) UA3 (
), (e) UA4 (s), (f) UA5 () membranes.
shrinkage of the grafted chains are hindered, and the extent of the change in
the permeability is reduced, meaning that the permeability depends on the
amount of grafting and the environmental pH.
We have prepared pH/temperature-sensitive polymer membranes by grafting
AAc or NIPAAm or AAc and NIPAAm on the surface of polyamide and
polysulfone membranes, utilizing plasma and UV radiation techniques. The
structure of the graft chain was conﬁrmed by XPS and ATR-FTIR spectra.
Through this study, we investigated the morphology and permeability of the
riboﬂavin of the unmodiﬁed and modiﬁed polymer membranes. AAc or
NIPAAm or AAc and NIPAAm-grafted polymer membranes showed the pH
or temperature and pH-dependent permeation behaviours of riboﬂavin,
Therefore, the present stimuli-responsive membrane system was valid in
pH/temperature-responsive drug delivery or intelligent separation membranes.
This study envisioned the possibility of controlling the permeability of the
membrane by varying the pH of the external solution. These pH/temperature-
responsive membranes will be useful for sensing and modulating external
chemical signals, and also for drug-delivery applications, because they change
their chain conformation according to the surrounding circumstances.
122 Smart ﬁbres, fabrics and clothing
Financial support from the Korea Institute of Science Technology
Evaluation and Planning through National Research Laboratory Programme
is greatly appreciated.
1 Okano T, Bae Y H, Jacobs H and Kim S W, ‘Thermally on—oﬀ switching polymers
for drug permeation and release’ J. Controlled Release, 1990, 11, 255.
2 Okano T, Bae Y H and Kim S W, ‘On—oﬀ thermocontrol of solute transport: II.
Solute release from thermosensitive hydrogels’ Pharmaceut. Res., 1991, 8, 624.
3 Nozawa I, Suzuki Y, Sato S, Sugibayashi K and Morimoto Y, ‘Preparation of
thermo-responsive polymer membranes’, J. Biomed. Mater. Res., 1991, 25, 243.
4 Okahata Y, Lim H J, Nakamura G and Hachiya S, ‘A large nylon capsule coated
with a synthetic bilayer membrane permeability control of NaCl by phase
transition of the dialkylammonium bilayer coating’, J. Amer. Chem. Soc., 1983, 105,
5 Kitano H, Akatsuka Y and Ise N, ‘pH-responsive liposomes which contain
amphiphiles prepared by using lipophilic radical initiator’, Macromolecules, 1991,
6 Siegel R A, Falamarzian M, Firestone B A and Moxley B C, ‘pH-controlled release
from hydrophobic/polyelectrolyte copolymer hydrogels’, J. Controlled Release,
1988, 8, 179.
7 Hoﬀman S and Dong L, ‘A novel approach for preparation of pH-sensitive
hydrogels for enteric drug delivery’, J. Controlled Release, 1991, 15, 141.
8 Park T G and Hoﬀman A S, ‘Synthesis and characterization of pH- and/or
temperature-sensitive hydrogels’, J. Appl. Polym. Sci., 1992, 46, 659.
9 Iwata H and Matsuda T G, ‘Preparation and properties of novel environment-sensitive
membranes prepared by graft polymerization onto a porous membrane’, J.
Membrane Sci., 1988, 38, 185.
10 Klumb L A and Horbett T A, ‘Design of insulin delivery devices based on glucose
sensitive membranes’, J. Controlled Release, 1992, 18, 59.
11 Kim J H, Kim J Y, Lee Y M and Kim K Y, ‘Controlled release of riboﬂavin and
insulin through crosslinked poly(vinyl alcohol)/chitosan blend membrane’, J. Appl.
Polym. Sci., 1992, 44, 1823.
12 Chung J, Ito Y and Imanishi Y, ‘An insulin-releasing membrane system on the basis
of oxidation reaction of glucose’, J. Controlled Release, 1992, 18, 45.
13 Ito Y, Kotera S, Ibana M, Kono K and Imanishi Y, ‘Control of pore size of
polycarbonate membrane with straight pores by poly(acrylic acid)’, Polymer, 1990,
14 Kim Y H, Bae Y H and Kim S W, ‘pH/temperature-sensitive polymers for
macromolecular drug loading and release’, J. Controlled Release, 1994, 28, 143.
15 Iwata H, Kishida A, Suzuki M, Hata Y and Ikada Y, ‘Oxidation of polyethylene
surface by corona discharge and the subsequent graft polymerization’, J. Polym.
Sci. Polym. Chem., 1988, 26, 3309.
Permeation control through stimuli-responsive polymer membrane 123
16 Suzuki M, Kishida A, Iwata H and Ikada Y, ‘Graft copolymerization of acrylamide
onto a polyethylene surface prepared with a glow discharge’, Macromolecules, 1986,
17 Iwata H, Oodate M, Uyama Y, Amemiya H and Ikada Y, ‘Preparation of
temperature-sensitive membranes by graft polymerization onto a porous membrane’,
J. Membrane Sci., 1991, 55, 119.
18 Osada Y, Honda K and Ohta M, ‘Control of water permeability by mechanochemical
contraction of poly(methacrylic acid)-grafted membranes’, J. Membrane Sci., 1986,
19 Ito Y, Inaba M, Chung D J and Imanishi I, ‘Control of water permeation by pH and
ionic strength through a porous membrane having poly(carboxylic acid) surface-
grafted’, Macromolecules, 1992, 25, 7313.
20 Kim J H, Lee Y M and Chung C N, ‘Permeation of drug through porous
polyurethane membranes grafted with poly(acrylic acid)’, J. Korean Ind. Eng.
Chem., 1992, 3, 233.
21 Lee Y M, Ihm S Y, Shim J K, Kim J H, Cho C S and Sung Y K, ‘Preparation of
surface-modiﬁed stimuli-responsive polymeric membranes by plasma and ultraviolet
grafting methods and their riboﬂavin permeation’, Polymer, 1994, 36, 81.
22 Palit S R and Ghosh P, ‘Quantitative determination of carboxyl endgroups in vinyl
polymers by the dye-interaction method, a theoretical investigation of molecular
core binding and relaxation’, J. Polym. Sci., 1962, 58, 1225.
23 Beamson G and Briggs D, High Resolution XPS of Organic Polymers, Wiley, UK,
1992, pp. 110—11, 188—201.
24 Clark D T, Cromarty B J and Dilks A H R, ‘A theoretical investigation of molecular
core building and relaxation energies in a series of oxygen-containing organic
molecules of interest in the study of surface oxidation of polymer’, J. Polym. Sci.
Polym. Chem., 1978, 16, 3173.
25 Rabek J F, Polymer Degradation, 1st. edn., Chapman Hall, London, 1995, p. 317.
26 Kuroda S I, Mita I, Obata K and Tanaka S, ‘The tendency of chain scission and
crosslinking of poly(ether sulfone) ﬁlms below and above the glass transition
temperature (Tg)’, Polym. Degrad. Stabil., 1990, 27, 257.
27 Yamashita T H, Tomitaka T, Kudo K, Horie K and Mita I, ‘The photodegradation
of poly(ether sulfone) and PSF in the presence and absence of oxygen’, Polym.
Degrad. Stabil., 1993, 9, 47.
28 Tazuke S, Matoba T, Kimura H and Okada T, ACS Symposium Series 121,
American Chemical Society, Washington, DC, 1980, p. 217.
29 Lee Y M and Shim J K, ‘Plasma surface graft of acrylic acid onto porous
poly(vinylidene ﬂuoride) membrane and its riboﬂavin permeation’, J. Appl. Polym.
Sci., 1996, 61, 1245.
30 Mandel M, ‘Energies in a series of oxygen-containing organic molecules of interest
in the study of surface oxidation of polymers’, Eur. Polym. J., 1970, 6, 807.
Mechanical properties of ﬁbre Bragg gratings
XIAOGENG TIAN AND XIAOMING TAO
Self-organized Bragg grating in optical ﬁbres, or changes in refractive index
induced by radiation was ﬁrst observed in 1978. Since permanent Bragg
gratings were ﬁrst written by Meltz et al. in 1989 by the transverse
holographic method, they have attracted great attention in the ﬁelds of
telecommunication, sensing, smart materials and structures. Fibre Bragg
grating (FBG)-based sensors have some distinct advantages. First, they give an
absolute measurement insensitive to any ﬂuctuation in the irradiance of the
illuminating source, as the information is directly obtained by detecting the
wavelength-shift induced by strain or temperature change. Secondly, they can
be written into a ﬁbre without changing the ﬁbre size, making them suitable for
a wide range of situations where small diameter probes are essential, such as in
advanced composite materials, the human body, etc. Thirdly, they can be mass
produced with good repeatability, making them potentially competitive with
traditional strain gauges from the fabrication cost point of view. Finally,
they can be multiplexed in a way similar to methods used on conventional
ﬁbre-optic sensors, such as wavelength-, frequency-, time- and spatial-division-
multiplexing and their combination, making quasi-distributed sensing
feasible in practice.
Because of these advantages, FBGs have been applied as embedded sensors
to monitor or measure the internal strain of composite structures.— Friebele
et al. reported internal distribution strain sensing with ﬁbre grating arrays
embedded in continuous resin transfer moulding2+ (CRTM2+) composites.
Bullock and his colleagues used a translaminar embedded ﬁbre grating
sensor system to monitor the structure of composites. Du et al. embedded
ﬁbre Bragg gratings in a glass woven fabric laminated composite beam for
internal strain measurements. FBGs are also used in mine operating accurate
stability control and medical monitoring.
With FBG sensors being prepared for ﬁeld applications, growing interest is
focused on the mechanical reliability of the ﬁbre gratings. The inﬂuence of
various parameters like humidity, chemical composition of coating,
Mechanical properties of ﬁbre Bragg gratings 125
chemical agent, stripping methods and ﬁbre splicing have been
investigated. At the same time, more than ten diﬀerent models have been
developed to estimate the lifetime from static and dynamic fatigue measurement
under diﬀerent environmental conditions.— In this chapter, we will
examine the inﬂuence of the fabrication procedure and the mechanical
properties of ﬁbre Bragg grating sensors.
8.2 Fabrication techniques
8.2.1 Optical ﬁbres
As shown in Fig. 8.1, an optical ﬁbre consists of a core surrounded by a
cladding whose refractive index is slightly smaller than that of the core. The
optical ﬁbre is coated during the ﬁbre drawing process with a protective layer.
Inside the ﬁbre core, light rays incident on the core-cladding boundary at
angles greater than the critical angle undergo total internal reﬂection and are
guided through the core without refraction. Silica glass is the most common
material for optical ﬁbres, where the cladding is normally made from pure
fused silica, and the core from doped silica containing a few mol % of
germania. Other dopants, such as phosphorus, can also be used. Extra-low
absorption occurs in a germanosilicate ﬁbre, with a local minimum attenuation
coeﬃcient : 0.3 dB/km at 1.3 m and an absolute minimum : 0.16 dB/km
at 1.55 m. Therefore, light in the two windows travels down tens of kilometres
of ﬁbre without strong attenuation in a correctly guided mode condition.
8.2.2 Fibre Bragg gratings
A ﬁbre Bragg grating consists of a modulation in the refractive index, n(z),
along a short length (z) of the core in germania-doped silica ﬁbre with a period
of , which is given by:
n(z) : n ; n · cos[(2 / ) · z ;
where n is the linear refractive index for a guided mode in the ﬁbre core, n is
8.1 Structure of optical ﬁbre.
126 Smart ﬁbres, fabrics and clothing
8.2 The set-up of FBG fabrication.
the modulation amplitude of the refractive index and
is the initial phase of
The inscription of permanent Bragg grating can be achieved in the core of an
optical ﬁbre by interference of two coherent ultra-violet light beams. The
grating thus has a holographically induced refractive index modulation with a
period : /2 sin( /2), where is the angle between the two writing beams
of wavelength . When a broadband light source is coupled into the ﬁbre,
those components with wavelengths that satisfy the Bragg condition are
strongly reﬂected, but all other components pass through the grating with
negligible insertion loss and no change in signal. The central reﬂecting
wavelength, referred to as the Bragg wavelength ( ) of a ﬁbre grating, is
determined by the Bragg condition:
: 2n [8.2]
The central reﬂectivity is given by:
R : tanh( n L/ ) [8.3]
where L is the grating length. The modulation amplitude of the refractive
index, n , represents the grating strength and is dependent on the time of
exposure to UV illumination. The width of the FBG reﬂecting band is
determined by L and n . The higher the values of n and L, the narrower the
Nowadays, the gratings are often fabricated by phase mask technology.
Figure 8.2 shows an experimental set-up for writing Bragg gratings on single
Mechanical properties of ﬁbre Bragg gratings 127
mode germanium-doped silica ﬁbres. The light is spread by using a lens after it
is guided from an ArF excimer laser, then paralleled by passing through a
cylindrical lens and focused on the optical ﬁbre by using another cylindrical
lens, which is normal to the other lens.
8.3 Mechanisms of FBG sensor fabrication
Why can UV irradiation cause a change in the refractive index? To date, there
appear to be three possible mechanisms by which a photo-induced refractive
index change can occur in germanosilica optical ﬁbres: (i) through the
formation of colour centres (GeE), (ii) through densiﬁcation and increase in
tension, and (iii) through formation of GeH. Broadly speaking, all three
mechanisms prevail in germanosilica optical ﬁbres. The relative importance of
each contribution depends on the type of optical ﬁbre and the photosensitization
8.3.1 The formation of colour centres (GeE) and GeH
There are a lot of defects in the germanium-doped core. The paramagnetic
Ge(n) defects, where n refers to the number of next-nearest-neighbour Ge
atoms surrounding a germanium ion with an associate unsatisﬁed single
electron, were ﬁrst identiﬁed by Friebele et al. These defects are shown
schematically in Fig. 8.3.
The Ge(1) and Ge(2) have been identiﬁed as trapped-electron centres. The
characteristic absorption of Ge(1) and Ge(2) are 280 nm and 213 nm. The
GeE, previously known as the Ge(0) and Ge(3) centres, which is common in
oxygen-deﬁcient germania, is a hole trapped next to a germanium at an oxygen
vacancy, and has been shown to be independent of the number of
next-neighbour Ge sites. Here, an oxygen atom is missing from the tetrahedron,
while the germanium atom has an extra electron as a dangling bond. Other
defects include the non-bridging oxygen hole centre (NBOHC), which is
claimed to have absorption at 260 nm and 600 nm, and the peroxy radical,
believed to have absorption at 163 nm and 325 nm. Both are shown in Fig. 8.3.
If the optical ﬁbre is treated with high temperature hydrogen, germania will
decrease and the concentration of GeO molecules will be enhanced. The
reduction process may occur as follows:
Ge O Si + 1/2 H2 Ge + OH Si
Most ﬁbres, if not all, show an increase in the population of the GeE centre
(trapped hole with an oxygen vacancy) after UV exposure. This is formed by
128 Smart ﬁbres, fabrics and clothing
8.3 A schematic of proposed Ge defects of germania-doped silica.
the conversion of the electron-trapped Ge(I) centre, which absorbs at : 5 eV,
and the GeO defect. GeO defect is shown in Fig. 8.4. It has a germanium atom
coordinated with another Si or Ge atom. This bond has the characteristic
240 nm absorption peak that is observed in many germanium-doped
photosensitive optical ﬁbres. On UV illumination, the bond readily breaks,
creating the GeE centre. It is thought that the electron from the GeE centre is
liberated and is free to move within the glass matrix via hopping or tunnelling,
or by two-photon excitation into a conduction band. The change in the
population of the GeE centres causes changes in the UV absorption spectra,
which lead to a change in the refractive index of the ﬁbre at a wavelength
directly through the Kramers—Kronig relationship:
1 H ( ) ·
n: G d [8.4]
(2 ) ( 9 )
where the summation is over discrete wavelength intervals around each of the i
changes in measured absorption, . Therefore, a source of photoinduced
change in the absorption at O O will change the refractive index at
wavelength . This process is common to all ﬁbres. The colour centre model,
originally proposed by Hand and Russel, only explains part of the observed
refractive index changes of : 2 ; 10 in non-hydrogenated optical ﬁbres.
Mechanical properties of ﬁbre Bragg gratings 129
8.4 The capital GeO defect of germania-doped silica, in which the atom
adjacent to germanium is either a silica or another germanium.
For molecular hydrogen, the suggested reaction is the formation of GeH
and OH ions from a Ge(2) defect. The possible route may be as follows:
Ge O Ge + H2 Ge +H O Ge
After the treatment, the concentration of GeE and GeH will increase greatly.
8.3.2 Densiﬁcation and increase in tension
The refractive index of glass depends on the density of the material also,
so that a change in the volume through thermally induced relaxation of the
glass will lead to a change n. The refractive index n is shown as:
n V 3n
: : [8.5]
n V 2
where the volumetric change V as a fraction of the original volume V is
proportional to the fractional change in linear dimension of the glass.
A possible eﬀect of the irradiation is a collapse of a higher-order ring
structure leading to densiﬁcation. The densiﬁcation of silica under UV
irradiation is well documented. The process of densiﬁcation has been shown
to occur in ﬁbres, as evidenced by scans using an atomic force microscope of
the surface of D-shape ﬁbres and in etched ﬁbres, and in preform samples
that were drawn into a D-shaped ﬁbre. These observations are on the surface
of the sample and are unable to replicate the stress proﬁles within the core of
the ﬁbre directly. Direct optical measurement of in-ﬁbre stress has indicated
that, rather than the relief of the stress, tensile stress actually increases with an
associated reduction in the average refractive index by : 30% of the observed
UV induced refractive index change in non-hydrogen loaded, high germania-
130 Smart ﬁbres, fabrics and clothing
content ﬁbre. The changes in the stress proﬁle of the ﬁbre are consistent with
the shift in the Bragg wavelength of a grating during inscription.
8.4 Mechanical properties
Telecommunication optical ﬁbres are made from silica glass with ring
structures of Si—O tetrahedral. Defects or small imperfections which have been
created on the surface of optical ﬁbre during the ﬁbre fabrication processing
lead to a reduced ﬁbre strength. Griﬃth suggested that these defects, called
ﬂaws, act as stress intensiﬁers and cause fracture, when they induce large
enough stress to break chemical bonds mechanically. The stress intensity
factor K at a crack tip as a function of time, t, can be written as:
K (t) : Y (t)( (t) [8.6]
where Y is the dimensionless crack geometry shape parameter which is
assumed to be constant for a given ﬂaw type, is the applied stress and is the
ﬂaw depth, i.e. the ﬂaw size normal to the direction of the applied stress.
When the applied stress, , increases to its allowable maximum given by the
intrinsic strength, S, of the crack, a catastrophic failure occurs. Equation (8.6)
K : YS( [8.7]
K is an intrinsic constant of silica and has been empirically determined to be:
K : 0.79 MPa m.
If n( ) denotes a ﬂaw distribution, then the number of the ﬂaws which will
fail between and ; d is n( )d . The total number of ﬂaws whose strengths
are less than is:
N( ) : n( )d [8.8]
According to the Weibull distribution, the empirical form of the cumulative
ﬂaw distribution is given by:
N( ) : [8.9]
where is the applied stress to the ﬁbre during the fatigue test, m is the scaling
factor and is a constant characteristic of the material. The probability of a
breakage between stress level and ; d is given by the joint probability
that the sample contains a ﬂaw whose strength falls into this interval and that
the sample has survived a stress level :
Mechanical properties of ﬁbre Bragg gratings 131
dF( ) : F( ; d ) 9 F( ) : (1 9 F( ))n( )d [8.10]
F( ), commonly referred to as the cumulative failure probability, is deﬁned as
the probability of breakage below a stress level . Consequently 1 9 F( ) is the
survival probability. Assuming a group of M samples, F( ) is calculated as below:
i 9 0.5
F( ) : i : 1, 2, . . ., M [8.11]
The failure stresses are listed with increasing magnitude as , , . . ., , . . .,
so that the cumulative failure probability F( ) can be determined. In the
Weibull plot, the breaking stress is plotted versus the cumulative failure
probability F. To compare diﬀerent Weibull distributions, we use the median
breaking stress, , which corresponds to 50% failure probability. Combining
Eqs. (8.9) and (8.10) we obtain:
log ln : m log [8.12]
1 9 F( )
The slope of the curve is the Weibull scaling parameter m, which indicates the
shape of the distribution. Low m-values indicate a large range of surface ﬂaw
sizes, while high m-values indicate high surface quality and a close approach to
the tensile strength of a ﬂaw-free ﬁbre under normal condition. m-Values for
pristine ﬁbres are normally of the order of 80—150.
8.4.2 Young’s modulus and hardness
The tensile test can provide information on the average Young’s modulus and
mechanical strength. A nano-indenter can measure the Young’s modulus and
hardness locally on a much smaller scale. Interest in load and displacement-
sensing indentation testing as an experimental tool for measuring elastic
modulus began in the early 1970s. The nano-indenter is made of very hard
material. When it is pressed on the surface of the tested material, deformation
occurs on both the indenter and the tested material; according to the
deformation of the material and the acted force, the material properties, such
as Young’s modulus and hardness, can be obtained.
The eﬀects of the non-rigid indenter on the load-displacement behaviour
can be eﬀectively accounted for by deﬁning a reduced modulus, E , through the
1 19 19
: Q; G [8.13]
E E E
P Q G
where E and are the Young’s modulus and Poisson’s ratio for the indenter
and E and are those of the material being tested. Therefore, the Poisson’s
132 Smart ﬁbres, fabrics and clothing
8.5 A schematic representation of load vs. indenter displacement
showing quantities used in the analysis as well as the graphical
interpretation of the contact depth.
ratio must be estimated for the material being tested to determine the modulus.
Using instrumented microhardness testing machines, the indentation
load-displacement curve can be obtained as shown in Fig. 8.5. They are
analysed according to the equation:
S: : E (A [8.14]
Here, S : dP/dh is the experimentally measured stiﬀness of the upper portion
of the unloading data, E is the reduced modulus (previously deﬁned) and A is
the projected area of the elastic contact.
The contact area at peak load can be determined by the geometry of the
indenter and the depth of contact, h , assuming that the indenter geometry can
be described by an area function G(h) which relates the cross-sectional area of
the indenter to the distance from its tip, h. Given that the indenter does not
itself deform signiﬁcantly, the projected contact area at peak load can then be
computed from the relation A : G(h ). The functional form of G must be
established experimentally prior to analysis.
At any time during loading, the displacement, h, can be written as:
h:h ;h [8.15]
where h is the displacement of the surface at the perimeter of the contact,
which can be ascertained from the load-displacement data. At the peak, the
load and displacement are P and h , respectively. We have h :
the geometrical constant, which relates to the geometry of the indenter. for
diﬀerent geometries of indenter are listed in Table 8.1. The contact depth, h ,
can be expressed as:
h :h 9
Mechanical properties of ﬁbre Bragg gratings 133
Table 8.1 for different shapes of indenter
Indenter indenter pyramid Flat punch
0.72 0.75 1.00
So the contact area, A, can be obtained from Eq. (8.14) and combining it with
Eq. (8.13), Young’s modulus of the tested material can be expressed as:
2 (A 1 9
E : 9 G ·(1 9 ) [8.17]
Q ( S E Q
The data obtained using the current method can be used to determine the
hardness, H. The hardness is deﬁned as the mean pressure the material will
support under load. The hardness is computed from:
8.5 Inﬂuence of the UV-irradiation on mechanical
8.5.1 The inﬂuence on the mechanical strength
126.96.36.199 The mechanical strength of gratings not aﬀected
Although type I grating has a reﬂectivity of only a few per cent, it can easily be
written at any arbitrary position along the ﬁbre. Such FBG arrays are
ideally suited for distributed sensing, where low reﬂectivity is not a major
drawback. Askins et al. and Hagemann et al. have studied the mechanical
strength of optical ﬁbre containing FBG fabricated in this method. In their
experiment, laser exposures occurred only immediately before the protective
jacketing was applied during ﬁbre drawing.
FBG sensors produced on-line during the process using an excimer laser
pulse suﬀer no measurable loss of strength relative to unirradiated ﬁbre. This
emphasizes the fact that it is favourable to use draw-tower FBGs as sensor
elements to overcome the problem related to ﬁbre stripping and high ﬂuence
188.8.131.52 Mechanical strength degradation of gratings
Feced et al. has studied the inﬂuence of diﬀerent wavelength UV irradiation
on the strength of optical ﬁbres with a single pulse radiation. The single mode
optical ﬁbres used in their investigations were Corning’s SMF-28 ( : 3 mol %
of germanium), and a highly photosensitive germanium and boron (Ge—B)
co-doped ﬁbre (10 mol % of germanium) from the University of Southampton.
Their results suggest that the fabrication of Bragg gratings using 193 nm
irradiation will yield higher-strength gratings with enhanced reliability. A
similar analysis shows that the diﬀerence in strength between Ge—B doped
ﬁbre and SMF-28 when exposed to 248 nm radiation is signiﬁcantly higher.
It has previously been reported that the processes induced in the ﬁbre by
248 nm radiation are diﬀerent from those induced by 193 nm radiation. In
addition, it is thought that the exposure of optical ﬁbre to UV increases the
stress in the core. The results reinforce these concepts; they suggest that the
248 nm mechanism increases the internal core stress of the ﬁbre signiﬁcantly
more than the 193 nm mechanism, such that 248 nm radiation causes a larger
degradation of the ﬁbre strength.
We have tested the fracture strength of FBG sensors fabricated by ourselves.
In order to eliminate the mechanical strength degradation of the coating
stripping, we decoated the coating of the ﬁbre with acetone prior to UV laser
exposure. The UV radiation was a laser operating at 193 nm. The light
focused with a cylindrical lens then passed through a phase mask before
irradiating the ﬁbre. The frequency of the UV irradiation is 5 Hz.
Figure 8.6 shows the mechanical strength and the reﬂectivity of the FBG
sensors. In the fracture strength test, the length of the gauge is 0.25 m and the
strain rate is 1 mm/min. It can be seen that the mechanical strength of the
Mechanical properties of ﬁbre Bragg gratings 135
8.7 SEM of the cross-section of the broken grating. The start of the break
is at the lower side. The UV laser is radiated from bottom to top.
FBG sensor degraded drastically with the increase in UV irradiation, and
after a certain dose the mechanical strength will not degrade with the growth
of UV irradiation. The strength of the FBG sensor is only about one-third of
the optical ﬁbre without UV irradiation. We can also see that the reﬂectivity
increases sharply once the reﬂected peak appears, and then ﬂattens as the UV
irradiation increases. The strength degradation has been completed even
before the reﬂected peak appears in our experiment, as if there were an
obvious relation between the strength degradation and the reﬂectivity of the
The SEM of the cross-section of the broken FBG sensor is shown in Fig.
8.7. The UV light irradiated the optical ﬁbre from bottom to top. The
beginning of the fracture was not always at the UV irradiation side, and the
lateral side of optical ﬁbre with UV irradiation was observed carefully with
SEM; no ﬂaw could be seen. This means the mechanical strength degradation
takes place not only because of the ﬂaws on the ﬁbre surface induced by UV
radiation. The mechanism of the mechanical strength degradation of the
FBGs is not clear. Possibly, it is related to the structural change of the optical
ﬁbre molecule after UV irradiation.
Figure 8.8 is the comparison of the strength degradation with diﬀerent
irradiation energy/pulse at the same frequency. The strength degradation is
larger with higher irradiation energy/pulse than with lower energy/pulse. This
means that, in order to increase the mechanical strength of the FBGs, the
136 Smart ﬁbres, fabrics and clothing
Broken stress (GPa)
0 5 10 15 20 25 30 35
Total irradiation dose (mJ/cm )
8.8 Strength degradation with different energy/pulse: —— lower energy
per pulse, · · ·
· · · higher energy per pulse.
irradiation energy/pulse should be lowered. We also observed that, not only
does the reﬂectivity increase slowly with the growth of the total dose of UV
irradiation after certain reﬂectivity (99%), but also the line-width of the
reﬂected peak gets wider. The wide reﬂected peak is disadvantageous for the
accuracy of the test. Thus, in FBG fabrication, the UV irradiation time should
not be too long.
Because FBG fabrication is a complex procedure and glass ﬁbre is brittle,
the mechanical strength degradation is related not only to the UV irradiation
but also to the coating stripping method. We have stripped coating with
diﬀerent methods in our FBG fabrication and compared their inﬂuence on the
mechanical strength of the optical ﬁbre. Optical ﬁbres were divided into two
groups, each with 20 samples. One group had the coating stripped with
acetone, and the other with sulfuric acid. Coating stripped with acetone was a
physical procedure. The stripped part of the optical ﬁbre was soaked into
acetone for several minutes, the acetone caused the costing to soften and swell;
the coating then separated from the cladding. The coating can be pulled oﬀ
gently. When the optical ﬁbre was immersed in sulfuric acid (98%) at room
temperature ( : 20 °C), the coating was ablated by sulfuric acid, which took
about 5 minutes. The optical ﬁbre was then rinsed in water to remove the
residual acid and other materials. No mechanical shock occurred to ﬁbres in
these two coating stripping procedures. The mechanical fracture during stripping
was reduced to as little as possible. The mechanical strength of these stripped
Mechanical properties of ﬁbre Bragg gratings 137
1 F( )
0 1 4
Broken stress (GPa)
8.9 Weibull plot of optical ﬁbre with different coating stripping method.
— pristine ﬁbre, —— decoated with acetone, —s— decoated with
1 F( )
Broken stress (GPa)
8.10 Inﬂuence of UV irradiation frequency on mechanical strength of
FBGs. —— 26 kV, 5 Hz, —
— 26 kV, 8 Hz.
optical ﬁbres was tested. The Weibull plot is shown in Fig. 8.9. Table 8.2 gives
the parameters for the distribution. The mechanical strength degraded notably
when the coating was stripped with acetone. This may be related to the
properties of these two solvents.
We have also compared the mechanical strength of FBGs fabricated with
diﬀerent frequencies of UV irradiation. The energy per pulse was the same
138 Smart ﬁbres, fabrics and clothing
Table 8.2 Mechanical strength of optical ﬁbre with different stripping method
Stripped with Stripped with
acetone sulfuric acid Pristine ﬁbre
Mean of broken stress 1.14 1.76 4.09
Median stress 1.16 1.67 4.09
m value 2.8 2.8 52.0
Table 8.3 The inﬂuence of UV irradiation frequency
irradiation 5 Hz 8 Hz
Mean of broken stress 1.76 0.47 0.63
Median stress 1.67 0.44 0.55
m value 2.8 4.0 4.1
Coating stripped with H2SO4.
with diﬀerent frequencies. Figure 8.10 is the Weibull plot of FBGs with
diﬀerent UV irradiation. We can ascertain that the mechanical strength
degradation is larger with lower frequency irradiation. As shown in Table 8.3,
the m-values are almost the same in both situations and, obviously, the
median broken strength of gratings with 8 Hz irradiation is higher than that of
gratings fabricated with 5 Hz irradiation. This may be because irradiation
with high frequency can increase the surface temperature of the ﬁbre, resulting
in the thermal annealing of some of the ﬂaws produced in the ﬁrst phase,
thereby increasing the median break stress of the ﬁbre.
We have also studied the inﬂuence of spot size on the mechanical strength.
In FBG fabrication, we have found that when UV lasers pass through the
phase mask, the density of light is not uniform. There was a notable change in
the area of the edge of the phase mask. We have fabricated FBGs under
diﬀerent fabrication conditions and compared their mechanical strength.
Group 1 was fabricated under normal fabrication conditions. The spot size is
27 mm ; 1 mm. When Group 2 was fabricated, part of the UV light was
covered so that the spot size was only within the mask area. The spot size was
9 mm ; 1 mm. The edge eﬀect of the phase mask was avoided. The Weibull
plot of the FBG is shown in Fig. 8.11.
Mechanical properties of ﬁbre Bragg gratings 139
1 F( )
Broken stress (GPa)
8.11 Weibull plot of FBGs with different spot size during fabrication:
—— 27 mm ; 1 mm, —s— 9 mm ; 1 mm.
184.108.40.206 Enhancing the mechanical performance of FBG sensors
Because the strength degradation of the FBG sensors has important conse-
quences for the reliability of the UV-induced Bragg gratings which are used as
strain, temperature, and pressure sensors in a variety of ﬁelds, Varelas et
al. have examined the inﬂuence of homogeneous irradiation, using a
continuous wave (CW) laser in the mechanical degradation of the ﬁbre and
compared it with the equivalent irradiation dose delivered by a pulsed laser
source. Imamura et al. have developed a new method for fabricating Bragg
gratings with direct writing. The strength of Bragg gratings has been enhanced
CW laser irradiation results in the mechanical resistance of a ﬁbre being
similar to that of a pristine ﬁbre. This is in contrast to the case where the ﬁbre
undergoes pulse excimer irradiation. The total dose dependence is also less
pronounced in the case of CW irradiation. This phenomenon has important
consequences for Bragg grating fabrication, where high mechanical resistance
is required for strain applications.
Although high strength Bragg gratings with higher reﬂectivity can be
fabricated by CW UV exposure after chemical stripping of the protective
polymer coating, this is not practical as it requires recoating and packaging. It
has the potential for reducing the ﬁbre strength due to exposure of the bare
ﬁbre to air. A direct ﬁbre Bragg grating writing method through the coating
has been demonstrated. Imamura et al. directly fabricated ﬁbre gratings
through the coating and have succeeded in producing a high strength ﬁbre
140 Smart ﬁbres, fabrics and clothing
Young’s modulus (GPa)
irradiation without Grating
0 10 20 30 40 50 60
8.12 Young’s modulus of the optical ﬁbre.
grating. Tin-codoped germanosilicate ﬁbre is more photosensitive than
germanium-doped ﬁbre. The germanosilicate single mode ﬁbre was codoped
with 15 000 ppm Sn and 900 ppm Al in the core. To further enhance the ﬁbre
sensitivity, the ﬁbres were treated under low temperature hydrogen for 2
weeks at 20 MPa prior to the UV exposure. The silica cladding had a diameter
of 125 m and was single coated with a UV-transparent UV-curable resin to
an outer diameter of 200 m.
8.5.2 Inﬂuence of UV irradiation on Young’s modulus and
hardness of ﬁbre
The inﬂuence of UV irradiation on the mechanical strength of optical ﬁbres is
notable. How about the inﬂuence of UV irradiation to the other mechanical
properties of optical ﬁbres? Young’s modulus and hardness of the optical ﬁbre
with and without UV irradiation have been tested using the Nano Indenter IIp.
In the test, the surface of the sample should be a smooth plane. The optical
ﬁbre is so thin that the lateral side has a large curvature. In order to get a plane
in the lateral side of the optical ﬁbre, the tested ﬁbres were put into a polymer,
then the polymer was polished carefully with lapping ﬁlm (0.2 m) so that a
very smooth plane along the ﬁbre was obtained. The sample contained three
parts: optical ﬁbre without UV irradiation, with UV irradiation but without
phase mask, and grating. The result of Young’s modulus of the cladding is
Mechanical properties of ﬁbre Bragg gratings 141
Without UV irradiation
irradiation without Grating
0 10 20 30 40 50 60
8.13 Hardness of the optical ﬁbre.
shown in Fig. 8.12. There is no notable diﬀerence between the three parts.
Statistical analysis was performed. Suppose the measured data belong to
normal distribution, with a 95% conﬁdence level, the conﬁdence interval of
three parts are 71.29 GPa : : 75.30 GPa, 66.00 GPa : : 77.97 GPa and
73.28 GPa : : 76.76 GPa, respectively to optical ﬁbre without UV irradiation,
with UV irradiation without phase mask, and grating. They are almost in the
same range. That is to say, the UV irradiation cannot inﬂuence Young’s
modulus of the optical ﬁbre. Figure 8.13 is the hardness of the optical ﬁbre. The
UV irradiation cannot inﬂuence the hardness of the optical ﬁbre either.
Changing the depth of the plane (by polishing the tested ﬁbre so that the test
plane is closer to the core of the ﬁbre), the results are the same.
From the experiment above we can conﬁrm that it is reasonable to assume
that the deformation of optical ﬁbre contains uniform Bragg grating during
the tension and the strain measured is believable.
8.6 Polymeric ﬁbre
8.6.1 Properties of polymer optical ﬁbre
Polymer optical ﬁbre (POF) is a circular optical waveguide. POF is receiving
increasing interest in short-distance communication systems because of its
large power-carrying capacity, ease of joining and light weight. The structure
142 Smart ﬁbres, fabrics and clothing
0 2 4 6 8
8.14 Extension properties of plastic optical ﬁbre with ten cycles.
of POF is as the same as silica optical ﬁbre. It consists of a central part, the
core, with refractive index n and of cylindrical shape, surrounded by a second
part, the cladding, with a lower refractive index n . These two areas, which are
essential for the light guiding, are composed of two diﬀerent but transparent
organic materials. In order to avoid external damage or the deterioration of
this surface during the handling or use of the optical ﬁbre, it is often covered
with a protective coating which plays no part in the light guiding.
The core diameter varies according to the type of ﬁbre, but is of the order of
a millimetre, except in special cases. For economic reasons, the thickness of the
cladding is much less, of the order of tens of micrometres. The surface of the
core/cladding separation must be as even as possible.
A possible classiﬁcation of POF can be based on the principal core material.
The principal types of POF are ﬁbres with PMMA (polymethyl methacrylate)
core, ﬁbres with PS (polystyrene) core, ﬁbres with PC (polycarbonate) core
and ﬁbres with deuterated core.
Physical properties, such as tensile resistance, compression resistance,
shock resistance, torsion resistance, the eﬀect of permanent winding, bending
resistance, etc., temperature property and the chemical properties of POF
have been studied systematically.
220.127.116.11 The mechanical property
Figure 8.14 shows the elongation property of the measured ﬁbre. In the
measurement, the gauge length was 100 mm. The measurement was controlled
by a programme, in which ten cycles were set. Each cycle contained loading
and unloading; the speed was 0.5 mm/min. The elongation of the cycles was
Mechanical properties of ﬁbre Bragg gratings 143
8.15 DSC of the sample of the plastic optical ﬁbre.
0.5%, 1.0%, 1.25%, 1.5%, 1.75%, 2%, 2.5%, 3.5%, 5% and 8%, respectively.
In this ﬁgure, the unloading curves were not the same as the loading curves.
Like plastic material, the ﬁbre has the hysteresis property. In the meantime,
we ﬁnd that, if the elongation of the ﬁbre is larger than 1.5%, the sample
cannot return to its original length even when the external force is released:
this means that permanent deformation was induced in the sample. Sonic
modulus was measured as 6.3 GPa.
18.104.22.168 DSC results
The heat ﬂow to a sample can be measured in thermally controlled conditions
with diﬀerential scanning calorimetry (DSC) by Mettler TA4000 Thermal
Analysis System. The DSC measurement result is shown in Fig. 8.15. At
67.5 °C, some physical properties of the ﬁbre were changed. This temperature
is called the glass transition temperature. At 330 °C, the ﬁbre began to melt. At
384.3 °C, the ﬁbre began to be oxygenated, and it was completely oxygenated
at 456.9 °C.
8.6.2 Bragg grating of polymer optical ﬁbre
Although silica optical ﬁbre Bragg gratings can be used to measure many
physical parameters, the changes in the Bragg wavelength due to the change of
these measured values are small. The measured range is limited, typically a few
nanometres. This is because silica glass has a small thermal eﬀect and large
Young’s modulus. In the case of polymer optical ﬁbre, the situation is diﬀerent.
Its Young’s modulus (1 GPa), for example, is more than 70 times smaller than
that of glass (72.9 GPa), and its elongation is much larger than that of glass
144 Smart ﬁbres, fabrics and clothing
optical ﬁbre. The refractive index changes that can be induced by photoreaction
are relatively high ( n : 10). Therefore, it is expected that a Bragg grating
written into a polymer optical ﬁbre would be tunable over a very wide
wavelength range. In addition, polymer optical ﬁbre gratings are ideal devices
for inclusion in an organic solid-state ﬁbre laser, which in turn provides a
compact and low-cost optical source over a broad range of wavelengths
throughout the visible spectrum.
Xiong et al. have fabricated a photosensitive polymer optical ﬁbre, whose
refractive index in the core region can be changed under irradiation from a
pulse UV laser beam, and have shown that it is possible to write gratings in
these ﬁbres. They have fabricated several types of grating, including surface
gratings on the ﬂat surface of a preform, gratings in preform core, and gratings
in the core of a multimode polymer optical ﬁbre.
The polymer preform was prepared according to the method reported in
Peng et al., except that the core monomer used contained a much lower level
of lauryl peroxide and chain transfer agent so as to increase its photosensitivity.
The preform was then cut into a square block with the core exposed and
polished. A grating was fabricated by means of a phase mask with a period of
1.06 m. The illumination period was 10 ns, and the pulse energy was about
5 mJ. The grating created at wavelength 248 nm was a surface grating formed
by period removal of the core polymer. An atomic force microscope (AFM)
was used to obtained a surface proﬁle which has a grating period of 1.06 m,
coinciding with that of the pulse mask. The diﬀraction eﬃciency is 15%.
The mechanisms responsible for the formation of periodic structures in
polymers have been explained.— They can be classiﬁed into photolysis,
oxidization and laser ablation for the surface relief gratings, while chain
scission, cross-link and photopolymerization are considered to be responsible
for bulk or volume gratings and in-ﬁbre gratings. The cross-link in Bragg
grating fabrication can be shown as:
[ H2 C C ] [ H2 C C ]
CH CH2 M H2 C HC
Peng et al. have written Bragg gratings in single-mode polymer optical
ﬁbre and have shown that these gratings can be readily tuned over a
wavelength range of 12 nm without changing their reﬂection spectra.
Mechanical properties of ﬁbre Bragg gratings 145
The mechanism and procedure of FBG fabrication are discussed, and the
inﬂuences of UV irradiation on the mechanical strength of optical ﬁbres are
studied. The mechanical strength of optical ﬁbres is unaﬀected by the on-line
writing of a single pulse during ﬁbre drawing. The strength degrades
drastically with UV irradiation after the coating is stripped, and will degrade
further with 248 nm single pulse UV irradiation than with 193 nm. The
strength degradation is more serious with higher radiation energy per pulse
than lower radiation energy. Lower UV irradiation frequency degrades the
mechanical strength more than higher frequency. The mechanical strength of
the optical ﬁbre will not be lowered signiﬁcantly after certain doses of UV
irradiation. The mechanical strength of the FBG sensor can be increased
notably with CW UV irradiation and the direct writing method without
stripping the coating. Young’s modulus and the hardness of the optical ﬁbre
will not change with UV irradiation.
Because of its large elongation property and relatively high refractive index
changes induced by photoreaction, a Bragg grating written into a plastic
optical ﬁbre would be tunable over a very wide wavelength range. Plastic
FBGs can be used to measure large strain and other physical properties with a
large change range of structures.
The authors wish to acknowledge Hong Kong Research Grants Council for
supporting this work (Grant No Polyu5112/98E) and Dr Dongxiao Yang for
conducting the measurement of PMMA optical ﬁbres.
1 Hill K, Fujii Y, Johnson D C and Kawasaki B S, ‘Photosensitivity in optical ﬁbre
wave guide applications to reﬂection ﬁlter fabrication’, Appl. Phys. Lett., 1978, 32,
2 Kawasaki B S, Hill K O, Johnson C D and Fujii Y, ‘Narrow-band Bragg reﬂectors
in optical ﬁbres’, Opt. Lett., 1978, 3, 66—8.
3 Meltz G, Morey W W and Glenn W H, ‘Forming of Bragg grating in optical ﬁbres
by a transverse holographic method’, Opt. Lett., 1989, 14, 823—5.
4 Askins C C, Putnam M A, Williams G M and Friebele E J, ‘Stepped-wavelength
optical-ﬁbre Bragg grating arrays fabricated in line on a draw tower’, Opt. Lett.,
1994, 14, 823—4.
5 Archambault J L, Reekie L and Russell, ‘High reﬂectivity and narrow bandwidth
ﬁbre grating written by single excimer pulse’, Electron. Lett., 1993, 29, 28—9.
146 Smart ﬁbres, fabrics and clothing
6 Kersey A D, ‘Interrogation and multiplexing techniques for ﬁbre Bragg grating
strain-sensors’, Proc. SPIE, 1993, 2071, 30—48.
7 Rao Y J, ‘In ﬁbre Bragg grating sensors’, Meas. Sci. Technol., 1997, 8, 355—75.
8 Mather M H, Tabrizi K, Prohaska J D and Snitzer E, ‘Fibre Bragg gratings for civil
engineering applications’, Proc. SPIE, 1996, 2682, 298—302.
9 Friebele E J, Askins C G, Putnam M A et al., ‘Distributed strain sensing with ﬁbre
Bragg grating arrays embedded in CRTM2+ composite’, Electron. Lett., 1994, 30,
10 Friebele E J, Askins C G, Putnam M A et al., ‘Demonstration of distributed strain
sensing in production scale instrumented structures’, Proc. SPIE, 1996, 2721, 118—24.
11 Bullock D E, Dunphy J R, Hufstetler G H, ‘Embedded Bragg grating ﬁbre optic
sensor for composite ﬂexbeams’, Proc. SPIE, 1993, 1789, 253—61.
12 Chen B X, Mather M H and Nawy E G, ‘Fibre-optic Bragg grating sensor for
nondestructive evaluation of composite beam’, J. Struct. Eng., 1994, 12(12), 3456—70.
13 Measures R M, Alavie A T, Maaskant R, Ohn M, Karr S and Huang S, ‘Structurally
integrated Bragg grating laser sensing system for a carbon ﬁbre pre-stressed
concrete highway bridge’, Smart Mater. Struct., 1995, 4(1), 20—30.
14 Du W C, Tao X M, Tam H Y and Choy C L, ‘Optical Bragg grating sensors in smart
textile structural composite’, Proceeding of the 4th International Conference on
Composite Engineering, ICCE/4, Hawaii, USA, 1997, 289—90.
15 Ferdinand P, Ferragu O, Lechien J L et al. ‘Mine operating accurate stability
control with optical ﬁbre sensing and Bragg grating technology: the European
brite/euram stabilos project’, J. Lightwave Technol., 1995, 13, 1303—12.
16 Rao Y J, Jackson D A, Zhang L and Bennion I, ‘In-ﬁbre Bragg grating temperature
sensor system for medical applications’, J. Lightwave Technol., 1997, 15, 779—85.
17 Griﬃoen W, ‘Mechanical life time model for optical ﬁbre in water’, Proc. SPIE,
1994, 2074, 2—10.
18 Haslove P, Jensen K B and Skovgaard N H, ‘Degradation of stressed optical ﬁbres
in water: new worst case lifetime estimation model’, J. Am. Ceram. Soc., 1994, 77,
19 Bouten P C P and Broer D J, ‘Coating composition and ﬁbre life time’, Proc. SPIE,
1994, 2074, 59—64.
20 Inniss D, Brownlow D L and Kurkjian C R, ‘Chemical eﬀects on the fatigue of
light-guide ﬁbres’, Proc. SPIE, 1992, 1791, 3—10.
21 Wei T, Yuee H H, Hasz C H and Key P L, ‘Degradation of ﬁbre strength during
coating stripping’, Int. Wire and Cable Symp. Proc., 1989, 199—204.
22 Rondinella V V and Matthewson M J, ‘Eﬀect of chemical stripping on the strength
and surface morphology of fused silica ﬁbre’, Proc. SPIE, 1994, 2074, 52—8.
23 Damsgaard H and Hansen O, ‘Factory spliced ﬁbres: technology, performance and
ﬁeld experience’, Int. Wire and Cable Symp. Proc., 1990, 284—90.
24 Olshansky R and Maurer D R, ‘Tensile strength and fatigue of optical ﬁbres’, J.
Appl. Phys., 1976, 47(10), 4497—9.
25 Mitsunaga Y, Katsuyama Y and Ishida Y, ‘Reliability assurance for long-length
optical ﬁbre based on proof testing’, Electron. Lett., 1981, 17, 568—71.
26 Griﬃoen W, Breuls T, Cocito G, Dodd S, Ferri G, Haslov P, Oksanen L, Stockon D
and Svensson T, ‘COST 218 evaluation of optical ﬁbre lifetime models’, Proc. SPIE,
1992, 1791, 190—5.
Mechanical properties of ﬁbre Bragg gratings 147
27 Friebele E J, Griscom D L and Siegal G H Jr, ‘Defect centers in germania doped
silica optical ﬁbre’, J. Appl. Phys., 1974, 45, 3424—8.
28 Kawazoe H, ‘Eﬀects of modes of glass formation on the structure of intrinsic or
photoinduced defects centered on III, IV, or V cations in oxide glasses’, J. Non-cryst.
Solids, 1985, 71, 213—34.
29 Tsai T E, Griscom D L, Friebele E J and Fleming J W, ‘Radiation induced defect
centers in high purity GeO glass’, J. Appl. Phys., 1987, 62, 2262—8.
30 Griscom D L and Mizuguchi M, ‘Determination of the visible range optical
absorption spectrum of peroxy radicals in gamma irradiation fused silica’. In Bragg
Gratings, Photosensitivity and Poling in Glass Fibres and Waveguides: Fundamentals
and Applications, 1997 OSA Technical Digest Series, 17, Paper JMD2, 139—41.
31 Honso H, Abe Y, Kinser D L, Weeks R A, Muta K and Kawazoe H, ‘Nature and
origin of the 5eV band in SiO : GeO glasses’, Phys. Rev. B, 1995, 46, II-445—II-451.
32 Tsai T E and Friebele E J, ‘Kinetics of defects centers formation in Ge—SiO ﬁbre of
various compositions’. In Bragg Gratings, Photosensitivity and Poling in Glass
Fibres and Waveguides: Fundamentals and Applications, 1997, OSA Technical
Digest Series, 17, Paper JMD2, 101—3.
33 Hand D P and Russel P St J, ‘Photoinduced refractive index changes in
germanosilicate optical ﬁbres’, Opt. Lett., 1990, 15(2), 102—4.
34 Williams D L, Davey S T, Kashyap R, Armitage J R and Ainslie B J, ‘Direct
observation of UV-induced bleaching of 240 nm absorption band in photosensitive
germanosilicate glass ﬁbres’, Electron. Lett., 1992, 28(4), 369—71.
35 Riant I, Borne S and Sansonetti P, ‘Evidence of densiﬁcation in UV-write Bragg
gratings in ﬁbres’. In Photosensitivity and Quadratic Nonlinearity in Waveguides:
Fundamentals and Applications, 1995, 22, 51—5.
36 Poumellec B, Guenot P, Riant I et al., ‘UV induced densiﬁcation during Bragg
grating inscription in Ge : SiO preforms’, Opt. Mater., 1995, 4, 441—9.
37 Bernardin J P and Lawandy N M, ‘Dynamics of the formation of Bragg gratings in
germanosilicate optical ﬁbres’, Opt. Commun., 1990, 79, 194—8.
38 Rothschild M, Erlich D J and Shaver D C, ‘Eﬀects of excimer irradiation on the
transmission, index of refraction, and density of ultraviolet grade fused silica’, Appl.
Phys. Lett., 1989, 55(13), 1276—8.
39 Douay M, Ramecourt D, Tanuay T et al. ‘Microscopic investigations of Bragg
gratings photo-written in germanosillicate ﬁbres’. In Photosensitive and Quadratic
Nonlinearity in Waveguides: Fundamentals and Applications, 1995, OSA Technical
Digest Series, 22, 48—51.
40 Fonjallaz P Y, Limberger H G, Salathe, Cochet F and Leuenberger B, ‘Tension
increase correlated to refractive index change in ﬁbres containing UV written Bragg
gratings’, Opt. Lett., 1995, 20(1), 1346—8.
41 Griﬃth A A, ‘The phenomena of rupture and ﬂaw in solids’, Phil. Trans. Roy. Soc.,
1920, 221A, 163—9.
42 Kurkjian C R and Paek U C, ‘Single value strength of perfect silica ﬁbres’, Appl.
Phys. Lett., 1983, 42, 251—3.
43 Oliver W C and Pharr G M, ‘An improved technique for determining hardness and
elastic modulus using load and displacement sensing indentation experiments’, J.
Mater. Res., 1992, 7(6), 1564—83.
44 Sneddon I N, ‘The relation between load and penetration in the axisymmetric
148 Smart ﬁbres, fabrics and clothing
boussinesq problem for a punch of arbitrary proﬁle’, Int. J. Engng. Sci., 1965, 3, 47—57.
45 Askins C G, Putnam M A, Williams G M and Friebele E J, ‘Stepped-wavelength
optical ﬁbre Bragg grating arrays fabricated in line on a draw tower’, Opt. Lett.,
1994, 19(2), 147—9.
46 Askins C G, Putnam H J, Patrick H J and Friebele E J, ‘Fibre strength unaﬀected by
on-line writing of single-pulse Bragg grating’, Electron. Lett., 1997, 33(15), 1333—4.
47 Hagemann V, Trutzel M N, Staudigel L, Rothhardt M, Muller H-R and
Krumpholz O, ‘Mechanical resistance of draw-tower-Bragg grating sensors’,
Electron. Lett., 1998, 34(2), 211—12.
48 Feced R, Roe-Edwards M P, Kanellopoulos S E, Taylor N H and Handerick V A,
‘Mechanical strength degration of UV exposed optical ﬁbres’, Electron Lett., 1997,
49 Albert J, Malo B, Hill K O, Bilodeau F, Johnson D C and Theriault S, ‘Comparison
of one-photon and two-photon eﬀects in photosensitivity of germanium-doped
silica optical ﬁbres exposed to intense ArF excimer laser pulses’, Appl. Phys. Lett.,
1995, 67(24), 3529—31.
50 Varelas D, Limberger H G, Salathe R P and Kotrotsios C, ‘UV-induced mechanical
degradation of optical ﬁbres’, Electron. Lett., 1997, 33(9), 804—5.
51 Varelas D, Limberger H G and Salathe R P, ‘Enhanced mechanical performance of
single mode optical ﬁbres irradiated by a CW UV laser’, Electron. Lett., 1997, 33(8),
52 Imamura K, Nakai T, Moriura K, Sudo Y and Imada Y, ‘Mechanical strength
characteristics of tin-codoped germanosilicate ﬁbre Bragg gratings fabricated by
writing through UV-transparent coating’, Electron. Lett., 1998, 34(10), 1016—17.
53 Chao L, Reekie L and Ibsen M, ‘Grating writing through ﬁbre coating at 244 and
248 nm’, Electron. Lett., 1999, 35(11), 924—5.
54 Imamura K, Nakai T, Sudo Y and Imada Y, ‘High reliability of tin-codoped
germanosilicate ﬁbre Bragg gratings fabricated by direct writing method’, Electron.
Lett., 1998, 34(18), 1772—4.
55 Dong L, Cruz J L, Reekie L, Xu M G and Payne D N, ‘Enhanced photosensitivity in
tin-codoped germansilicate optical ﬁbres’, IEEE Photon. Technol. Lett., 1995, 7,
56 Sanders D H, Statistics: A Fresh Approach, McGraw-Hill, Inc., 1990.
57 Marcou J (ed.), Plastic Optical Fibres: Practices and Applications, John Wiley, New
58 Hill K O and Meltz G, ‘Fibre Bragg grating technology fundamental and overview’,
J. Lightwave Technol., 1997, 15(8), 1263—76.
59 Kaminov I P, Weber H P and Chandross E A, ‘Poly(methyl methacrylate) dye laser
with internal diﬀraction grating resonator’, Appl. Phys. Lett., 1971, 18, 497—9.
60 Dodabalapur A, Chandross E A, Berggren M and Slusher R E, ‘Organic solid-state
lasers: past and future’, Science, 1997, 277, 1787—8.
61 Peng G D, Xiong Z and Chu P L, ‘Photosensitivity and gratings in dye-doped
polymer optical ﬁbres’, Optical Fibre Technol., 1999, 5(2), 242—51.
62 Peng G D, Chu P L, Xiong Z, Whitbread T and Chaplin R P, ‘Dye-doped
step-index polymer optical for broadband optical ampliﬁcation’, J. Lightwave
Technol., 1996, 14, 2215—23.
63 Tomlinson W J, Kaminow I P, Chandross A, Fork R L, and Silfvast W T,
Mechanical properties of ﬁbre Bragg gratings 149
‘Photoinduced refractive index increase in poly(methylmethacrylate) and its
applications’, Appl. Phys. Lett., 1970, 16, 486—9.
64 Bolle M, Lazare S, Blanc M L and Wilmes A, ‘Submicron periodic structures
produced on polymer surfaces with polarized excimer laser ultraviolet radiation’,
Appl. Phys. Lett., 1992, 60, 674—6.
65 Decker C, ‘The use of UV irradiation in polymerization’, Polymer Int., 1998, 45, 133—7.
66 Xiong Z, Peng G D, Wu B and Chu P L, ‘Highly tunable Bragg gratings in
single-mode polymer optical ﬁbres’, IEEE Photon. Technol. Lett., 1999, 11(3), 352—4.
Optical responses of FBG sensors
DONGXIAO YANG, XIAOMING TAO AND
Many sensors— can be used to measure the strain and deformations, such as
traditional strain-meter sensors, piezoelectric sensors, piezo-resistive sensors,
optic sensors based on ﬂuorescence spectroscopy or Raman spectroscopy,
ﬁbre optic sensors based on Brillouin scattering, ﬁbre optic sensors based on
interferometer or/and polarimeter, ﬁbre optic sensors based on photography
and ﬁbre Bragg grating (FBG) sensors. FBG sensors have been considered
excellent sensing elements, suitable for measuring static and dynamic ﬁelds,
like temperature, strain and pressure. Since the measured information is
wavelength encoded,— FBG makes the sensor self-referencing, rendering it
independent of ﬂuctuating light levels and the system immune to source power
and connector losses that plague many other types of ﬁbre optic sensors. The
advantages of FBG sensors include light weight, ﬂexibility, stability, potential
low cost, longer lifetime, higher temperature capacity, unique wavelength-
multiplexing capacity, suitable size for embedding into composites without
introducing signiﬁcant perturbation to the characteristics of the structure,
good invulnerability to electro-magnetic interference, and even durability
against high radiation environments, making reproducible measurements
possible. Therefore, FBG sensors seem to be ideal for realizing ﬁbre optic
smart structures where sensors are embedded in or attached to structures for
achieving a number of technical objectives, such as health monitoring, impact
detection, shape control and vibration damping, via the provision of real-time
sensing information, such as strain, temperature and vibration. FBG sensors
have been used for measurements of a wide variety of parameters: some FBG
sensor systems have been installed in large-scale practical applications, and
some are commercially available. FBG sensors have been used in bridges,
highways, textiles, mines, marine vehicles, medical therapies and aircrafts.—
They— can be used for quasi-static strain monitoring, dynamic strain
sensing, time- and wavelength-division multiplexing, and temperature/strain
Optical responses of FBG sensors under deformations 151
discrimination. The combination of FBG and long period ﬁbre grating can be
used to simultaneously determine strain and temperature. FBGs can also be
used in laser sensors and interferometer sensors.
Most of the sensing applications of FBG sensors focus on its reﬂection
spectra, which depend on the relationship between the Bragg wavelength of
FBG and its physical quantities. The key detection issue is the determination
of the often small measurand-induced Bragg wavelength shift. In addition to
ﬁbre grating spectra, the polarization optics of FBG sensors will also be
discussed in this chapter. The contents include optical methodologies, optical
responses under tension, torsion, lateral compression and bending.
9.2 Optical methodology for FBG sensors
An optical ﬁbre is a cylindrical dielectric waveguide made of low-loss materials
such as silica glass. It has a central core in which the light is guided, embedded
in an outer cladding of slightly lower refractive index. Light rays incident on
the core-cladding boundary at angles greater than the critical angle undergo
total internal reﬂection and are guided through the core without refraction.
Rays of greater inclination to the ﬁbre axis lose part of their power into the
cladding at each reﬂection and are not guided.
Light in ﬁbre propagates in the form of modes. In mathematics, a mode in
optic ﬁbre is a solution of the Maxwell’s equations under the boundary
conditions. The guided modes are electric and magnetic ﬁelds that maintain
the same transverse distribution and polarization at all distances along the
ﬁbre axis. Each mode travels along the axis of the ﬁbre with a distinct
propagation constant and group velocity, maintaining its transverse spatial
distribution and its polarization. There are two independent conﬁgurations of
electric and magnetic vectors for each mode, corresponding to two states of
polarization. When the core diameter is small, only a single mode is permitted
and the ﬁbre is said to be a single mode ﬁbre. Fibres with large core diameters
are multimode ﬁbres.
9.2.1 Electric ﬁeld in single mode ﬁbre
In a single mode ﬁbre, the weakly guiding approximation n 9 n 1 is
satisﬁed, where n and n are the refractive index of the core and the cladding,
respectively. The fundamental mode is hybrid mode HE , which can be
simpliﬁed in the analysis by linear polarized mode LP . This fundamental
mode consists of two orthogonal modes HEV and HEW in accordance with
their polarization directions, so the electric ﬁelds in a single mode ﬁbre which
is not under Bragg condition can be well represented as:
152 Smart ﬁbres, fabrics and clothing
E(x, y, z; t) : c (z)E (x, y)exp[ 9 i( t 9 z)] [9.1]
K K K
where c and c denote the slowly varying amplitudes of the orthogonal HE
modes, , , , E and E are the angular frequency, the propagation
constants of HEV , and HEW , the transverse spatial distribution of electric
ﬁeld HEV , and the transverse spatial distribution of electric ﬁeld HEW ,
E (x, y) : F (r)e ; (i/ )cos [dF (r)/dr]e [9.2]
E (x, y) : F (r)e ; (i/ )sin [dF (r)/dr]e [9.3]
where F (r) represent the zero-order Bessel functions J in the core, and
modiﬁed Bessel functions K in the cladding, respectively, , e , e and e are
V W X
the propagation constant of the mode in an ideal single mode ﬁbre, the unit
vectors in x, y and z directions, respectively.
The coupled mode theory is often used to describe the polarization
characteristics, or modes coupling in optical ﬁbre, and the reﬂection spectra
of FBG sensors. When the optical response of an optical ﬁbre is analysed
based on the coupled mode theory, the electric ﬁeld is normalized as
E · E* dxdy : 1. Based on the perturbation approach, the slowly varying
amplitudes c are determined by the following coupled mode equations:
dc (z)/dz : i+ c (z) ; c (z)exp[( 9 )z], [9.4]
dc (z)/dz : i+ c (z)exp[ 9 ( 9 )z] ; c (z), [9.5]
where the subscripts 1 and 2 denote the modes HEV and HEW , respectively.
The amplitude coupling coeﬃcient from mode m to mode n is given by:
: (k/2 )
( E ) · E*dxdy,
GH K L
n, m : 1, 2 [9.6]
where is the dielectric permittivity perturbation tensor.
9.2.2 Polarization optics—
When the polarization behaviour of FBGs under various deformations is
discussed, one has to consider three types of perturbation, that is, those
induced by the ﬁbre making process (intrinsic), UV side exposure and strain
caused by deformation.
An evolution velocity is usually introduced to describe qualitatively the
polarization characteristics of speciﬁc polarization behaviour. in a generalized
Poincare sphere can be expressed by the coupled coeﬃcients as:
: [( 9 ) ; 4 ] [9.7]
Optical responses of FBG sensors under deformations 153
2 : arg( ; 9 9 ) [9.8]
2 : arctan[( 9 )/(4 )] [9.9]
where 2 and 2 are the latitude and longitude of the generalized Poincare ´
sphere, respectively. Hence the general approach of the polarization analysis
based on the coupled mode theory is used, by analysing the permittivity
perturbation ﬁrst, then inserting it into the coupled mode equations, obtaining
the solutions of c and c , and qualitatively presenting the polarization
characteristics by the evolution velocity.
The Poincare sphere, which has a unit radius and the spherical angular
coordinates 2 (longitude) and 2 (latitude), is often used to represent the
diﬀerent states of polarization geometrically. According to the traditional
terminology which is based on the apparent behaviour of the electric vector
when ‘viewed’ face on by the observer, we say that the polarization is
right-handed when to an observer looking in the direction from which the light
is coming, the end point of the electric vector would appear to describe the
ellipse in the clockwise sense. Hence right-handed polarization is represented
by points on the Poincare sphere which lie below the equatorial plane, and
left-handed by points on the Poincare sphere which lie above this plane.
Linear polarization is represented by points on the equator. Right- and
left-handed circular polarization are represented by the south and north pole
on the Poincare sphere, respectively.
9.2.3 Reﬂection spectra
A ﬁbre Bragg grating (FBG) consists of a periodic modulation of refractive
index in the core of a single mode ﬁbre. The electric ﬁelds in FBGs are
represented by the superposition of the ideal modes travelling in both forward
and backward directions:
E(x, y, z; t) : [a (z)exp(i z)
; b (z)exp( 9 i z)]E (x, y)exp( 9 i t) [9.10]
I I I
where a and b are slowly varying amplitudes of the kth mode travelling in the
; z and 9 z directions. The transverse mode ﬁelds E (x, y) might describe the
LP modes, or the cladding modes. The modes are orthogonal in an ideal
waveguide, hence do not exchange energy. The presence of a dielectric
perturbation causes them to be coupled. Based on the slowly varying envelope
approximation, the coupled mode equations for amplitudes a and b can be
154 Smart ﬁbres, fabrics and clothing
H : i ( R ; X )a (z)exp[i( 9 )z]
dz HI HI I I H
; i ( R 9 X )b (z)exp[ 9 i( ; )z]
HI HI I I H
H : 9 i ( R 9 X )a (z)exp[i( ; )z]
dz HI HI I I H
9 i ( R ; X )b (z)exp[ 9 i( 9 )z]
HI HI I I H
where the transverse coupling coeﬃcients between modes k and j are given by:
R : ( E ) · E* dxdy [9.13]
HI 2 P I R HR
where is the permittivity perturbation. It is often treated as a scalar term for
FBG sensors, and can be approximately expressed by index perturbation as
: 2n · n. However, in the cases where there is signiﬁcant linear birefringence
in an optical ﬁbre, such as in polarization maintaining ﬁbre, or under high
lateral compression, it should be corrected. The longitudinal coeﬃcient X can
usually be neglected, since generally X R for modes. In most FBGs, the
induced index change is non-existent outside the core, and the core refractive
index changes can be expressed as:
n : n (z) 1 ; · cos z ;
where n (z) is the DC index change spatially averaged over a grating period,
is the fringe visibility of the index change, is the nominal period, and
describes the grating chirp, respectively. Figure 9.1 shows some reﬂection
spectra of normal FGBs with diﬀerent fringe visibility.
If we insert the perturbation term Eq. (9.14) into Eq. (9.13), we can obtain
quantitative information about the reﬂection spectra of ﬁbre gratings. One of
the most important results of FBGs is the phase-matching condition, or Bragg
condition. The phase-matching condition of FBGs with period is given by
9 : 2 / , where and are the propagation constants of forward
and backward propagation modes. : 9 : for directional coupling
between the same modes. The phase-matching condition can then be
simpliﬁed to : / . If the eﬀective refractive index is used to represent the
propagation characteristics as : 2 · n / , it can then be expressed as:
: 2n [9.15]
Optical responses of FBG sensors under deformations 155
9.1 Reﬂection spectra of an FBG sensor with different ‘AC’ modulation
dose (a) 2.0 ; 10−4; (b) 1.0 ; 10−4; (c) 0.67 ; 10−4; (d) 0.5 ; 10−4).
where the Bragg wavelength is the free space centre wavelength of the input
light that will be back-reﬂected from the Bragg grating. Equation (9.15) is the
ﬁrst-order Bragg condition of the grating.
This ﬁrst-order Bragg condition is simply the requirement that satisﬁes both
energy and momentum conservation. Energy conservation requires that the
frequencies of the incident radiation and the scattered radiation are the same,
: , where : h/2 , h is Planck’s constant, and and are radian
frequencies of incident radiation and scattered radiation, respectively.
Momentum conservation requires that the incident wave-vector ki, plus the
FBG wave-vector kg, equal the wave-vector of the scattered radiation
ks : ki ; kg, where kg has a direction normal to the FBG planes with a
magnitude 2 / , is the spacing period of the FBG, ki has a direction along
the propagation direction of the incident radiation with a magnitude 2 n / ,
is the free space wavelength of the incident radiation, n is the modal index
(the eﬀective refractive index of the ﬁbre core) at the free space wavelength, ks
has a direction along the propagation direction of the scattered radiation with
a magnitude 2 n / , and is the free space wavelength of the scattered
radiation. If the scattered radiation is the reﬂected radiation of incident
radiation, that is, k : 9 k : 9 2 n / e , the momentum conservation
condition becomes the ﬁrst-order Bragg condition Eq. (9.15). The guided light
along the core of an optical ﬁbre will be scattered by each FBG plane. If the
Bragg condition is not satisﬁed, the reﬂected light from each of the subsequent
planes becomes progressively out of phase and will eventually cancel out. It
will experience very weak reﬂection at each of the FBG planes because of the
156 Smart ﬁbres, fabrics and clothing
index mismatch. This reﬂection accumulates over the length of the FBG.
A very important advantage of FBG sensors is that they are wavelength
encoded. Shifts in the spectrum, seen as a narrow-band reﬂection or dip in
transmission, are independent of the optical intensity and uniquely associated
with each FBG, provided no overlap occurs in each sensor stop-band. FBG
sensors have achieved signiﬁcant applications in monitoring or inspecting the
mechanical or temperature response in smart materials and structures. Most
of these applications focus on the axial deformation (or strain) and temperature
measurements, because the sensitivities to axial deformation and temperature
are much higher than those to other modes of deformation.
It is known from Eq. (9.15) that the Bragg wavelength is proportional to the
modal index and the FBG spacing period. Both the index and period may
change with external conditions which can be divided to temperature and
applied disturbances, such as deformations. The induced Bragg wavelength
shift of mode j (including polarization mode) can be expressed by:
:2 n ; H T
H H *T *T
* *n [9.16]
; n ; H u
H *u *u G
G G G
where n and u are the eﬀective refractive index of mode j and a perturbation,
respectively. Measurement of the perturbation-induced Bragg wavelength
shift from a single FBG does not facilitate the discrimination of the response to
these variables. The simplest approach is to isolate the unwanted perturbations.
In applications, sensors must be embedded with minimal intrusion. In case the
deformation sensing is considered, temperature is the main unwanted
perturbation. Temperature-compensating methods may be classiﬁed as
intrinsic or extrinsic. The elimination of cross-sensitivity may be achieved by
measurements at two diﬀerent wavelengths or two diﬀerent optical modes, in
which the strain and the temperature sensitivity are diﬀerent. The sensor
schemes can be constructed by the combination of FBGs with diﬀerent grating
types, such as FBGs with diﬀerent diameter, diﬀerent Bragg wavelength,
diﬀerent codope, hybrid FBGs and long period ﬁbre grating, Fabry—Perot
cavity, stimulated Brillouin scattering or ﬁbre polarization rocking ﬁlter. The
measurands may be Bragg wavelength, intensity, Brillouin frequency or
polarization rocking resonant wavelength.— In this chapter, only the
optical responses of FBG sensors under deformations are included.
9.3 Optical responses under tension
No signiﬁcant polarization signals can be observed for FBG sensors under
tension. But an FBG sensor has good linear characteristics when it is applied
Optical responses of FBG sensors under deformations 157
to measure the axial strain by reﬂection spectra. According to Eq. (9.16), the
relative shift of the Bragg wavelength due to strain is given by:
1 *n 1 *
: ; [9.17]
n * G * G
G G G G
where is the applied strain ﬁeld to the FBG sensor. According to the
photoelastic eﬀect, the ﬁrst term on the right side of Eq. (9.17) can be written as:
1 *n n
:9 p [9.18]
n * G 2 GH G
G G G
where p is the strain-optic tensor. For a homogeneous isotropic medium,
p p p 0 0 0
p p p 0 0 0
p p p 0 0 0
GH 0 0 0 p 0 0 [9.19]
0 0 0 0 p
0 0 0 0 0 p
where p : (p 9 p )/2. For the case of tension, the strain response arises
due to both the change in ﬁbre index due to photoelastic eﬀect, and the
physical elongation including the corresponding fractional change in grating
pitch of the FBG. If a uniaxial longitudinal stress is applied to the FBG
sensor in the z-direction, the resulting strain from ﬁrst-order elastic theory has
three principal components:
:[9 9 0 0 0]2 [9.20]
G X X X
where the superscript T denotes the transpose of a matrix, : /E is the
longitudinal strain, E is Young’s modulus and is Poisson’s ratio. The
index-weighted strain-optic coeﬃcient is then given by:
p : n [p 9 (p ; p ) ]2 [9.21]
Hence the right side of Eq. (9.18) can be written as 9 p .
If it can be assumed that the strain-induced change in the period of the FBG
is only dependent on the axial strain, the second term on the right side of Eq.
(9.17) will be equal to . Equation (9.17) is then expressed as:
/ : (1 9 p ) [9.22]
If the ﬁbre is extended at both ends and no body force applied, the ﬁbre core
and cladding can be regarded as homogeneous and isotropic, the strain
response of the germanosilicate FBG sensor at constant temperature under
tension is then given by:
158 Smart ﬁbres, fabrics and clothing
( / )/ : 0.78 [9.23]
In a silica ﬁbre there are three transmission wavelength windows in which the
losses are very low, such as 0.15 dB/km at 1550 nm. According to Eq. (9.23),
typical values for the sensitivity to an applied axial strain in these windows are
1.2 nm/milli-strain at 1550 nm, 1 nm/milli-strain at 1300 nm, and 0.66 nm/milli-
strain at 850 nm. The resolutions of FBG are 8.3 micro-strain at 1550 nm, 9.8
micro-strain at 1300 nm and 15 micro-strain at 850 nm by an optical spectrum
analyser with a wavelength resolution of 10 pm.
9.4 Optical responses under torsion
Unlike the optical responses of an FBG sensor under tension, the sensitivity of
the Bragg wavelength shift of an FBG sensor under torsion is very small.
However, the polarization response to torsion is signiﬁcant. The coupled
mode theory can be used to analyse the polarization behaviour of an FBG
sensor under torsion.
9.4.1 Shear strain-induced polarization behaviour
The torsion introduces shearing stress in the cross-section of the ﬁbre. If the
twisted length of a ﬁbre is L, and the angle of twist is
: L, where is torsion
ratio that is the angle of twist per unit length along the axis of the ﬁbre, the
matrix for the strain due to this torsion is:
: [0 0 0 x 9 y 0]2 [9.24]
so that the matrix for D , perturbation in optical impermeability, is:
D : p : [0 0 0 p x 9 p y 0]2 [9.25]
G GH G
The relationship between the dielectric permittivity perturbation and the
optical impermeability perturbation can be expressed as:
: 9 n D [9.26]
GH AM GH
The induced polarization behaviour can be analysed by using Eq. (9.26) and
Subsection 9.2.2. The induced circular birefringence in a single mode optical
ﬁbre is given by:
B :n (p 9 p )/(2 ) [9.27]
9.4.2 UV-induced polarization behaviour
The polarization of pulse UV beam and asymmetric geometry associated with
the side-exposure of UV light during the FBG fabrication process will
Optical responses of FBG sensors under deformations 159
induce linear birefringence. The peak birefringence of the FBG can be
calculated from the expression:
n: phase(Q ) 9 phase(Q ) [9.28]
where L is the length of the FBG, Q and Q are the eigenvalues of the
corresponding Jones matrix:
det[T (t)T(0) 9 QI] : 0 [9.29]
where T, t and I are the Jones matrix, the time from the beginning of the UV
exposure and the identity matrix, respectively. The symbol det and the
superscript denote the determinant and the inverse of a matrix, respectively.
Based on the birefringence, a permittivity perturbation tensor can be used to
represent its polarization behaviour:
: 0 0 [9.30]
0 0 0
where 9 : 2n · n. By considering the azimuth
of the faster or
slow axis of the FBG sensor and the tilted angle q, Eq. (9.30) becomes:
: T T T2T2 [9.31]
34 X V 34 V X
where T and T are the rotation matrix around z, x axes, respectively. The
induced polarization behaviour can be analysed by using Eq. (9.31) and
In the case of an FBG sensor under torsion, both shear strain-induced
birefringence and UV-induced birefringence are considered:
: ; [9.32]
GH GH 34
There are UV-induced linear birefringence and shear strain-induced circular
birefringence in the ﬁbre.
9.4.3 Simulated and experimental results
In numeric simulations, the parameters of the FBG sensor are the same as
those used in the corresponding experiments. The core radius, cladding radius
and the eﬀective refractive index are 4.25 m, 62.5 m and 1.46, respectively.
The strain-optic coeﬃcients p and p are taken as 0.113 and 0.252, respectively.
Based on the preceding theoretical analysis, the FBG sensors can be treated
as the wave-plates. Apparently, when an FBG sensor is under torsion, these
160 Smart ﬁbres, fabrics and clothing
9.2 FBGs under torsion. The length of the FBG and the torsion gauge of
the ﬁbre are 1 cm and 17.5 cm, respectively.
9.3 Simulated polarization signals of an FBG under torsion. The
orientation is 0, /12, /6, /4, respectively, and the angle of ellipticity is
zero in (a), and /8 in (b).
wave-plates will be rotated. This means the geometric parameter, the azimuth
, will be changed during the twisting of an optical ﬁbre. Then the output
polarization signals will represent the combination eﬀects of the torsion-induced
circulation birefringence and the UV irradiation-induced linear birefringence.
The torsion model under investigation is shown in Fig. 9.2, where the FBG
is located at the middle point of an optical ﬁbre. The experimental setup is
similar to that of T. Erdogan and V. Mizrahi, and the UV-induced
birefringence of a FBG is approximately 2.5 ; 10. The wavelength of the
incident laser is set at 1525 nm, and the loading rotation angle is from 0 to 360°.
The simulated results are presented in Fig. 9.3. According to these simulations,
the initial orientations do not appear to aﬀect the shape of the output
polarization signals. However, the ellipticity of the input light will aﬀect the
output polarization signals signiﬁcantly.
The position of the FBG can inﬂuence the output polarization signals
signiﬁcantly. On one side, it will change the direction of the angular velocity
vector of the FBG sensor, and on the other side, it will provide a diﬀerent initial
state of polarization from the FBG segment. Although both their directions
vary along the equator in a generalized Poincare sphere, their respective
variation velocities are diﬀerent. These diﬀerences will result in diﬀerent
output polarization signals for various FBG sensor positions.
Figure 9.4 shows one measured polarization signal of an FBG sensor under
Optical responses of FBG sensors under deformations 161
9.4 Measured polarization signal of an FBG under torsion.
torsion. The twisted length was 17.5 cm, the Bragg wavelength without
external strain was 1555 nm, the wavelength of incident laser was 1525 nm, the
torsion ratios were 0—0.36 rad/cm with a step of 0.005 rad/cm. The states of
polarization were measured by a commercial polarimeter. The simulated
result coincides with the experimental result.
The reﬂective spectrum of the FBG sensor was measured by an optical
spectrum measuring system composed of a tunable laser, an optical power
meter with GP-IB interface, and a computer. The wavelength resolution is
10 pm. The measured wavelength shift under the torsion ratio of 1 rad/cm is
smaller than the resolution of the optical spectrum measuring system.
9.5 Optical responses under lateral compression
In the case of optical ﬁbres under lateral compression, linear birefringence will
be induced based on the strain—optic relationship. Thus a ﬁbre can be used to
sense the lateral compression by measuring the change of state of polarization
of travelled light. For general FBG sensors the wavelength-compression
sensitivity is relatively small compared with the axial strain sensitivity, but
spectrum bifurcation, or spectrum split, will occur with the compression-induced
birefringence in optical ﬁbres. The transverse strain can also be sensed by an
FBG written into a polarization-maintaining ﬁbre (PMF) by measuring the
Bragg wavelength shifts of two reﬂective peaks associated with the orthogonal
polarization modes.— In addition, transverse strain can be measured by a
long-period ﬁbre grating.
162 Smart ﬁbres, fabrics and clothing
9.5 FBG under lateral compression. The length of FBG and compressed
length of ﬁbre are 1 cm and 1.8 cm, respectively.
9.5.1 Polarization responses under lateral compression
The strain of an optical ﬁbre under lateral compression will induce linear
birefringence. Since the glass optical ﬁbre is a rigid medium, the birefringence
induced by the geometric property, such as tilted angle for tilted FBG, is small.
The polarization behaviour of the FBG under lateral compression can be
determined by the combination eﬀects of both the compression-induced linear
birefringence and the UV-induced linear birefringence.
The case that an uncoated silica optical ﬁbre is laminated by two rigid plates
is considered, as shown in Fig. 9.5. Since the silica optical ﬁbre is a rigid
medium, this contact problem can be simpliﬁed to line force loading. Then the
close form of the stress solutions can be obtained with the help of the plane
stress assumption. Since the electric ﬁeld in a single mode ﬁbre is concentrated
in the core region, the solution in the centre is approximately selected to
represent the stress of a single mode ﬁbre under lateral compression. The stress
in the core can be expressed as:
: f/( · r ) [9.33]
: : :0 [9.36]
where f is the lateral loading, and r is the radius of optical ﬁbre cladding.
Based on the strain—optic relationship, the permittivity perturbation can be
derived. It can be inserted into the coupled mode equations, Eqs. (9.4) and (9.5),
and the coupled mode coeﬃcients can be obtained by coupling integrals, Eq.
(9.6). The strain induces a linear birefringence:
4n · f
B : (1 ; )(p 9 p ) [9.37]
In the simulated analysis, the lateral loading is from 0 to 1000 N/m, and the
Optical responses of FBG sensors under deformations 163
9.6 Polarization signals of FBG under lateral compression. The normal
compression is shown in (a), and slant compression with 45° in (b); the
angle of ellipticity is 0. The orientations are 0, /12, 6 and /4, respectively.
permittivity perturbation induced by the transverse strain and UV-induced
birefringence are considered together. For a normal lateral compression, the
UV irradiation-induced birefringence axis coincides with the strain-induced
birefringence. Since the silica optical ﬁbre is a rigid medium, the compression-
induced displacement is small, and it has little eﬀect on the geometric
parameters of the UV-induced perturbation. Thus, the output polarization
signal is the same as the single mode ﬁbre. The output polarization signals are
shown in Fig. 9.6(a). They are insensitive to the FBG position.
For a slant compression, there is an angle between the strain- and UV
irradiation-induced birefringence axis. Though the UV irradiation-induced
component change is small during the loading, it still aﬀects the output
polarization signals during the compression. Apparently, the eﬀects are related
to the angle and the position of the FBG. The output polarization signals are
shown in Fig. 9.6(b).
9.5.2 Spectrum responses under lateral compression
As shown in the previous section, lateral compression will induce linear
birefringence in a single mode optical ﬁbre. This means that a diﬀerence of the
propagation constants in the two orthogonal polarization modes in the ﬁbre is
induced. Based on the phase-matching condition Eq. (9.15), these two
propagation constants correspond to two diﬀerent Bragg wavelengths. Thus,
with the increasing of compression loading, the spectrum bifurcation or
spectrum split will be observed. An extended multidimension measurement is
applying the double wavelength measurement in the birefringent FBG. Since
the eﬀective indices of the orthogonal LP modes are diﬀerent from each other
164 Smart ﬁbres, fabrics and clothing
in birefringent optical ﬁbre, every FBG in a birefringent ﬁbre has two
corresponding Bragg wavelengths. If we write two diﬀerent FBGs in a single
optical ﬁbre, then it is expected to obtain four diﬀerent Bragg wavelengths,
which can establish four equations as Eq. (9.16), and to measure not only the
axial strain and temperature, but also two transverse strain components.
In the case of lateral compression, the propagated fundamental mode HE
perfectly degenerates into x- and y-polarized modes with diﬀerent propagation
constants. According to the photoelastic eﬀect and the stress—strain relationship,
the eﬀective index changes of the two polarized modes can be expressed as:
n (x, y, z) : 9 +(p 9 2 p ) (x, y, z)
V 2E V
; [(1 9 )p 9 p ] (x, y, z), [9.38]
n (x, y, z) : 9 +(p 9 2 p ) (x, y, z)
W 2E W
; [(1 9 )p 9 p ] (x, y, z), [9.39]
Using the stress—strain relationship and Eq. (9.17), the relative shifts of the
Bragg wavelength of two polarized modes at any point of the FBG due to
lateral compression are then obtained by:
V:9 +(p 9 2 p ) (x, y, z) ; [(1 9 )p 9 p ] (x, y, z),
2E V W
9 [ (x, y, z) ; (x, y, z)]/E [9.40]
W:9 +(p 9 2 p ) (x, y, z) ; [(1 9 )p 9 p ] (x, y, z),
2E W V
9 [ (x, y, z) ; (x, y, z)]/E [9.41]
The spectrum split of the polarized modes at any point is then given by:
(x, y, z) 9 (x, y, z) n
W V :9 (1 ; )(p 9 p )[ (x, y, z)
9 (x, y, z)] [9.42]
Figure 9.7 represents the reﬂection spectra of an FBG under diﬀerent lateral
loads. The spectrum of the FBG splits in more than one peak at the Bragg
wavelength. For higher values of applied force, the peaks become totally separate.
Optical responses of FBG sensors under deformations 165
1539 1539.5 1540 1540.5 1541 1541.5
9.7 Reﬂection spectra of an FBG sensor under lateral compression
(loadings a–d are 0.0, 1.5, 2.0 and 3.0 kN/m, respectively), the angle
between the orientation of input linear polarized light and the compression
direction is 45°.
9.6 Optical responses under bending
The major eﬀects of FBG under bending (see Fig. 9.8) may come from the
geometrically bent structure and non-uniform lateral stress. Using the
perturbation method, the scalar propagation characteristics of a geometrically
bent optical waveguide can be analysed. Corrected electric ﬁelds or Gaussian
approximations have been proposed to describe the ﬁeld deformations.
The equivalent straight waveguide is often used to describe its electric ﬁeld in
the bent waveguide. More rigorous description adopted a full-vectorial wave
propagation theory. Based on the photoelastic relationship, the non-uniform
stress distribution-induced birefringence has been presented.— The
induced linear birefringence can be expressed as:
B : 0.25n (p 9 p )(1 ; )(r /r ) [9.43]
Assuming that the mode holds and the phase-matching condition works well
in the bent FBG, the eﬀects under bending can be qualitatively analysed. Then
the shift of Bragg wavelength is determined by the changes of propagation
constants or eﬀective refractive index, and grating period. In the case of
stress-induced birefringence, only the eﬀects of non-uniform lateral compressive
stress are considered, since it is only sensitive to the diﬀerence of that in two
orthogonal directions. But, in order to obtain an absolute change of refractive
index, the eﬀect of the axis component is required. According to the
166 Smart ﬁbres, fabrics and clothing
9.8 Fibre Bragg gratings under bending.
photoelastic relationship, the index of the optical ﬁbre is decreased by tension
and is increased by compression. Since the electric ﬁeld in the bent optical ﬁbre
shifts towards the outer core/cladding boundary, and the outer side of the bent
optical ﬁbre is under tension, the ﬁeld deformation will induce a decrement of
eﬀective refractive index. Apparently due to the birefringence of the bending
optical ﬁbre, two independent Bragg wavelengths occur. The diﬀerence of
these two Bragg wavelengths is small, and only a broader bandwidth of
reﬂection spectrum can be observed.
Another characteristic of the silica ﬁbre is the non-linear stress—strain
relationship. It is known that the neutral axis is also shifted toward the outer
side of the ﬁbre under bending. Its direct eﬀect on the FBG is that the
grating period will be compressed, so these eﬀects should also be considered,
together with the change of eﬀective refractive index of the FBG under bending.
Other ﬁbre gratings can also be used in bend sensing, such as long-period
ﬁbre grating and multicore ﬁbre Bragg gratings.
This chapter has given the optical responses of FBG sensors under diﬀerent
modes of deformation. Both the polarization behaviour and optical spectrum
of FBGs have been used to analyse the deformation perturbations. In the case
of an FBG under tension, the wavelength sensitivity to tension is signiﬁcant. In
the case of torsion, the wavelength sensitivity is very small, and the
polarization behaviour is sensitive to it. In the case of lateral compression, the
wavelength sensitivity is much smaller than that under tension, but the
deformation induced birefringence can broaden and split the reﬂection peaks.
Optical responses of FBG sensors under deformations 167
Table 9.1 Optical responses of normal germanosilicate FBG under different
UV induced Deformation induced
Bragg linear linear/circular
Mode of wavelength birefringence83 birefringence82,85
deformation shift 14,85,102 Bl B l /B c
Tension 1200 pm/m , at 2.5 ; 10−5 0
wavelength 1550 nm
Torsion : 10 pm, at torsion 2.5 ; 10−5 B l = 9.7 ; 10−7 ,
ratio 0.072 rad/mm, [ ] = rad/mm, at
from experiment wavelength 1550 nm
Lateral 2.0 pm/N (parallel), 2.5 ; 1095 Bl = 5.1 ; 10−4, at
compression 8.6 pm/N 10 N/mm
Pure bending : 260 pm, at 2.5 ; 10–5 Bl = 1.5 ; 10−5 (1/rbent)2,
curvature 2.43 cm−1 [rbent] = cm
The lateral compression can be sensed by the spectrum behaviour in some
sensing schemes. Both the polarization behaviour and the optical spectrum of
FBGs can be used to analyse lateral compression. Bending of FBGs can be
analysed for both the polarization behaviour and the optical spectrum, but it is
diﬃcult to measure the polarization evolution of ﬁbre under bending. The
optical responses of normal germanosilicate FBG under diﬀerent individual
modes of deformations are summarized in Table 9.1.
In practical FBG sensors, temperature must be considered in the spectrum
because of their high sensitivity to temperature. Some approaches include
isolating or compensating or simultaneously measuring the temperature
The authors wish to thank Hong Kong Research Grants Council for
supporting this work (Grant No. PolyU5112/98E).
1 Gardner J W, Microsensors: Principles and Applications, John Wiley Sons,
Chichester, UK, 1994.
2 Yang X and Young R J, ‘Determination of residual strains in ceramic-ﬁbre
168 Smart ﬁbres, fabrics and clothing
reinforced composites using ﬂuorescence spectroscopy’, Acta Metallurgica et
Materialia, 1995, 43(6), 2407—16.
3 Grattan K T V and Sun T, ‘Fiber optic sensor technology: an overview’, Sensors and
Actuators, A-Physical, 2000, 82(1—3), 40—61.
4 Posey R and Vohra S T, ‘An eight-channel ﬁber-optic Bragg grating and stimulated
Brillouin sensor system for simultaneous temperature and strain measurements’,
IEEE Photonics Technol. Lett., 1999, 11(12), 1641—3.
5 Brown A W, DeMerchant M D, Bao X et al., ‘Spatial resolution enhancement of a
Brillouin-distributed sensor using a novel signal processing method’, IEEE J.
Lightwave Technol., 1999, 17(7), 1179—83.
6 Kim S H, Lee J J, Lee D C et al., ‘A study on the development of transmission-type
extrinsic Fabry—Perot interferometric optical ﬁber sensor’, IEEE J. Lightwave
Technol., 1999, 17(10), 1869—74.
7 Udd E, Fiber Optic Sensors: An Introduction for Engineers and Scientists, John
Wiley Sons, New York, 1991.
8 Van Steenkiste R J, Strain and Temperature Measurement with Fiber Optic Sensors,
Technomic Publishing Company, Lancaster, 1997.
9 Johnson P, ‘Strain ﬁeld measurements with dual-beam digital speckle photography’,
Optics Lasers Eng., 1998, 30(3—4), 315—26.
10 Johnson P, ‘Strain ﬁeld measurements in industrial applications using dual-beam
digital speckle photography’, Optics Lasers Eng., 1998, 30(5), 421—31.
11 Hack E and Broennimann R, ‘Electronic speckle pattern interferometry deformation
measurement on lightweight structures under thermal load’, Optics Lasers Eng.,
1999, 31(3), 213—22.
12 Rae P J, Goldrein H T, Bourne N K et al., ‘Measurement of dynamic large-strain
deformation maps using an automated ﬁne grid technique’, Optics Lasers Eng.,
1999, 31(2), 113—22.
13 Kersey A D, Davis M A, Patrick H J et al., ‘Fiber grating sensors’, IEEE J.
Lightwave Technol., 1997, 15(8), 1442—63.
14 Othonos A and Kalli K, Fiber Bragg Gratings: Fundamentals and Applications in
Telecommunications and Sensing, Artech House, Boston, 1999.
15 Rao Y J, ‘In-ﬁber Bragg grating sensors’, Measurement Sci. Technol., 1997, 8(4),
16 Rao Y J, ‘Recent progress in applications of in-ﬁber Bragg grating sensors’, Optics
Lasers Eng., 1999, 31(4), 297—324.
17 Friebele E J, ‘Fiber Bragg grating strain sensors: present and future applications in
smart structures’, Optics Photon. News, 1999, 9(1), 33—7.
18 Hill K O and Meltz G, ‘Fiber Bragg grating technology fundamentals and
overview’, IEEE J. Lightwave Technol., 1997, 15(8), 1263—76.
19 Kashyap R, Fiber Bragg Gratings, Academic Press, San Diego, 1999.
20 Meltz G, ‘Overview of ﬁber grating-based sensors’. In Proc. SPIE—Distributed and
Multiplexed Fiber Optic Sensors VI, 1996, 2838, 2—22.
21 Goyal A and Muendel M, ‘Optical ﬁber Bragg gratings have a wide variety of uses’,
Photonics Spectra, 1998, 32(9), 116—22.
22 Udd E, Fiber Optic Smart Structures, John Wiley, New York, 1995.
23 Morey W W, Ball G A and Singh H, ‘Applications of ﬁber Bragg grating sensors’. In
Proc. SPIE — Fiber Optic and Laser Sensors XIV, 1996, 2839, 2—7.
Optical responses of FBG sensors under deformations 169
24 Measures R M, Maaskant R, Alavie T et al., ‘Fiber-optic Bragg gratings for bridge
monitoring’, Cement Concrete Composites, 1997, 9(1), 21—3.
25 Meissner J, Nowak W, Slowik V et al., ‘Strain monitoring at a prestressed concrete
bridge’. In Proc. 12th Int. Conf. Optical Fiber Sensors, Williamsburg, 48—51, 1997.
26 Schulz W L, Udd E, Seim J M et al., ‘Advanced ﬁber grating strain sensor systems
for bridges, structures, and highways’. In Proc. SPIE — Smart Structures and
Materials 1998: Smart Systems for Bridges, Structures, and Highways, 1998, 3325,
27 Prohaska J D, Snitzer E, Chen B et al., ‘Fiber optic Bragg grating strain sensor in
large scale concrete structures’. In Proc. SPIE — Fiber Optic Smart Structures and
Skins V, 1992, 1798, 286—94.
28 Du W C, Tao X M, Tam H Y et al., ‘Fundamentals and applications of optical ﬁber
Bragg grating sensors to textile structural composites’, Composite Structures, 1998,
29 Jin X D, Sirkis J S, Venkateswaran V S et al., ‘Simultaneous measurement of two
strain components in composite structures using embedded ﬁber sensors’. In Proc.
12th Int. Conf. Optical Fiber Sensors, Williamsburg, 44—7, 1997.
30 Ferdinand P, Ferragu O, Lechien J L et al., ‘Mine operating accurate stability
control with optical ﬁber sensing and Bragg grating technology: the European
BRITE/EURAM STABILOS project’, IEEE J. Lightwave Technol., 1995, 13(7),
31 Hjelme D R, Bjerkan L, Neegard S et al., ‘Application of Bragg grating sensors
in the characterization of scaled marine vehicle modes’, Appl. Optics, 1997, 36(1),
32 Friebele E J, Askins C G, Bosse A B et al., ‘Optical ﬁber sensors for spacecraft
applications’, Smart Mater. Struct., 1999, 8(6), 813—38.
33 Ezbiri A, Kanellopoulos S E and Handerek V A, ‘High resolution instrumentation
system for demodulation of Bragg grating aerospace sensors’, In Proc. 12th Int.
Conf. Optical Fiber Sensors, Williamsburg, 456—9, 1997.
34 Tang L Q, Tao X M and Choy C L, ‘Eﬀectiveness and optimization of ﬁber Bragg
grating sensor as embedded strain sensor’, Smart Mater. Struct., 1999, 8(1), 154—60.
35 Rao Y J, Webb D J, Jackson D A et al., ‘In-ﬁber Bragg grating temperature sensor
system for medical applications’, IEEE J. Lightwave Technol., 1997, 15(5), 779—85.
36 Arie A, Lissak B and Tur M, ‘Static ﬁber-Bragg grating strain sensing using
frequency-locked lasers’, IEEE J. Lightwave Technol., 1999, 17(10), 1849—55.
37 Kersey A D, Berkoﬀ T A and Morey W W, ‘Multiplexed ﬁber Bragg grating sensor
system with a ﬁber Fabry—Perot wavelength ﬁlter’, Optics Lett., 1993, 18(16), 1370—2.
38 Davis M A, Bellemore D G and Kersey A D, ‘Design and performance of a ﬁber
Bragg grating distributed strain sensor system’. In Proc. SPIE — Smart Structures
and Materials 1995: Smart Systems for Bridges, Structures, and Highways, 1995,
39 Kersey A D, Davis M A and Bellemore D G, ‘Development of ﬁber sensors for
structural monitoring’. In Proc. SPIE — Nondestructive Evaluation of Aging Bridges
and Highways, 1995, 2456, 262—8.
40 Dunphy J R, Ball G, Amato F D et al., ‘Instrumentation development in support of
ﬁber grating sensor arrays’, In Proc. SPIE — Distributed and Multiplexed Fiber Optic
Sensors III, 1993, 2071, 2—11.
170 Smart ﬁbres, fabrics and clothing
41 Jackson D A, Ribeiro A B L, Reekie L et al., ‘Simple multiplexing scheme for a ﬁber
optic grating sensor network’, Optics Lett., 1993, 18(14), 1192—4.
42 Davis M A and Kersey A D, ‘A ﬁber Fourier transform spectrometer for decoding
ﬁber Bragg sensors’, IEEE J. Lightwave Technol., 1995, 13(7), 1289—95.
43 Kersey A D and Berkoﬀ T A, ‘Fiber optic Bragg diﬀerential temperature sensor’,
IEEE Photon. Technol. Lett., 1992, 4(10), 1183—5.
44 Ferreira L A, Diatzikis E V, Santos J L et al., ‘Frequency-modulated multimode
laser diode for ﬁber Bragg grating sensors’, IEEE J. Lightwave Technol., 1998, 16(9),
45 Moreira P J, Ferreira L A, Santos J L et al., ‘Dynamic range enhancement in ﬁber
Bragg grating sensors using a multimode laser diode’, IEEE Photon. Technol. Lett.,
1999, 11(6), 703—5.
46 Tanaka Y and Ogusu K, ‘Tensile-strain coeﬃcient of resonance frequency of
depolarized guided acoustic-wave Brillouin scattering’, IEEE Photonics Technol.
Lett., 1999, 11(7), 865—7.
47 Lissak B, Arie A and Tur M, ‘Highly sensitive dynamic strain measurements by
locking lasers to ﬁber Bragg gratings’, Optics Lett., 1998, 23(24), 1930—2.
48 Ogawa O, Kato T and Kamikatano M, ‘Technique for measuring the dynamic
strain on an optical ﬁber based on Brillouin ring ampliﬁcation’, IEEE J. Lightwave
Technol., 1999, 17(2), 234—42.
49 McGarrity C and Jackson D A, ‘A network for large numbers of interferometric
sensors and ﬁber Bragg gratings with high resolution and extended range’, IEEE J.
Lightwave Technol., 1998, 16(1), 54—65.
50 Berkoﬀ T A, Davis M A, Bellemore D G et al., ‘Hybrid time and wavelength division
multiplexed ﬁber grating array’, In Proc. SPIE — Smart Structures and Materials
1995: Smart Sensing, Processing, and Instrumentation, 1995, 2444, 288—94.
51 Friebele E J, Putnam M A, Patrick H J et al., ‘Ultrahigh-sensitivity ﬁber-optic
strain and temperature sensor’, Optics Lett., 1998, 23(3), 222—4.
52 Chan C C, Jin W, Rad A B et al., ‘Simultaneous measurement of temperature and
strain: an artiﬁcial neural network approach’, IEEE Photon. Technol. Lett., 1998,
53 James S W, Dockney M L and Tatam R P, ‘Simultaneous independent temperature
and strain measurement using in-ﬁber Bragg grating sensors’, Electron. Lett., 1996,
54 Xu M G, Archambault J L, Reekie L et al., ‘Discrimination between strain and
temperature eﬀects using dual-wavelength ﬁber grating sensors’, Electron. Lett.,
1994, 30(13), 1085—7.
55 Cavaleiro P M, Araujo F M, Ferreira L A et al., ‘Simultaneous measurement of
strain and temperature using Bragg gratings written in germanosilicate and
boron-codoped germanosilicate ﬁbers’, IEEE Photon. Technol. Lett., 1999, 11(12),
56 Patrick H J, Williams G M, Kersey A D et al., ‘Hybrid ﬁber Bragg grating/long
period ﬁber grating sensor for strain/temperature discrimination’, IEEE Photon.
Technol. Lett., 1996, 8(9), 1223—5.
57 Du W C, Tao X M and Tam H Y, ‘Temperature independent strain measurement
with a ﬁber grating tapered cavity sensor’, IEEE Photon. Technol. Lett., 1999, 11(5),
Optical responses of FBG sensors under deformations 171
58 Du W C, Tao X M and Tam H Y, ‘Fiber Bragg grating cavity sensor for
simultaneous measurement of strain and temperature’, IEEE Photon. Technol.
Lett., 1999, 11(1), 105—7.
59 Lo Y L, ‘In-ﬁber Bragg grating sensors using interferometric interrogations for
passive quadrature signal processing’, IEEE Photon. Technol. Lett., 1998, 10(7), 1003—5.
60 Koo K P, LeBlanc M, Tsai T E et al., ‘Fiber-chirped grating Fabry—Perot sensor
with multiple-wavelength-addressable free-spectral ranges’, IEEE Photon. Technol.
Lett., 1998, 10(7), 1006—8.
61 Smith J, Brown A, DeMerchant M et al., ‘Simultaneous strain and temperature
measurement using a Brillouin scattering based distributed sensor’. In Proc. SPIE —
Smart Structures and Materials 1999: Sensory Phenomena and Measurement
Instrumentation for Smart Structures and Materials, 1999, 3670, 366—73.
62 Kanellopoulos S E, Handerek V A and Rogers A, ‘Simultaneous strain and
temperature sensing with photogenerated in-ﬁber gratings’, Optics Lett., 1995,
63 Kang S C, Kim S Y, Lee S B et al., ‘Temperature-independent strain system using a
tilted ﬁber Bragg grating demodulator’, IEEE Photon. Technol. Lett., 1998, 10(10),
64 Sinha P G and Yoshino T, ‘Acoustically scanned low-coherence interrogated
simultaneous measurement of absolute strain and temperature using highly
birefringent ﬁbers’, IEEE J. Lightwave Technol., 1998, 16(11), 2010—15.
65 Yun S H, Richardson D J and Kim B Y, ‘Interrogation of ﬁber grating sensor arrays
with a wavelength-swept ﬁber laser’, Optics Lett., 1998, 23(11), 843—5.
66 Putnam M A, Dennis M L, Duling III I N et al., ‘Broadband square-pulse operation
of a passively mode-locked ﬁber laser for ﬁber Bragg grating interrogation’, Optics
Lett., 1998, 23(2), 138—40.
67 LeBlanc M, Huang S, Ohn M et al., ‘Distributed strain measurement based on a
ﬁber Bragg grating and its reﬂection spectrum analysis’, Optics Lett., 1996, 21(17),
68 Huang S, Ohn M M and Measures R M, ‘A novel Bragg grating distributed-strain
sensor based on phase measurements’. In Proc. SPIE — Smart Structures and
Materials 1995: Smart Sensing, Processing, and Instrumentation, 1995, 2444,
69 Volanthen M, Geiger H and Dakin J P, ‘Distributed grating sensors using
low-coherence reﬂectometry’, IEEE J. Lightwave Technol., 1997, 15(11), 2076—82.
70 Bhatia V and Vengsarkar A M, ‘Optical ﬁber long-period grating sensors’, Optics
Lett., 1996, 21(9), 692—4.
71 Patrick H, Kersey A D, Pedrazzani J R et al., ‘Fiber Bragg grating demodulation
system using in-ﬁber long period grating ﬁlters’. In Proc. SPIE — Distributed and
Multiplexed Fiber Optic Sensors VI, 1996, 2838, 60—5.
72 Kersey A D and Morey W W, ‘Multiplexed Bragg grating ﬁber laser strain sensor
system with mode-locked interrogation’, Electron. Lett., 1993, 29(1), 112—14.
73 Kersey A D and Morey W W, ‘Multi-element Bragg grating based ﬁber laser strain
sensor’, Electron. Lett., 1993, 29(11), 964—66.
74 Koo K P and Kersey A D, ‘Bragg grating based laser sensor systems with
interferometric interrogation and wavelength division multiplexing’, IEEE J.
Lightwave Technol., 1995, 13(7), 1243—9.
172 Smart ﬁbres, fabrics and clothing
75 Born M and Wolf E, Principles of Optics, 7th (Expanded) edn, Cambridge
University Press, Cambridge, 1999.
76 Huard S, Polarization of Light, John Wiley, New York, 1997.
77 Ulrich R and Simon A, ‘Polarisation optics of twisted single-mode ﬁbers’, Appl.
Optics, 1979, 18(13), 2241—51.
78 Buck J A, Fundamentals of Optical Fibers, John Wiley, New York, 1995.
79 Zhou W, Chen X F and Yang D X, Fundamentals of Photonics, Zhejiang University
Press, Hangzhou, 2000.
80 Marcuse D, Theory of Dielectric Optical Waveguides, 2nd edn, Academic Press,
81 Wangsness R K, Electromagnetic Fields, John Wiley, New York, 1979.
82 Zhang A P, Tao X M and Tam H Y, Prediction of polarization behavior of twisted
optical ﬁbres containing Bragg grating sensors, J. Textile Inst., 2000, Part 3, 105—16.
83 Jeunhomme L B, Single-Mode Fiber Optics: Principles and Applications, 2nd edn,
Marcel Dekker, New York, 1990.
84 Erdogan T and Mizrahi V, ‘Characterization of UV-induced birefringence in
photosensitive Ge-doped silica optical ﬁber’, J. Opt. Soc. Amer. B, 1994, 11(10), 2100—5.
85 Vengarkar A M, Zhong Q, Inniss D et al., ‘Birefringence reduction in side-written
photoinduced ﬁber devices by a dual-exposure method’, Optics Lett., 1994, 19(16),
86 Gafsi R and El-Sherif M A, ‘Analysis of induced-birefringence eﬀects on ﬁber Bragg
gratings’, Opt. Fiber Technol., 2000, 6(3), 299—323.
87 Kawase L R, Valente L C G, Margulis W et al., ‘Force measurement using induced
birefringence on Bragg grating’. In Proc. 1997 SBMO/MTT-S International
Microwave and Optoelectronics Conference, (1) 394—6, 1997.
88 Lawrence C M, Nelson D V, Makino A et al., ‘Modeling of the multi-parameter
Bragg grating sensor’, In Proc. SPIE — Third Paciﬁc Northwest Fiber Optic Sensor
Workshop, 1997, 3180, 42—9.
89 Udd E, Nelson D V and Lawrence C M, ‘Multiple axis strain sensing using ﬁber
gratings written onto birefringent single mode optical ﬁber’, In Proc. 12th Int. Conf.
Optical Fiber Sensors, Williamsburg, 48—51, 1997.
90 Udd E, Lawrence C M and Nelson D V, ‘Development of a three axis strain and
temperature ﬁber optical grating sensor’. In Proc. SPIE — Smart Structures and
Materials 1997: Smart Sensing, Processing, and Instrumentation, 1997, 3042, 229—36.
91 Udd E, Schulz W L, Seim J M et al., ‘Transverse ﬁber grating strain sensors based
on dual overlaid ﬁber gratings on polarization preserving ﬁbers’. In Proc. SPIE —
Smart Structures and Materials 1998: Sensory Phenomena and Measurement
Instrumentation for Smart Structures and Materials, 1998, 3330, 253—63.
92 Udd E, Schulz W L and Seim J M, ‘Measurement of multidimensional strain ﬁelds
using ﬁber grating sensors for structural monitoring’. In Proc. SPIE — Fiber Optic
Sensor Technology and Applications, 1999, 3860, 24—34.
93 Udd E, Schulz W L and Seim J M, ‘Multi-axis ﬁber grating strain sensor
applications for structural monitoring and process control’. In Proc. SPIE —
Process Monitoring Applications of Fiber Optic Sensors, 1999, 3538, 206—14.
94 LeBlanc M, Vohra S T, Tsai T E et al., ‘Transverse load sensing by use of
pi-phase-shifted ﬁber Bragg gratings’, Optics Lett., 1999, 24(16), 1091—3.
Optical responses of FBG sensors under deformations 173
95 Canning J and Sceats M G, ‘ -phase-shifted periodic distributed structures in
optical ﬁbers by UV post-processing’, Electron. Lett., 1994, 30(16), 1344—5.
96 Liu Y, Zhang L, Bennion I, ‘Fibre optic load sensors with high transverse strain
sensitivity based on long-period gratings in B/Ge co-doped ﬁbre’, Electron. Lett.,
1999, 35(8), 661—3.
97 Gambling W A, Matsumura H and Ragdale C M, ‘Field deformation in a curved
single-mode ﬁber’, Electronics Lett., 1978, 14(5), 130—2.
98 Garth S J, ‘Modes on a bent optical wave-guide’, IEE Proc. J: Optoelectronics,
1987, 134(4), 221—9.
99 Lui W W, Xu C L, Hirono T et al., ‘Full-vectorial wave propagation in
semiconductor optical bending waveguides and equivalent straight waveguide
approximations’, J. Lightwave Technol., 1998, 16(5), 910—14.
100 Ulrich R, Rashleigh S C and Eichoﬀ W, ‘Bending-induced birefringence in single
mode ﬁbers’, Optics Lett., 1980, 5(6), 273—5.
101 Garth S J, ‘Birefringence in bent single-mode ﬁbers’, J. Lightwave Technol., 1988,
102 Sakai J I and Kimura T, ‘Birefringence and polarization characteristics of
single-mode optical ﬁbers under elastic deformations’, IEEE J. Quantum Electron.,
1981, 17(6), 1041—51.
103 Dai C, Yang D X, Tao X M et al., ‘Eﬀects of pure bending on the sensing
characteristics of ﬁber Bragg gratings’, In Proc. SPIE — International Conference
on Sensors and Control Techniques, 2000, 4077, 92—6.
104 Suhir E, ‘Eﬀect of the nonlinear stress—strain relationship on the maximum stress
in silica ﬁbers subjected to two-point bending’, Appl. Optics, 1993, 32(9), 1567—72.
105 Liu Y, Zhang L, Williams J A R et al., ‘Optical bend sensor based on measurement
of resonance mode splitting of long-period ﬁber grating’, IEEE Photon. Technol.
Lett., 2000, 12(5), 531—3.
106 Ye C C, James S W and Tatam R P, ‘Simultaneous temperature and bend sensing
with long-period ﬁber gratings’, Optics Lett., 2000, 25(14), 1007—9.
107 Gander M J, MacPherson W N, McBride R et al., ‘Bend measurement using Bragg
gratings in multicore ﬁbre’, Electron. Lett., 2000, 36(2), 120—1.
Smart textile composites integrated
with ﬁbre optic sensors
The rapid development in textile structural composites (TSCs) has created new
marketing and research opportunities for the textile industry and textile
scientists. According to their structural integrity, three-dimensional textile
composites have a network of yarn bundles in an integrated manner, thereby
giving rise to signiﬁcant increases in inter- and intralaminar strength, higher
feasibility of complex structural shape formation, and greater possibility of
large-scale manufacturing at reduced cost as compared with traditional
laminated composites. Their higher strength and stiﬀness with lighter weight
have led to increasing applications in aerospace, automobile industries and
civil engineering. It has been predicted that the improvement of TSC
fabrication technologies and their combination with smart structure technologies
will lead to major industrial growth in the next century by challenging the
position of metals and other conventional engineering materials.
A success in developing TSC fabrication technology relies on a better
understanding of the processing structure—properties relationship. An important
step in this direction involves the monitoring of the internal strain/stress
distributions in realtime during the fabrication of textile preforms and the
subsequent solidiﬁcation to their ﬁnal structures. Another important issue in
the application of TSCs is to make them sensitive to their internal health
conditions and external environments. Integration of sensing networks inside
fabric-reinforced structures is considered to be the ﬁrst step to make the
materials smart. Furthermore, the complexity of the TSC structure, for
instance, the skin—core eﬀect of three-dimensional braid composites, makes
characterization of the material a very diﬃcult task. In the past, it has been
almost impossible to measure the internal stress/strain distribution of such a
complex material by using conventional methods such as strain gauges and
ultrasonic sensors. In addition, there is a need for some kind of sensing
network embedded in the structures to oﬀer a means to (1) monitor the
Smart textile composites integrated with ﬁbre optic sensors 175
internal stress distribution of TSCs in situ during the manufacturing process,
(2) allow health monitoring and damage assessment of TSCs during services,
and (3) enable a control system to actively monitor and react to the changes in
the working environment.
Fibre optic technologies oﬀering both sensing and signal transmission
functions have attracted considerable attention in recent years, especially in
smart concrete structures including highways, bridges, dams and buildings.
A number of researchers have applied ﬁbre optic sensor (FOS) technologies to
manufacture process monitoring and structure health assessment for
ﬁbre-reinforced composites.— Since optical ﬁbres are of small size and
lightweight, compatible with textile yarns, and readily embedded or even
woven inside TSCs, they are the most promising medium to form the sensing
network mentioned above.
This chapter provides a review of various types of ﬁbre optic sensors, major
issues of smart textile composites integrated with ﬁbre Bragg grating sensors,
that is temperature and strain coupling, sensitivity, multiaxial strain
measurement, measurement eﬀectiveness and reliability issues, as well as
various measurement systems for smart textile composites integrated with
ﬁbre optic sensors.
10.2 Optical ﬁbres and ﬁbre optic sensors
Normally, an optical ﬁbre consists of a core surrounded by a cladding whose
refractive index is slightly smaller than that of the core. The optic ﬁbre is
coated during the ﬁbre drawing process with a protective layer of polymer.
Inside the ﬁbre core, light rays incident on the core-cladding boundary at
angles greater than the critical angle undergo total internal reﬂection and are
guided through the core without refraction. Silica glass is the most common
material for optical ﬁbres, where the cladding is normally made from pure
fused silica, and the core from doped silica containing a few mol % of
germanium. Other dopants, such as phosphorus, can also be used. Extra-low
absorption occurs in a germanosilicate ﬁbre with a local minimum attenuation
coeﬃcient : 0.3 dB/km at 1.3 m and an absolute minimum : 0.16 dB/km
at 1.55 m. Therefore, light in the two windows travels down tens of kilometres
of ﬁbre without strong attenuation in a correct guided mode condition. This is
why optical ﬁbre has been replacing copper coaxial cable as the preferred
transmission medium for electromagnetic waves, revolutionizing the world’s
Parallel with the rapid development in the area of optical ﬁbre communica-
tions, ﬁbre optical sensors have also attracted much attention and experienced
a fast growth in the recent years. They are lightweight, small and ﬂexible; thus
they will not aﬀect the structure integrity of the composite materials and can
176 Smart ﬁbres, fabrics and clothing
be integrated with the reinforcing fabrics to form the backbones in structures.
They are based on a single common technology that enables devices to be
developed for sensing numerous physical perturbations of a mechanical,
acoustic, electric, magnetic and thermal nature. A number of sensors can be
multiplexed along a single optical ﬁbre using wavelength-, frequency-, time-
and polarization-division techniques to form one-, two- or three-dimensional
distributed sensing systems. They do not provide a conducting path through
the structure and do not generate additional heat that could potentially
damage the structure. They do not require electrical isolation from the
structural material and do not generate electromagnetic interference; this
could be a crucial advantage in some applications.
For the applications in smart structures, FOSs can be divided according to
whether sensing is distributed, localized (point) or multiplexed (multipoint). If
sensing is distributed along the length of the ﬁbre, the measurand distribution
as a function of position can be determined from the output signal, so a single
ﬁbre can eﬀectively monitor the changes in the entire object into which it is
embedded. A localized sensor detects measurand variation only in the vicinity
of the sensor. Some localized sensors can lead themselves to multiplexing, in
which multiple localised sensors are placed at intervals along the ﬁbre length.
Each sensor can be isolated by wavelength, time or frequency discrimination,
thereby allowing the real-time proﬁling of parameters throughout the structure.
Before the invention of ﬁbre Bragg gratings (FBGs), FOSs could be
classiﬁed into two broad categories, intensiometric and interferometric,
according to the sensing scheme. Intensiometric sensors are simply based on
the amount of light detected through the ﬁbre. In its simplest form, a stoppage
of transmission due to breakage of a ﬁbre embedded in the structure indicates
possible damage. Interferometric sensors have been developed for a range of
high-sensitivity applications, such as acoustic and magnetic ﬁeld sensors, and
are usually based on single-mode ﬁbres. For example, the Mach—Zehnder
interferometer, as shown in Fig. 10.1, is one of the most common conﬁgurations.
With this type of device, strain can be monitored directly by embedding the
sensing ﬁbre arm in the structure, while the referencing arm of equal length is
isolated from the environment. Although such a conﬁguration is highly
sensitive to strain, the whole ﬁbre length in the signal arm responds to strain,
and thus localization of the sensing region is diﬃcult. An alternative
interferometric sensor, more suitable for localized sensing, is based on
interference between light reﬂected from two closely spaced surfaces, which
form a short gauge length Fabry—Perot (FP)-type interferometer (Fig. 10.2).
The strain or stress applied on the gauge inside the structure can be
determined by measuring the reﬂected spectrum or reﬂected light signal from
the FP cavity, which is a function of the distance between the two reﬂected
surfaces. The disadvantage of such devices is that it is diﬃcult to perform
Smart textile composites integrated with ﬁbre optic sensors 177
50%/50% Structure measured 50%/50%
(Power splitter) (Power splitter)
I = I0 [(I + cos (2 nL/ )]/2
L: optical path difference
between the two arms
10.1 Measurement by interferometric sensors with Mach–Zehnder
Fibre alignment Fibre
input light, T(L)
Reflected light, R(L) L
10.2 Measurement by interferometric sensors with Fabry–Perot-type
absolute measurements, and hard to form a multiplexing sensor array along a
single ﬁbre length due to the large loss of the discontinuing structure of an FP
cavity. Detailed review and analysis have been given by Udd and Measures.
10.3 Principal analysis of embedded ﬁbre Bragg
10.3.1 Principle of FBGS
As FBGs have many advantages over the other two groups, and show great
promise, we will concentrate on FBGs in this section. The FBG is fabricated by
modulation of the refractive index of the core in a single mode optic ﬁbre,
which has been described in detail in Chapters 8 and 9. Assume that the change
in the index modulation period is independent of the state of polarization of
the interrogating light and only dependent on the ﬁbre axial strain,
diﬀerentiating the Bragg wavelength in Eq. (9.15) yields:
: ; [10.1]
where is the total axial strain of the optic ﬁbre. Generally speaking, and n
will have diﬀerent values in the directions of polarization. Subscript i : 1, 2, 3
is denoted for and n as their values in the deﬁned polarized direction. A local
178 Smart ﬁbres, fabrics and clothing
Cartesian coordinate system is used, with 1, 2, 3 representing the three
principal directions respectively. Eq. (10.1) can be rewritten as:
G: ; G [10.2]
For strain, subscript (j : 1, 2, 3, 4, 5, 6) is used. The ﬁrst three represent the
normal strains in the ﬁrst (ﬁbre axis), second, third directions, respectively, the
latter three being the three shear strains, respectively. The strain of an optic
ﬁbre may be contributed by either thermal expansion or stress, hence the
symbol * is used for the optic ﬁbre strain induced by stress only. The
refraction index n is related to both temperature T and strain *, therefore:
n 1 *n *n
G: G *; G T [10.3]
n n ** H *T
G G H H
According to the strain optic theory:
1 *n n
G *:9 G P * [10.4]
n ** H 2 GH H
G H H H
where P is the strain-optic coeﬃcient matrix. For a homogeneous isotropic
P P P
where P : (P 9 P )/2.
For a homogeneous isotropic medium, it can be assumed that the index of
refraction n has a linear relation with temperature T:
: G [10.6]
where is regarded as a thermo-optic constant.
Because lights are transverse waves, only the transverse (2, 3 directions)
deviations of the reﬂective index can cause the shift of the Bragg wavelength.
Substituting Eqs. (10.4), (10.5) and (10.6) into Eq. (10.3), the peak wavelength
shifts for the light linearly polarized in the second and third directions are
Smart textile composites integrated with ﬁbre optic sensors 179
: 9 [P * ; P ( * ; *)] ; T [10.7]
: 9 [P * ; P ( * ; *)] ; T [10.8]
In many cases, the wavelength shift for the Bragg grating sensor observed for
each polarization eigen-mode of the optical ﬁbre depends on all the three
principal strain components within the optical ﬁbre. Sirkis and Haslach
extended Butter and Hocker’s model and have shown that their results are
closer to those observed in transverse loading experiments for the
interferometric optical ﬁbre sensor.
The general cases will be discussed in Section 10.4.2. Here we will only
discuss the axisymmetric problem where * : *. If the optic ﬁbre is a thermal
isotropic material with a constant expansion coeﬃcient , then * : 9 T
(j : 1, 2, 3). Eqs. (10.7), (10.8) can be written into the same form:
: 19 P ; (P ; P )
; (P ; 2P ) T ; T
:f ; * T [10.9]
f:19 P ; (P ; P ) [10.10]
*: ; (P ; 2P ) [10.11]
f is deﬁned as the sensitivity factor, * as the revised optic-thermal constant.
10.3.2 Sensitivity factor
10.3.2.1 Axial strain measurement alone
When the temperature change is so small that its eﬀect can be ignored, the
FBG can be considered as a strain sensor. Let us deﬁne * : ( 9 / ) as the
eﬀective Poisson’s ratio (EPR) of optic ﬁbre. From Eq. (10.11), it is obvious
that the sensitivity factor f is not a constant but a function of *,
180 Smart ﬁbres, fabrics and clothing
Table 10.1 Material parameters of single mode silica optic ﬁbres
Index of refraction Elastic modulus Poisson’s ratio
P11 P12 (n) E (GPa)
0.113 0.252 1.458 70 0.17
1.5 1 0.5 0 0.5 1 1.5
10.3 Sensitivity factor plotted against effective Poisson’s ratio.
f:19 [P 9 (P ; P ) *] [10.12]
Figure 10.3 shows a typical curve of the sensitivity factor as a function of the
eﬀective Poisson’s ratio, calculated by using the material parameters of optic
ﬁbre, provided in Table 10.1.
Let us consider the following special cases:
1 * : 0.17, f : 0.798: which implies that the EPR is equal to the ﬁbre
material Poisson’s ratio and meets the requirement of Butter and Hocker’s
assumption. The value of sensitivity factor, f : 0.798, is recommended by
many FBGS manufacturers;
2 * : 9 1, f : 0.344: which implies that the strains in three principal
directions of the ﬁbre are equal, which corresponds to the case of static
uniform stress or the case of thermal expansion;
3 * : 0.0, f : 0.732; which implies that there is no transverse deformation.
Therefore, if an FBGS is used as an embedded sensor, it is necessary to
make a correction of the sensitivity factor with respect to the transverse
principal strain. Otherwise, only when the transverse principal strain of the
optic ﬁbre is not sensitive to the host’s strain ﬁeld can the sensitivity factor be
regarded as a constant.
Smart textile composites integrated with ﬁbre optic sensors 181
10.3.2.2 Temperature measurement alone
If a stand-alone FBGS is subjected to a temperature change, then:
: : T
where is the isothermal expansion coeﬃcient of the optic ﬁbre. Substituting
the above equation into Eq. (10.9), we can derive the following:
: 19 (2P ; P ) ; * T:( ; ) T
Usually is over ten times greater than (for silica, : 0.55 ; 10,
: 8.3 ; 10), therefore the eﬀect of thermal expansion on the measurement
result may be negligible for such a stand-alone FBGS.
10.3.3 Temperature and strain coupling
As an embedded strain sensor, ideally, the measured strain in Eq. (10.9)
should represent the host strain in the optic ﬁbre direction. The temperature
compensation can be made simply by:
: ( / 9 * T)/f [10.13]
For the germanium-doped silica core, the thermal-optic coeﬃcient is
approximately equal to 8.3 ; 10, then the revised constant * is 8.96 ; 10.
If the measured strain is greater than 0.001 and the variation of the
temperature is smaller than 10 °C, comparatively the term * T in Eq. (10.13)
is one order of magnitude smaller than that of the strain, and the temperature
compensation would be unnecessary in some cases.
10.4 Simultaneous measurements of strain and
10.4.1 Simultaneous measurement of axial strain and
If the internal temperature of the host is unknown and its contribution to the
shift of the wavelength is compatible to that of the strain, it is impossible to
determine strain and temperature from Eq. (10.9) only. One of the most
signiﬁcant limitations of FBG sensors is their dual sensitivity to temperature
and strain. This leads to diﬃculty in the independent measurements for these
two measurands. The main approach is to locate two sensor elements which
have diﬀerent responses to strain and temperature. The sensor schemes are
based on the combination of FBGs with diﬀerent grating types, such as FBGs
with diﬀerent diameter, diﬀerent Bragg wavelength, diﬀerent codope, hybrid
182 Smart ﬁbres, fabrics and clothing
10.4 Structures of FBG cavity sensors: (a) FBG Fabry–Perot cavity, (b) FBG
slightly tapered cavity.
FBGs and long period ﬁbre grating, Fabry—Perot cavity, stimulated Brillouin
scattering or ﬁbre polarization rocking ﬁlter. The observables may be Bragg
wavelength, intensity, Brillouin frequency or polarization rocking resonant
wavelength.— This subsection introduces simultaneous axial strain and
temperature measurements by using an FBG Fabry—Perot cavity or
The structure of a FBG Fabry—Perot cavity sensor is shown in Fig. 10.4(a),
which consists of two identical FBGs separated by a short cavity with a length
of L . If the reﬂectivity of the two FBGs, R ( ), is small, the reﬂection spectrum
of the FBG Fabry—Perot cavity sensor, R ( ), is approximately given by:
R ( ) : a R ( )F( )
EA A E [10.14]
F( ) : 1 ; cos[
( )] : 1 ; cos(4 n L / )
where a is a constant, F( ) is an interference of the cavity,
( ) is the phase
diﬀerence between the light reﬂected by the two FBGs, and n is the eﬀective
refractive index of the section. The reﬂection spectrum of the FBG Fabry—Perot
cavity sensor is modulated by the cavity phase change. As a result, strain and
temperature are encoded into the Bragg wavelength shift and the variation in
the cavity’s phase diﬀerence or optical path. The change in the phase diﬀerence
can be decoded by measuring the change in the total reﬂected power or the
reﬂection spectrum proﬁle of light from the sensor.
When a minimum of F( ) occurs within the grating’s main reﬂection band,
the FBG Fabry—Perot cavity reﬂection spectrum is split into two peaks, one
Smart textile composites integrated with ﬁbre optic sensors 183
on each side of the Bragg wavelength . If this minimum coincides with
the intensities of the two peaks become equal. With applied strain or
temperature, both the spectrum and the interference function as a result of
change in the phase diﬀerence variation. The respective shifts of and
can be expressed by:
/ K K T
: 2 K [10.15]
/ K K
where K and K are the temperature and strain coeﬃcients of the FBG
(i : 1) and the cavity (i : 2) sections, respectively. If the two sections have
equal coeﬃcients such as K : K and K : K , the relative position
K K 2 2
between and will not change with applied strain or temperature. In this
case the reﬂection spectrum of the FBG Fabry—Perot cavity sensor shifts, but
its proﬁle remains unchanged. Thus temperature and strain cannot be
determined separately. However, if the FBG and cavity sections have diﬀerent
strain and temperature coeﬃcients, that is K 9 K or K 9 K , will
K K 2 2
move at a faster rate than . This results in a reduction in the intensity of
peak 1 and an increase in the intensity of peak 2 when strain or temperature
increases. When increases to coincide at the next maximum of F( ) at ,
peak 2 reaches a maximum value and peak 1 vanishes. Further increase in
strain or temperature will result in two peaks in the FBG Fabry—Perot cavity
reﬂection spectrum, but in this case the intensity of peak 2 (corresponding to
the longer wavelength) will decrease, whereas the intensity of peak 1
(corresponding to the shorter wavelength) increases. Therefore, the intensity of
the two peaks changes periodically with strain and temperature.
The intensity ﬂuctuation of the light source can be eliminated by introducing
a normalized parameter M : (I 9 I )/(I ; I ), where I and I are
. . . . . .
the respective intensities of peaks 1 and 2. If the relationship between , M,
and T is assumed to be linear, then the two measurands can be determined
simultaneously by measuring the changes in M and the wavelength shift of
either peak 1 or peak 2 with respect to strain and temperature:
A A T
. : 2 K [10.16]
M A A
In order that the strain and temperature coeﬃcients of the cavity section are
diﬀerent from those of the grating sections, a short (1 mm long) and thin
aluminium tube (with an inside diameter of 0.3 mm and wall thickness of
0.15 mm) was glued onto the cavity section. This section is more diﬃcult to
stretch than the grating sections, and thus its strain coeﬃcient is correspondingly
smaller, so that K : K . On the other hand, its temperature coeﬃcient
becomes larger (K 9 K ). This is because the thermal expansion coeﬃcient
184 Smart ﬁbres, fabrics and clothing
of aluminium (23.5 ; 10/°C) is much larger than that of the silica glass ﬁbre
(0.55 ; 10/°C), and expansion of the aluminium tube due to temperature
rise induces additional strain to the cavity section.
Figure 10.4(b) shows another FBG Fabry—Perot cavity structure, that is an
FBG tapered cavity sensor, in which the cavity section is tapered slightly. The
maximum change of diameter at the cavity section is smaller than 15%, hence
no obvious changes in transmission and mode-eﬀective refractive index are
induced. The tapered cavity section possesses the same strain and temperature
coeﬃcients as those of the grating section. However, the average strain
suﬀered by the tapered cavity ( ) becomes larger than that at the grating
section ( ), which is given by : , where is an average ratio of
cross-sectional areas between the grating and cavity sections. The relative
movement between F( ) and R ( ) remains zero when the temperature
changes, therefore the spectral proﬁle is only sensitive to the strain applied
along the sensor:
where and are the temperature and strain coeﬃcients of the grating
Superstructured FBG sensors were developed for this purpose, which
have advantages of easier manufacturing and no need to alter the mechanical
properties and geometry of ﬁbre sensor. FBG sensors generally consist of a
single FBG or a combination of FBGs written in low-birefringent optical ﬁbre.
In the former case, the Bragg wavelength shift can be used to measure the axial
component of strain or a change in temperature. In the latter case, axial strain
and temperature can be simultaneously determined according to the Bragg
wavelength shifts, or the Bragg wavelength shifts and the intensities.
10.4.2 Simultaneous measurement of multi-axial strain and
10.4.2.1 Polarization-maintaining (PM) FBG
The transverse strain-induced wavelength sensitivity of FBGs in silica optical
ﬁbres is low. For instance, in lateral compression, the changes in ﬁbre
birefringence are smaller than 10. This level of birefringence corresponds to
wavelength separations much smaller than the typical bandwidth of an FBG.
However, we have shown in Section 10.3.1 that the sensitivity factor is a
function of the two principal transverse strains and axial strain, which are
normally unknown. The needs are apparent for multi-axial measurements of
strain and temperature.
Smart textile composites integrated with ﬁbre optic sensors 185
FBGs were written in a polarization-maintaining ﬁbre for the measurement
of lateral strains.— A polarization-maintaining ﬁbre may consist of a
circular core and inner cladding surrounded by an elliptical stress-applying
region. Birefringence is induced by thermal stresses generated during the
cool-down from the drawing temperature due to the geometric asymmetry of
the stress-applying region. This stress-induced birefringence leads to diﬀerent
propagation constants for the two orthogonal polarization modes in the ﬁbre.
The x and y axes are parallel to the fast and slow axes of the principal
polarization axes of the ﬁbre, respectively, which correspond to the minor and
major axes of the elliptical stress-applying region. Polarization-maintaining
ﬁbre has an initial birefringence that is suﬃcient to split the grating completely
into two separate spectra. Because of the diﬀerence in eﬀective refractive
indices of the two orthogonal polarization modes, two eﬀective FBGs result in
one along the polarization axes by writing one FBG. For the case of
low-birefringent FBG, if the temperature sensitivity of the FBG remains
constant, the relative Bragg wavelength shifts can be written as:
/ : 9 0.5 ; n [p ; p ( ; )]
?V ?V V [10.18]
/ : 9 0.5 ; n [p ; p ( ; )]
?W ?W W
where and are the Bragg wavelength for the two orthogonal polarization
modes, respectively, and are the initial unstrained Bragg wavelength
for the two orthogonal polarization modes, respectively, and n and n are
the eﬀective refractive indices of the two orthogonal polarization modes,
respectively. Supposing that the axial strain is known, the relative Bragg
wavelength shifts can be written in matrix:
/ K K
?V ?V : [10.19]
/ K K
where the coeﬃcient matrix contains p , p , , n and n . For the case of
high-birefringent FBG, such as polarization-maintaining FBG (PM-FBG),
the sensor must be calibrated to the ﬁnite-element predictions by performing a
least-squares ﬁt to determine the coeﬃcient matrix from the measured
wavelength data. According to Eq. (10.19), the lateral components of the
strain can be determined. In many structures, one would like an FBG sensor
that could measure both lateral axes of strain, axial strain and temperature.
An approach to solving this problem is to use dual overlaid FBGs at diﬀerent
Bragg wavelengths written onto a PM ﬁbre. If two FBGs of diﬀerent Bragg
wavelengths, such as 1300 nm and 1550 nm, were written at a single location
in a PM ﬁbre, four eﬀective FBGs result in one along the corresponding
polarization axis and at corresponding Bragg wavelength. The relative Bragg
wavelength shifts can be written as:
186 Smart ﬁbres, fabrics and clothing
K K K K
/ K K K K
?W ?W :
/ K K K K
/ K K K K T
where and are the Bragg wavelength for the two orthogonal polarization
modes of the second FBG, respectively, and and are the initial
unstrained Bragg wavelength for the two orthogonal polarization modes of
the second FBG, respectively. Assuming linearity in sensor response and that
the element of the 4 ; 4 coeﬃcient matrix is independent of strain and
temperature, and the matrix is not singular, the elements of the matrix can be
determined by performing separate experimental and least-squares ﬁtting
calibrations of the response of the sensor to lateral strain, to axial strain and to
10.4.2.2 -Phase-shifted FBG
Another approach is to use -phase-shifted FBGs. If a regular FBG is
irradiated with UV light at a certain region in the middle of the FBG, the
refractive index in the region is raised. Such processing produces two FBGs
out of phase with each other, which act as a wavelength-selective Fabry—Perot
resonator, allowing light at the resonance to penetrate the stop-band of the
original FBG. The resonance wavelength depends on the size of the phase
change. When the shifted phase is equal to at a wavelength in the
stop-band of the original FBG, the strong reﬂections from the two FBG
sections are out of phase, resulting in strong transmission at this wavelength.
This post-processing FBG is called -phase-shifted FBG ( -FBG). The
transmission window of -FBG can be made very narrow and is split in two
when the FBG is birefringent. This sharpness permits very high accuracy
measurement of the FBG birefringence. Furthermore, the birefringence required
for separating the peak is much smaller than for regular FBGs and can be
provided by the intrinsic birefringence of an FBG written in non-PM ﬁbre.
The ﬁbre has birefringence in the absence of an external load, of which
several factors, such as geometric, UV-induced and stress-induced, may be at
the origin. However, for mathematical convenience, it is assumed that the
initial birefringence in the FBG is due to a residual strain state in the ﬁbre core
that is described by the principal strains and ( 9 ). These principal
strains are in directions perpendicular to each other and to the ﬁbre axis, and
direction 1 makes an angle
with the x axis. According to Eq. (10.18), the
wavelength separation can be expressed as:
: 9 : 0.5 [(n ; n )/2]
(p 9 p )( 9 ) [10.21]
Smart textile composites integrated with ﬁbre optic sensors 187
The new wavelength separation can be obtained by a function of
) : a ; b cos(2
where a and b are positive values which are independent of
. Thus, the larger
is, the lower the sensitivity to lateral strain.
10.5 Measurement effectiveness
For the FBGS to be an ideal embedded strain sensor in a textile composite, the
following conditions will have to be met: (1) the integrated optic ﬁbre has
little eﬀect on the host strain ﬁeld; (2) the axial strain of optic ﬁbre can
represent the nearby host strain in the optic ﬁbre direction; and (3) the eﬀective
Poisson’s ratio * is constant during the measurement period. The embedded-
optic-ﬁbre—host system can be illustrated as a composite comprising a
cylindrical ﬁbre and two concentric shell layers, with ﬁbre, coating and host
from the centre to the outer surface (Fig. 10.5). The height of the composite
cylinder is 2H, the radius of the ﬁbre is R , which is also the interior radius of
coating, R is the outer radius of the coating and the inner radius of the host,
and R is the outer radius of the host. The following basic assumptions have
been made so that the case can be simpliﬁed as an axial-symmetric problem: (1)
The optical ﬁbre, ﬁbre coating and host are linear elastic. (2) The thermal
expansion coeﬃcients of ﬁbre, coating and host are constants. (3) There is no
discontinuity in displacement at the interfaces of ﬁbre and coating, coating
and host under loading. (4) Thermal load is uniform in the whole composite
cylinder. (5) The two ends (z : H) are assumed to be free from any external
force and there is no constraint on displacement.
10.5.1 General views of the normalized strain distribution
Figure 10.6(a), (b) and (c) illustrate the normalized strain distribution in the
ﬁbre, host and coating, respectively, along the ﬁbre axial direction with
various values of radius r. Figure 10.6(a) shows that the normalized strain of
10.5 Three-layer composite model of host, coating, and ﬁbre.
188 Smart ﬁbres, fabrics and clothing
0 2 4 6 8 10
(a) z (mm)
0 2 4 6 8 10
(b) z (mm)
0 2 4 6 8 10
(c) z (mm)
10.6 Strain distribution in the embedded optic ﬁbre–host sytem:
(a) distribution of ﬁbre’s axial strain at various radial positions, ——
0.007875; —— 0.023625; —s— 0.039375; —;— 0.055125;
(b) distribution of host’s axial strain at various radial positions, ——
0.248; —— 0.498; —s— 0.748; —×— 0.998; (c) distribution of coating’s
axial strain at various radial positions, —— 0.0705; —— 0.0855; —s—
0.1005; —;— 0.1155.
Smart textile composites integrated with ﬁbre optic sensors 189
ﬁbre declines with increasing length z. Because the thermal expansion
coeﬃcient of the optic ﬁbre is more than one order of magnitude smaller than
that of the host, the strain level of the optic ﬁbre depends largely on the
restriction of the host. As the middle part of the optic ﬁbre is restricted more
than the parts near the two ends, the strain of the middle optic ﬁbre is closer to
that of the host without the embedded ﬁbre sensor (e : 1). The strain
distribution curves are identical, regardless of the radial position in the ﬁbre,
thus the strain of the ﬁbre can be regarded as a function of z only.
Figure 10.6(b) shows the reverse trends of strain distribution in the host. The
strain level of the middle host is lower than that of the host near the boundary,
which is because the middle host is restricted more by the ﬁbre and the host
near the boundary can expand more freely under a thermal load. The
normalized strain values of the host are very close to 1 (0.995 : e : 1), which
implies that the host with the embedded ﬁbre sensor has a strain ﬁeld very
close to that without the embedded optic ﬁbre.
Because of its lower elastic modulus, the strain distribution of the coating is
signiﬁcantly aﬀected by both the ﬁbre and the host, as shown in Fig.10.6(c).
The strain distribution along z is similar with that of the ﬁbre when r
approaches R , and the strain near the outer surface of the coating varies little
along z, like that of the host.
10.5.2 Effects of parameters on effectiveness coefﬁcient
The term H has been introduced, at which e has a value of 0.95. The
physical meaning of H is that only when the z of the optic ﬁbre grating is
smaller than H is the measurement result of the ﬁbre eﬀective. The length of
the zone represents the limits of eﬀective measurement of host strain by an
embedded FBGS. The longer the zone length, the more eﬀective an FBGS in a
host. Thus the relative length of the eﬀective zone is deﬁned as the eﬀectiveness
The eﬀectiveness coeﬃcient is inﬂuenced by a number of factors, the elastic
modulus, Poisson’s ratio of coating, tension stiﬀness ratio, the thickness of
composite etc. Figure 10.7 shows that increasing E leads to a sharp
increment in when E varies from 0.045 to 1 GPa. The curve then reaches a
plateau and the eﬀect on becomes very small. Thus E : 1 GPa can be
regarded as a threshold value for the speciﬁed conditions.
Figure 10.8 plots the eﬀective Poisson’s ratio of the optic ﬁbre against the
ﬁbre length. Within a range from zero to 7 mm, the eﬀective Poisson’s ratio
190 Smart ﬁbres, fabrics and clothing
1.5 1 0.5 0 0.5 1 1.5 2
Log (E c )
10.7 Effect of elastic modulus of coating on the effectiveness coefﬁcient
of optic ﬁbre.
2 4 6 8 10
10.8 Distribution of ﬁbre’s effective Poisson’s ratio along the ﬁbre length
at various radial positions.
declines slightly with the increment of z. Thus it can be regarded as a constant
along the z axis except for the short portion near the boundary. The value of *
near z : 0 is 0.13 which is not equal to the Poisson’s ratio of the ﬁbre (0.17).
This indicates that the transverse strain of the optic ﬁbre is not dominated by
the host strain (otherwise it should be close to 9 1) but by the Poisson’s ratio
of the ﬁbre.
In the particular case under our investigation, the elastic modulus of the
coating should be equal to or greater than the threshold value f : 0.78 GPa, if
the measurement eﬀectiveness is concerned (see Fig. 10.7). However, the
increment of E will aﬀect the value of the eﬀective Poisson’s ratio, *, then the
sensitivity factor, f. Figure 10.9 plots * as a function of E , which exhibits the
reversed trend compared with that of the eﬀectiveness . When the coating
modulus is smaller than, or equal to, the threshold value of 1 GPa, the
variation of * is rather small. By considering the eﬀects of the coating elastic
modulus on both measurement eﬀectiveness and the eﬀective Poisson’s ratio,
Smart textile composites integrated with ﬁbre optic sensors 191
1.5 1 0.5 0.5 1 1.5 2
Log (E c )
10.9 Effect of elastic modulus of coating on ﬁbre’s effective Poisson’s
the optimal coating modulus should be chosen as the threshold value
E : 1 GPa. This case illustrates the necessity of selecting optimal material
properties of coating in order to make eﬀective measurements.
10.6 Reliability of FBGs
A single-mode silica optic ﬁbre has a typical cladding diameter of 125 microns
and an outer diameter of 250 microns. It can be introduced into a textile
preform in its manufacturing processes such as weaving, knitting and braiding.
Alternatively, it can be introduced at the consolidation process of the textile
composites. In both cases, caution should be exercised when integrating it into
the textile structure. Apart from avoiding the damage to the optic ﬁbre during
manufacturing processes, the reliability of an embedded ﬁbre Bragg grating
sensor is inﬂuenced by a number of other factors as follows:
1 Grating-making method: an optic ﬁbre is normally decoated around the
grating location before UV pulse laser exposure and recoated afterward.
During the decoating and UV irradiation processes, the optic ﬁbre may get
damaged, as shown in Chapter 8. Further, the new coat may cause some
variation in the ﬁbre. The sensitivity to strain may be diﬀerent for FBG
sensors, even with the same central reﬂecting wavelength.
2 Location and direction of sensors in composite hosts: usually the FBG
sensor is used to measure certain positional and directional normal strain
in the host. However, in the procedure of embedding the FBG sensor into
the composite host, some deviation of the optic ﬁbre sensor may occur
from the designed position and direction. To reduce the measurement
error, determination of the real location of the grating of FBG sensors
inside the composite may be a key issue, especially when the sensors are
192 Smart ﬁbres, fabrics and clothing
embedded in a large gradient strain ﬁeld such as near the tip of a crack.
Furthermore, it is very diﬃcult to precisely detect the real position and
direction of the ﬁbre grating sensor after it is embedded into a composite.
The levels of errors induced by the deviation of position and direction of
the sensors will be given in Section 10.7.
3 The interfaces of ﬁbre/coating and coating/resin: stress concentration
exists around the interfaces and may cause cracks, which may aﬀect the
measurement results. Researchers have introduced a debonding phenomenon
into the interfaces between ﬁbre and coating as well as between coating and
host when fabricating the ﬁbre Bragg optic strain sensors and integrating
them into a laminated composite beam. The study showed that the
dual-ended sensors are reliable in cyclic bending deformation, while the
single-ended sensors are not when their interface bonding fails. To reduce
the measurement error, determination of the real location of the grating of
FBG sensors inside the composite may be a key issue for future work,
especially when the sensors are embedded in a large gradient strain ﬁeld
such as near the tip of a crack.
4 The environment and working conditions to which a textile composite is
subject, and how long it is subject to them, will greatly inﬂuence the
selection and integration of ﬁbre optic sensors. The analysis of measurement
eﬀectiveness in the previous section is based on the composite model
assuming perfect interfaces between the coating and ﬁbre as well as
between the coating and host. Another condition is that the strain
measured by the optic ﬁbre sensor is at a predetermined position and in a
predetermined direction. Hence, the following section will investigate their
eﬀects when these assumed conditions are not met.
10.7 Error of strain measurement due to deviation of
position and direction
10.7.1 Deviation of direction
Assume the principal strains in a structure are , and . If an FBG sensor is
embedded in the structure and the angles between the sensor and principal
strains are , and , the strain induced along the FBG sensor is:
0 0 cos
: [cos cos cos ] 0 0 cos [10.23]
0 0 cos
: cos ; cos ; cos
where cos ; cos ; cos : 1. The strain measured in the sensor is a
Smart textile composites integrated with ﬁbre optic sensors 193
function of the principal strains and the angles between them and the sensor.
In practice, when a sensor is embedded in the structure, it is most likely to show
deviation between the sensor and desired direction. Suppose the deviations of
the sensor are , and , then the strain in the sensor will be:
: cos( ; ) ; cos( ; ) ; cos( ; )
According to Eq. (10.24), if one wants to measure one of the principal strains,
the simplest method is to place sensors along the direction of the desired strain.
For example, if is desired, the sensor will be placed along this direction. Then
we have : 0 and : : /2. The inﬂuence of other strains ( and )
will be cancelled. If the deviations between the sensor and the desired direction
are , and , the strain along the sensor will be:
: cos ; cos( /2 ; ) ; cos( /2 ; )
: cos ; sin ; sin
The relative error between the measured and real values of strain is:
9 cos ; sin ; sin 9
error : ? :
If , and are small quantities, Eq. (10.26) can be expressed as:
9 ; ;
error : O ; ;
In Eq. (10.27), the third and higher orders of deviations are omitted. The
measurement error is quadratic to the deviations in the orientation angles.
10.7.2 Deviation of position
The strain ﬁeld of a structure is related to the position and the deformation of
the structure. Suppose the strain at point (x, y, z) can be expressed as
: f(x, y, z, ), where is a tensor and represents the displacement vector of
the structure. The variation of strain due to the deviations of the position
( x, y, z) can be expressed as:
*f(x, y, z, ) *f(x, y, z, )
: · x; · y
*f(x, y, z, ) [10.28]
; · z ; E( x, y, z)
194 Smart ﬁbres, fabrics and clothing
where E( x, y, z) is the second and higher-order quantities of the position
deviation ( x, y, z). When the deviations are small and E( x, y, z) can be
omitted, Eq. (10.28) can be simpliﬁed as:
*f(x, y, z, ) *f(x, y, z, ) *f(x, y, z, )
: · x; · y; · z [10.29]
*x *y *z
For a cantilever beam, if a concentrated load acts at its free end, the axial strain
of an arbitrary point (x, y, z) in the beam due to the normal displacement of
the free end is:
(x, y, z) : (L 9 x)z [10.30]
where L is the length of the beam, x is the location of the point along the beam,
y is the location of the point along the y-direction, and z is the distance between
the point and the neutral axis of the beam.
The strain in the beam is independent of the position of y. That means the
deviation of y will not inﬂuence the strain measurement. If there are any
deviations of the test point ( x, y, z), according to Eq. (10.29) the variation
of the strain will be:
3 z 3 (L 9 x)
:9 · x; · z [10.31]
The relative error of strain deduced from the position deviations is:
error : O ; [10.32]
(x, y, z) L9x z
If the sensors are placed near the ﬁxed end (x : x : 0) and far from the
neutral axis (z : z : h/2, h is the height of the cantilever beam) of the beam,
the measurement error will be the minimum.
10.7.3 Deviation of both direction and position
If deviations of direction and position occur simultaneously, then the total
relative error is:
error : error ; error O
; ; [10.33]
From Eq. (10.33) we know that, in order to obtain an accurate measurement
result, the deviations of direction and position should be as small as possible.
This derivation is more suitable for the surface-mounted FBGs. If
Smart textile composites integrated with ﬁbre optic sensors 195
embedded in a composite, the localized heterogeneity will normally lead to a
complicated strain ﬁeld. If the strain is not uniformly distributed along FBG,
grating apodization occurs. The strain may induce birefringence which may
cause peak split. Hence, the analysis of measurement error must consider at
least the above-mentioned factors.
10.8 Distributed measurement systems
By the means of measuring the shift of the peak wavelength of the reﬂective
spectrum, the average strain over the whole grating length is determined,
rather than the distribution of the strain. In many applications, the distribution
of strain and temperature is the major concern, thus a number of methods can
be implemented to serve this purpose. The grating length of FBGs can be made
very short (e.g. 2 mm), thus the strain measured by the shift wavelength of the
reﬂective spectrum can be regarded as a localized strain. The FGB arrays
render themselves as ideal candidates for multi-point or quasi-distributive
measurements by the multiplexing techniques used for several other optical
ﬁbre sensors, such as wavelength-division-multiplexing (WDM), time-division-
multiplexing (TDM) and spatial-division-multiplexing (SDM). Detailed reviews
have been given by Rao, Kersey et al. and Othonos and Kalli. Figure
10.10 shows a schematic diagram of the measurement systems, consisting of a
broad-band LED, a coupler or optic switch, an optical analyser, and an
embedded multiplexing FBG array by which we carried out our pseudo-
distributed measurement of strain-temperature in textile composites.
In simple cases, if it is monotonic, the strain distribution can be determined
along the grating by analysing the reﬂection spectrum. Volanthen and his
colleagues developed a measurement system of distributed grating sensors to
measure the wavelength and reﬂectivity of gratings as functions of time
delay.— By using low-coherence reﬂectometry, this technique was applied
to three-point bending experiments of a textile composite beam embedded
In conclusion, ﬁbre optic sensors are ideal candidates to be embedded in textile
structural composites for monitoring manufacturing processes and internal
health conditions. The sensors provide an eﬀective means by which the
distributions of a number of physical parameters, such as temperature,
stress/strain, thermal expansion, pressure, etc., can be quantitatively determined.
In integrating the sensors into textile composites, apart from the properties of
the sensors themselves, the reliability of the sensors and sensing scheme as well
10.10 Wavelength-division-multiplexing systems by FBG arrays embedded in composites.
Smart textile composites integrated with ﬁbre optic sensors 197
as the interaction between sensors and composites are very important issues to
The author wishes to acknowledge the Research Grants Council of the Hong
Kong SAR government for funding support (Project No. PolyU123/96E and
PolyU5512/98E). The author also thanks her colleagues, Dr Du W.C., Dr
Tang L.Q. and Dr Tian X.G. for their contributions in the development of
theoretical analysis and experiments.
1 Du C W, Tao X M, Tam Y L and Choy C L, ‘Fundamentals and applications of
optical ﬁber Bragg grating sensors to textile composites’, J. Composite Struct., 1998,
2 Matthews L K (ed.), Smart Structures and Materials 1995, Smart Systems for
Bridges, Structures, and Highways, SPIE, 1995, 2446.
3 Merzacher C I, Kersey A D and Friebele E J, ‘Fibre optic sensors in concrete
structures: a review’, Smart Mater. Struct., 1996, 5, 196—208.
4 Hayes S A, Brooks D, Liu T Y, Vicker S and Fernando G F, ‘In-situ self-sensing
ﬁbre reinforced composites’, Smart Structures and Materials 1996, SPIE, 2718, 376—84.
5 Hong C S, Kim C G, Kwon I and Park J W, ‘Simultaneous strain and failure sensing
of composite beam using an embedded ﬁbre optic extrinsic Fabry—Perot sensor’,
Smart Structures and Materials 1996, SPIE, 1996, 2718, 122—33.
6 Badcock R A and Fernando G F, ‘Intensity-based optical ﬁbre sensor for fatigue
damage detection in advanced ﬁbre-reinforced composites’, Smart Mater. Struct.,
1995, 4(4), 223—30.
7 Udd E, Fiber optic sensor overview. In Fiber Optic Smart Structures, ed. E Udd,
John Wiley, 1995.
8 Measures R M, Fiber optic strain sensing. In Fiber Optic Smart Structures, ed. E
Udd, John Wiley, 1995.
9 Butter C D and Hocker G P, ‘Fiber optics strain gauge’, Appl. Opt., 1992, 1370, 189—96.
10 Sirkis J S and Haslach H W Jr, ‘Full phase-strain relation for structurally embedded
interferometric optic ﬁber sensors’, Proc. SPIE, 1990, 1370, 248—59.
11 Jackson D A and Jones J D C, ‘Fibre optic sensors’, Pot. Acta, 1986, 33, 1469—503.
12 Takahashi S and Shibata S, ‘Thermal variation of attenuation for optical ﬁbers’,
J. Non-crystal. Solids, 1979, 30, 359—70.
13 Akhavan Leilabady P, Jones J D C and Jackson D A, Optics Lett., 1985, 10, 576.
14 Friebele E J, Putnam M A, Patrick H J et al., ‘Ultrahigh-sensitivity ﬁber-optic
strain and temperature sensor’, Optics Lett., 1998, 23, 222—4.
15 Chan C C, Jin W, Rad A B et al., ‘Simultaneous measurement of temperature and
strain: an artiﬁcial neural network approach’, IEEE Photon. Technol. Lett., 1998,
198 Smart ﬁbres, fabrics and clothing
16 James S W, Dockney M L and Tatam R P, ‘Simultaneous independent temperature
and strain measurement using in-ﬁber Bragg grating sensors’, Electron. Lett., 1996,
17 Xu M G, Archambault J L, Reekie L et al., ‘Discrimination between strain and
temperature eﬀects using dual-wavelength ﬁber grating sensors’, Electron. Lett.,
1994, 30, 1085—7.
18 Cavaleiro P M, Araujo F M, Ferreira L A et al., ‘Simultaneous measurement of
strain and temperature using Bragg gratings written in germanosilicate and
boron-codoped germanosilicate ﬁbers’, IEEE Photon. Technol. Lett., 1999, 11, 1635—7.
19 Patrick H J, Williams G M, Kersey A D et al., ‘Hybrid ﬁber Bragg grating/long
period ﬁber grating sensor for strain/temperature discrimination’, IEEE Photon.
Technol. Lett., 1996, 8, 1223—5.
20 Du W C, Tao X M and Tam H Y, ‘Fiber Bragg grating cavity sensor for
simultaneous measurement of temperature and strain’, IEEE Photon. Technol.
Lett., 1999, 11, 105—7.
21 Du W C, Tao X M and Tam H W, ‘Temperature independent strain measurement
with a ﬁber grating tapered cavity sensor’, IEEE Photon. Technol. Lett., 1999, 11(5),
22 Guan B O, Tam H Y, Tao X M and Dong X Y, ‘Simultaneous strain and
temperature measurement using a superstructure ﬁber Bragg grating’, IEEE
Photon. Technol. Lett., 2000, 12(6), 1—3.
23 Kawase L R, Valente L C G, Margulis W et al., ‘Force measurement using induced
birefringence on Bragg grating’, in Proc. 1997 SBMO/MTT-S International
Microwave and Optoelectronics Conference, 1, 394—6.
24 Lawrence C M, Nelson D V, Makino A et al., ‘Modeling of the multi-parameter
Bragg grating sensor’, in Proc. SPIE — Third Paciﬁc Northwest Fiber Optic Sensor
Workshop, 3180, 42—9.
25 Udd E, Nelson D and Lawrence C, ‘Multiple axis strain sensing using ﬁber gratings
written onto birefringent single mode optical ﬁber’, in Proc. 12th International
Conference on Optical Fiber Sensors, Williamsburg, USA, 1997, 48—51.
26 Udd E, Lawrence C M and Nelson D V, ‘Development of a three axis strain and
temperature ﬁber optical grating sensor’, in Proc. SPIE — Smart Structures and
Materials 1997: Smart Sensing, Processing, and Instrumentation, 3042, 229—36.
27 Udd E, Schulz W L, Seim J M et al., ‘Transverse ﬁber grating strain sensors based
on dual overlaid ﬁber gratings on polarization preserving ﬁbers’, in Proc. SPIE —
Smart Structures and Materials 1998: Sensory Phenomena and Measurement
Instrumentation for Smart Structures and Materials, 3330, 253—63.
28 LeBlanc M, Vohra S T, Tsai T E et al., ‘Transverse load sensing by use of
pi-phase-shifted ﬁber Bragg gratings’, Optics Lett., 1999, 24, 1091—3.
29 Canning J and Sceats M G, ‘ -phase-shifted periodic distributed structures in
optical ﬁbers by UV post-processing’, Electron. Lett., 1994, 30, 1344—5.
30 Tao X M, Tang L Q, Du W C and Choy C L, ‘Internal strain measurement by ﬁber
Bragg grating sensors in textile composites’, J. Composite Sci. Technol., 2000, 60(5),
31 Tang L Q, Tao X M and Choy C L, ‘Measurement eﬀectiveness and optimisation of
ﬁbre Bragg grating sensor as embedded strain sensor’, Smart Mater. Struct., 1999, 8,
Smart textile composites integrated with ﬁbre optic sensors 199
32 Tao X M, ‘Integration of ﬁbre optic sensors in smart textile composites — design and
fabrication’, J. Text. Inst., 2000, 91, Part 1 No.2.
33 Tang L Q, Tao X M, Du W C and Choy C L, ‘Reliability of ﬁbre Bragg grating
sensors in textile composites’, J. Composite Interfaces, 1998, 5(5), 421—35.
34 Du C W, Tao X M, Tam Y L and Choy C L, ‘Fundamentals and applications of
optical ﬁber Bragg grating sensors to textile composites’, J. Composite Struct., 1998,
35 Rao Y J, ‘In-ﬁbre Bragg grating sensors — Measurement and science technology’,
Measurement Sci. Technol., 1997, 8, 355—75.
36 Keysey A D, Davis M A, Patrick H J et al., ‘Fiber grating sensors’, J. Lightwave
Technol., 1997, 15(8), 1442—63.
37 Othonos A and Kalli K, Fibre Bragg Gratings: Fundamentals and Applications in
Telecommunications and Sensing, Artech House, 1999.
38 Volathen M, Geiger H, Cole M J, Laming R L and Dakin J P, ‘Low-coherence
technique to characterize reﬂectivity and time delay as a function of wavelength
within a long ﬁbre grating’, Electron Lett., 1996, 23(8), 847—9.
39 Volathen M, Geiger H, Cole M J and Dakin J P, ‘Measurement of arbitary strain
proﬁles within ﬁbre gratings’, Electron Lett., 1996, 23(11), 1028—9.
40 Volathen M, Geiger H, Cole M J and Dakin J P, ‘Distributed grating sensors using
low-coherence reﬂectometry’, J. Lightwave Technol., 1997, 15(11), 2076—82.
Hollow ﬁbre membranes for gas separation
PHILIP J. BROWN
11.1 Historical overview of membranes for gas
During the last century and a half, the development of membranes has resulted
in a voluminous amount of literature on the subject.
One review of membranes by Lonsdale still contained over 400 references,
even though the author claimed to have covered only the most relevant
references in the article. This review also does not therefore intend to be a
comprehensive review of the development of membrane technology; rather it
is a short account of the interesting developments that have taken place along
with the milestones